इंटरनेट मानक Disclosure to Promote the Right To Information Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public. “जान1 का अ+धकार, जी1 का अ+धकार” “प0रा1 को छोड न' 5 तरफ” “The Right to Information, The Right to Live” “Step Out From the Old to the New” Mazdoor Kisan Shakti Sangathan Jawaharlal Nehru IS 456 (2000): Plain and Reinforced Concrete - Code of Practice [CED 2: Cement and Concrete] “!ान $ एक न' भारत का +नम-ण” Satyanarayan Gangaram Pitroda “Invent a New India Using Knowledge” “!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता ह” है” ह Bhartṛhari—Nītiśatakam “Knowledge is such a treasure which cannot be stolen” IS. 456 : 2000 ( R••fflrmed 2005 ) Indian Standard PLAIN AND REINFORCED CONCRETE CODE OF PRACTICE ( Fourth Revision) Tenth Reprint APRIL 2007 (IncludingAmendments No. I and 2) ICS 91.100.30 C BI52000 BUREAU OF INDIAN STANDARDS MANAK BHAVAN. 9 BAHADUR SHAH ZAFAR MARG NEW DELIiI 110002 July 2000 Price Rs. 830.09 + Rs. 120.09 IS 456: 2000 CONTENTS PAGE SECTION 1 GENERAL J SCOPE )J 2 REFERBNCES 11 3 TERMINOLOGY 11 4 SVMBOU 11 SECTION 2 MATERIALS, WORKMANSHIP, INSPECTION AND TESTING 5 6 13 MATERIALS 5.1 Cement 13 5.2 Mineral Admixtures 13 5.3 Aggregates 5.4 Water 14 5.5 Admixtures 5.6 Reinforcement IS 15 5.7 15 14 Storage of Materials CONCRETE 15 6.1 Grades 15 6.2 Properties of Concrete 15 7 WORKABIUTY OF CONCRETE 17 8 DURABILITY OF CONCRETE 17 8.1 8.2 18 9 17 General Requirements for Durability CONCRETE MIX PROPORTIONING 22 9.1 9.2 Mix Proportion Design Mix Concrete 22 22 9.3 Nominal Mix Concrete 23 23 10 PRODUlllON OF CONCRETE 11 23 10.2 Quality AssuranceMeasures Batching 24 10.3 Mixing 24 10.1 FORMWORK 25 1J.1 11.2 General Cleaning and Treatment of Fonnwork 25 Stripping Time 25 11.3 25 12 ASSEMBLY OF REINFORCEMENT 25 ·13 TRANSPORTING, PLACING, COMPACTION AND CURING 26 J3.1 26 13.2 13.3 Transportingand Handling Placing Compaction 26 26 5 IS 456: ZOOO PAGE 27 27 27 13.4 ConstructionJoints and Cold Joints 13.5 Curing 13.6 Supervision 27 14 CONCRETING UNDER SPECIAL Cosornoss 15 27 14.1 Work in Extreme Weather Conditions 14.2 Under-Water Concreting 27 SAMPLING AND STRENGTH OF DESIGNED CONCRETE MIX 29 15.1 General 15.2 Frequency of Sampling IS.3 Test Specimen 15.4 Test Results of Sample 29 29 29 29 16 ACCEPTANCE CRITERIA 29 17 30 INS"EcrlON AND TESTING OF STRUCTURE SECTION 3 GENERAL DESIGN CONSIDERATION 18 19 20 BASES RlR DESIGN 32 18.1 Aim of Design 18.2 Methods of Design 32 32 18.3 Durability, Workmanship and Materials 18.4 Design Process 32 LOADS AND FORCES 32 t 9.1 32 32 General 19.2 Dead Loads 32 19.3 Imposed Loads, Wind Loads and Snow Loads 19.4 Earthquake Forces 32 32 19.5 Shrinkage, Creep and Temperature Effects 32 19.6 J9.7 19.8 19.9 33 Other Forces and Effects Combinationof Loads Dead Load Counteracting Other Loads and Forces Design Load 33 33 33 STABILITY OF THE STRUC1lJRE 33 20.1 33 Overturning 20.2 Sliding 20.3 Probable Variation in Dead Load 33 33 20.4 MomentConnection 20.5 Lateral Sway 33 33 21 FIRE REsiSTANCE 33 22 ANALYSIS 34 22.1 General 22.2 Effective Span 34 34 22.3 Stiffness 3.5 6 IS 456: 2000 PAGE 23 24 25 26 27 22.4 Structural Frames 35 22.5 Moment and Shear Coefficients for Continuous Beams 35 22.6 Critical Sections for Moment and Shear 36 22.7 Redistribution of Moments 36 36 BEAMS 23.0 Effective Depth 36 23.1 T-Beams and L-Beams 36 23.2 Control of Deflection 37 23.3 Slenderness Limits for Beams to Ensure Lateral Stability 39 SOLID SLABS 39 24. 1 General 39 24.2 Slabs Continuous Over Supports 39 24.3 Slabs Monolithic with Supports 39 24.4 Slabs Spanning in Two Directions at Right Angles 41 24.5 Loads on Supporting Beams 41 COMPRESSION MEMBERS 41 25.1 Definitions 41 25.2 Effective Length of Compression Members 42 25.3 Slenderness Limits for Columns 42 25.4 Minimum Eccentricity 42 REQUIREMENTS QOVERNING REINFORCEMENT AND DETAILING 42 26. I General 42 26.2 Development of Stress in Reinforcement 42 26.3 Spacing of Reinforcement 45 26.4 Nominal Cover to Reinforcement 46 26.5 Requirements of Reinforcement for Structural Members 46 50 EXPANSION JOINTS SECTION 4 SPECIAL DESIGN REQUIREMENTS FOR STRUCTURAL MEMBERS AND SYSTEMS 28 51 CONCRETE CORBELS 28.1 28.2 51 General Design 51 51 29 DEEP BEAMS 29.1 29.2 29.3 30 51 SI 51 General Lever Arm Reinforcement RIBBED, HOLU)W BLOCK OR VOlDEn SLAB 52 30.1 30.2 General 52 Analysis of Structure 52 30.3 30.4 Shear 52 Deflection 52 7 IS 456: 2000 PAGB 31 30.5 30.6 Size and Position of Ribs Hollow Blocks and Formers S2 52 30.7 30.8 Arrangement of Reinforcement PrecastJoists and HollowFiller Blocks 53 53 .53 53 FLAT SLABS 31.1 31.2 31.3 31.4 31.5 31.6 31.7 31.8 General Proportioning Detenninationof Bendin. Moment S3 S3 54 Direct Desip Method 5'6 EquivalentFnme Method Shear in Flat Slab Slab Reinforcement Openingsin Flat Slabs S1 .59 61 32 WAUS 32.1 General 32.2 EmpiricalDesignMethodfor Wall~ Subjected to Inplane Vertical Loads 32.3 WallsSubjectedto CombinedHorizontal and Vertical Forces 32.4 Design for Horizontal Shear 32.S Minimum Requirements for Reinforcement in Walls 61 61 33 63 34 STAIRS 33.1 Effective Span of Stairs 33.2 33.3 Distribution of Loadingon Stairs Depth of Section 61 62 62 62 63 63 63 FOOT1NOS 63 34. J 34.2 34.3 General 63 Moments and Forces Tensile Reinforcement 64 65 34.4 Transfer of Load at the Base of Column 6S 34.5 Nominal Reinforcement 66 SECTION 5 STRUCTURAL DESIGN (LIMIT STATE METHOD) 3S 3S.1 35.2 35.3 3S.4 36 67 SAFETY AND SERVICEAlIUI'Y RsoUIREMBNTS General Limit State of Collapse Limit States of Serviceability Other Limit States CHARACTBRISTIC AND DEsIGN 67 67 67 67 V ALtms AND PAR11AL SAFETY FACIORS 36.1 Ch8rIcteristic Strenath of Materials 36.2 CharacteristicLoads 36.3 Desip Values 36.4 Partial Safety Factors 67 67 68 68 68 37 ANALYSIS 37.1 67 68 Analysis of Structure 8 . IS 456: 1000 PAGE 38 LIMIT STATB OPCOLLAPSE: FLEXURE 69 38.1 69 A.lumptions 39 LIMIT STATB OF COUAPSS: COMPRESSION 39.1 Assumptions 39.2 39.3 39.4 39.5 39.6 39.7 70 MinimumEccentricity Short Axially Loaded Members in Compression Compression Members with HelicalReinforcement Memben Subjected to Combined Axial Load and U~iaxial Bendins Memben Subjectedto Combined Axial Load and Biaxial Bending SlenderCompression Members 72 40 LlMrr STATS OP COLLAPSE: SHEAR 40.1 40.2 40.3 40.4 4O.S 41 42 43 70 71 71 71 71 71 71 Nominal Shear Stress DesianShear Strensth of Concrete 72 12 Minimum ShearReinforcement DesiSD of Shear Reinforcement Bnhanced ShearStrength of Sections Close to Supports 72 72 74 LIMrr STATE OP COLLAPSB : TORSION 41.1 General 41.2 Critical Section 41.3 Shear and Torsion 41.4 Reinforcement in Members Subjected to Torsion 74 LIMIT STATE OF SBRVlCEABD.nY: DEFLECTION 75 42.1 75 74 7S 75 75 FlexuralMembers 43.1 FlexuralMembers 16 76 43.2 Compre~ion 76 LIMIT STATE OF SERVICEABILITY' CRACKING Members ANNEX A LIST OF REFERRED INDIAN STANDARDS 71 ANNEXB STRUCTURAL DESIGN (WORKING STRESS METHOD) 80 B-1 B-1.1 General Design Requirements 80 B-l.2 Redistribution of Moments Assumptions for Design of Members 80 80 B-l.3 B-2 80 80 80 80 PBRMIsslBLB STRESSBS 8-2.1 8-2.2 B-2.3 B-3 80 GENERAL Permissible Stresses in Concrete Permissible Stresses in Steel Reinforcement Increase in Permissible Stresses 81 PBRMIssIBLE LoADS IN COMPRBSSION MEMBERS B-3.1 8-3.2 B-3.3 8-3.4 211e 815/07-3 81 Pedestals and Sbort Columns with Lateral Ties Shon Columns with Helical Reinforcement Lon. Columns Composite Columns 81 81 "\r. 81 IS456:~ PAGI B-4 MEMBBRS SUlJBCTID TO COMBINED AxIAL loAD AND BINDING 83 8-4.1 B-4.2 83 83 83 B-4.3 D-S 83 SHEAR B-S,1 B-5,2 B-S.3 B-5.4 B·'.' B-6 De,iID Baed on Uncracked Section Delilft Baed on Cracked Section Members Subjected to Combined Direct Load and Flexure Nominal ShearStress . neaip ShearStrenlth of Concrete Minimum Shear Reinforcement Desiln of ShearReinforcement Enhanced Shear Strength of Sections Close to Supports TORSION B-6.1 General B-6.2 B-6.3 B-6.4 Critical Section Shear and Torsion Reinforcement in Members Subjected to Torsion e-l C-4 DIFLECI10N DUE TO CREEP DBPLECI10N DuE TO SHRINKAGE ANNEX D SLABS SPANNING IN TWO DIRECTIONS 0·1 D-2 IUmtAINID 85 8S 86 86 86 86 86 88 88 88 89 TOTAL D8PLIIcnON SHOIlT- TBIM DBPLICTION 84 8S 88 ANNEX C CALCULATION OF DEFLECTION C-2 C-3 83 90 90 90 SLAM SIM,ty SuppotnS SUBS ANNEX B SPPRCTIVI LaNOTH OF COLUMNS 92 ANNEX F CALCULAnONOF CRACK WID1lI ANNEX G MOM!NTS OP ltBSlSTANCB FORRECTANGULAR AND T-SECI10NS 95 G-l RscrANOULAR SBC110NS 0-1.1 0-1.2 0-2 Sections without Comprealion Reinforcement Sections with Compression Reinforcement 96 96 96 96 96 FLANOED SEC110N ANNEX H COMMITTEE COMPOSITION 98 10 AMENDMENT NO. I JUNI .1 TO IS 45' I 2000 PLAIN AND REINFORCED CONCIITI- CODI or PRACI'ICE ("owI" R,,,,,,,,,,) ,."bu'OII' (PIa' 2, FONWOrd, II,.,) - Subltltute 'Aa318: 1995' for tAClII', i.'. (PilI' 1I, C/4UH ~ ) -,Delete tII,maler 'L. - HorllDntll dlltlDCI c.DtIII oflateralllllnla,'. .&we.. (Pill' 15. c/tllU.,.J. Till,) - Subltltute 'CIa••leal Ad_lxlu. .' lor 'Ad.IIt.....'. . (Pal- 17, clGUIf 7.1 ) - SubltllUte Ibe followln, for tileexlaliDl IDfomal IIble: DI,,_o/ Placlll' CDndlllt»u WorluJbUlly BUDdinl concrete; Shallowaeetlonl; 'avementa ullns plven (11IIII) (2) (1) } • SIw¥ (3) Very low S.'.l.l Ma.. concrete; Uptly reinforced ICctioDi inIJ. hi, belma, willa, columna; 25-75 Low Floon; Hind placed pavements; Canal lining; Stripfootings Heavily reinforced sections inslabs, beams, walla, columna; Slipform work; Pumped concrete Trench fi1l; In-situ piling } Medium 50-100 ] ] Medium 75·100 Tremie concrete High 100 ·IS0 Veryhigh See 7.1.1 Nom - For moat of ... placiD. conditions, internal vilnlOIS (aeedle vibralorl) .re suitable. TIle eli..... fIl determined baaed 08 the density and spaciDI of reinforcement bars IDd thieD" of IeCIioIL For tlemi. ~ va 10 beused(su .Lto 113). .. aN ... (Page 19, Table 4, columnS, ,ub-heading) - Substitute 'Free' for 'Face' • ( Page 27, claus« 13.5.3) - Delete. ( PQge 29, clause 15.3 ): a) Substitute 'specimens' lor 'samples' in lines 2, 61nd 7. b) Substitute 'IS 9013' lor 'IS 9103' . (Page 29, clause 1'.1 ) - Substitute 'conditions' for 'condition' in line 3 and tbe foJlowinl ....ua for lilt e~ :'matter against 'I)' : 'I) The mean strengtb determined from any group of Cour non-ovcriappiM coftlCCUtive lal.-IIII'DIIPIIII_" appropriate limits in column2 of Table 11.' I. ( Ptl,~ 29, claus« 1'.3, par« 2 ) - Substitute 'col 3 t lor 'col 2' . ( Page 29, clalUe 1'.4, line2 ) - Substitute C16.1or 16.2 as the case may be'lor '1'.3-. :. ;~. ( Ptl,~ 30, Table II, colum" 3 ) - Substitute '~Ick - 3' lor 'a Ie..-3, Ind ,oj ,:~~·Prlc. Greup 3 1 a_ I.. "II 4 t,or '.!........ Amend No.1 to IS 456: 2000 (Page 33, clause21.3, line 2 ) Hll>stIMUlcticlt' f~'section'. -:- ~bstilUte 'b '-'O~ ~~lo' lor '1 [Page 37, clause 23.:.2~6 ( Page 46, clause Z6.4!"- ~bstil:F¥.\3rfor 8.2.3'. 0'. 'b'lor 'b' and 'b: lor 'b: in the formulae. I. l Page 49, clause 26.5.3.1 (c) (2), lasI line] - Substitute '6 mm' for' 16 mm'. (Page 62, clause3%.Z.5 ) - ~ubstitute 'H;" for 'Hw e ' in the explanation of e._ (Page 62, clause3%.3.1, line 4 ) - Substitute '32.4' lor '32.3'. [Page 62, clause3%.4.3 (b), line 6 ] - Insert '"few' between the words 'but' and 'shall'. [Page 65, clause34.%.4.1(1), lastline] - Insertthe foJlowing afterthe words 'depth of footing' : 'in case of footings on soils, and It a distance equalto half the effective deptbof footing', (Page 68, Table 18, col 4 ) - Substitute ,_, for '1.0' against tbe Load Combination DL +ll: (Page 72, clause 40.1 ) - Substitute 'bd' for 'bd ' in the formula. ( Page 83, clause B-4.J, line 2 ) - Delete the word 'and' . (Page 85, clauseB.5.5.1,para 2, line 6) - Substitute 'Table 24' for 'Table 23'. (Page 85, clause B-5.5.%) - Substitute the following for tbe existing formula: 'A. = Q) (T.y-2dT.e I Qy ) l«; ~ 0.4 Qyb / 0.87/., , (Page 90, clause »-1.11, line 1 ) - Substitute 'Where' lor 'Torsion'. ( Page 93, Fig. 27 ) - Substitute' 'efl' ' for 'IlL'. ( Page 95, Annex F ): a) The reference to Fig. 28 given in column 1 of tbe text along witb the explanationoCtbe symbols used in the Fig, 28 given thereafter may be read just before tbe formula given for the rectangular tension zone.. b) Substitute 'compression' for 'campression' in tbe explanationof symbol 'a ' . (Pages 98 to 100, Annex H) - Substitute the followingfor the existing Annex: ANNEX H (ForeM'ord) COMMfITEE COMI)OSITION Cementand Concrete Sectional Committee, CEO 2 CluJi,,,.,," DR tl. C. VDVESVARAYA ·Ch.ndrib·, 15· Cross, 63-64 EastParkRoad, a' MalleswaralD, Banplore-S60003 ~eprUQI/in, MeIJtbe,.f DaS. C. AHWWAUA OCL India Ltd, NewDelhi SHRIV. BAIASl/BRAMANlAN Stili R. P. SlNOH (Alle'lIDt~) Directorate General of Supplies andDisposals. NewDelhi SHRIG. R. BHAIUTKAR B. G. ShirkeConstruction TeQROlolY Lid,Pune SHRJA. K. CHADHA SHJU J. R. SIL (Al'erlUlle) Hindusran PreCab Limited, New Delhi . CmspENOINEBR (DfSlGN) ~ SUPI!IUNTBNDINO F.,NOINBa (S&,S) Central PuhlicWorksDepartment, NewDelhi (Alte'lUJle) CHIS' ENoINEBR (NAVOAM DAM) S.rdar Sarovlr Narmada Nipm Lad, Oandhilllir SUPElUNl'ENDINO ENaINEER (OCC) (Alter.'e) CHIEF ENGINEER (R!sfAICH}CUM..Dlitscroa IrriptiOlllnd Power ReIellCIa Institute. Amri..., REsEARCH OffICER (CONCREl! TecIINOUXiY) (A/terM/e) 2 ( CDIII~ CNI"" 3 ) Amend No.1 to IS 456: 2000 ( Coll,imuul from pa,e 2 ) RepresenJing Memben SHIll J. P. DesAi Gujaraa Ambuja Cements Lid, Ahmedabad SURI B. K. JAGEnA (A/ierMle) DlllEClOa JOINTDnucroR ""'muJte) AP. Engineering Research LahoralOries, Hyderabad DIRf.C1OIl (OdOD) (N&W) DPJVIY DIRlCIOR (CMDD) (NW&S) (A/tOlUJle) Cenlral Water Commission, New Delhi SHRIK. H.OANGWAL Hyderabad Industries lzd, Hyderabad StWV. PA1TABHI (Allemtlle) .r. SaNemrsl Engineering-It~r("h Centre (CSIR), Gha7jabad SHRIV. Ie.GHANBKAIl SHRIS. GoPINA11I SHRI R.TAM1lAJCAJlAN (Allenult~) TheIndia CemenlS LJd. Chennai SHIUS. K. GuttA THAKURTA SHIUS. SANKARANARAYANAN Gannon Dunkerley and Company. lAd, Mumbai (Alternate) SUIlI N.S. BUAL Central Building Research Institute (CSIR), Roorkee DR IRsHAD MASOOD PRoP (AltulIQle) University of Roorkee, Roorkee A K. JAIN SHRJ N.C. JAIN Cement Corporation of India Ltd,NewDelhi JOINT DlRBCTOR (STANDARDS) (B&S)(Cn..1) Research, Designs &. Standards Organization (Ministryor Railways). Lucknow JOINTDIIlPLiOR(STANDAaDS) (B&S) (CB-II) (Altenulte) SHIU N.G. JOSID The Indian Hume PipeCompany Lad, Mumbai SHRIP. D. KEUCAR (AIleJ'MIe) SHRI D. It KANUNOO SHuB. R. MBENA (Alterll4le) National Test Jlouse, Calculla SHRJ P. KJusilNAMUanlY Larsen &. Tuhro 1.Jd, Mumhai Stili S. CHoWOIWRY (AltulUlte) DRAG.MADHAVARAo SIW K. MAN! (AltnlUlle) Structural Engineering Research Centre(CSIR), Chennai SHIUJ. SAitUP Hospital Services Consultancy Corporation (Iodia) lid, NewDelhi SHRI V. Sl1RmH Housing andUrban Development Corporation lJd, NewDelhi Stili D.P.SINOH (AltmuJle) SHRJPRAFFuI.A KUMAR SHRI P. P.NAIR Ministry of Surface Transport. Department of Surface Transport(Roads Win&), New Delhi (A11el7Ulk) MBMBERSHCRETARY Central Board of Irrigation & Power, New Delhi DlllOCTOk(C'ML) (AlterlMle) SHRIS. K. NAnHANI Engineer-In-Chlef's Branch. ArmyHeadquarters, NewDelhi DR A S.GOBI.. (Alterll4.) SHRJ S.S. SEmIRA Central Road Research Institute (eJIR), NewDelhi SHRISATANDER KUMAR (AltOIUlIe) SHRIY. R. PHLU StlRl A. K SHARMA (AltG"rUIte) Indian Roads Congress. NewDelhi DR C. IWKUMAR DR K. MOHAN (Altemtllc) National Council forCement and Buildine Materials, BalJabprb SHRI S. A RBooI Gammon India lid. Mumbai REPRmIKl'A11W Builder's Association of India, Mumbai SHIIJ. S. SANOANEIUA SHIlL N. AnARWAL(AllemGle) Geological Survey of India. Calcutta Sl1PBRIN1BmING ENOINI'JIl (DfSION) ExID/l'M! ENoINm!.a (SMR DIVISION) (A/temale) PuNicWorks Depanment. OovemmeDI or TamilNadu, Cbennai SHIU Ie. K.. TAPAIUA SHIll A. Ie.JAIN (AI'......te) Indian Rayon andIndustries I.Jd, Puoe SHRI T.H" TIwARI OR D. GlaH (AlIe",,'e) The Associated CementCompanies l.Jd. Mumbai DR K. VINCATAaIALAN CentralSoil.nd MaterialsResearch StatiOft, New Delhi SHRI N. CHANDIlASIICAlAN (AI'.....Ic) 3 ( Continuel 011 POse .. ) Ant.nd No.1 &0 IS 4_ I 2000 (COIIIiIlMM"""" J J AI. .... If"""'", BnaI-- DaH.e. V.~AJAYA 'I\IlMdlutlol or StW YINOD KuMAa DIrtcIo, 0.1....1. 81S (I:M-oIJtc1tJ",....) SHII D.C. CM1\JMDI(A~"") (lDdI.~ Callull 0111010' (elY Bag) M..".,.",.ti• • taU I. Ie. PI.AMD Addition.. DlrtOIOr (elv Bla). ,., Depu~ I'IIIIAMIAY PANT PtrNlOr (Ov __• 811 Concrete IUbcq",mlne" CEO 2:3 It.,..".", Nadonal Council torClm.Dllnd Bulldin. MI••rlall, SHRI C. R. AuMCHANDANI BaU."'" I hlp Conaullintl LId, Mumbal SHRII. RANaAIWAN (AII.rlllll.) DaP.C. OiowDHURY OaC.S. VISHWANA11IA (A't.'IIII'.) SHRll.·P. DIBAI SHKi B. It JAOBTIA (Alte,,,.,.) Torsteel ROlelrch Poundalloa InIndia, Calcutta Oujlnl Ambuja Cemenll Lad, Ahmedabad Celli'll SoliIDd Mlteria. DIRSC10R ae..ucb 5lado.. New Deihl SHRI N. OwmIWBlCAIAN (A"erute) Ceaenl WlterCommiuion. New Delbi DUUICIOa (CANDO) DBPUTY DIUC10I (CANDD) (AI,.",.,-) JOINT DIIBC10RSTANDAIlDI CB.lS)CB-1I JOINTDIIBC1015TANDAaDS (A It.,,,,,,.) Re_reb. DeliJIII ud SliDell" O'alnizatioD ( MlDistry of Railwayl). lJacbow (BAs)ICB-r SUPERINTI!NDINO ENaMEl cDJ!SIONS) Central Public Worb Department. New Delhi Ex!cUl1Vl ENGINeeR (DBIIONS)-111 (Aile,.".'.) SHRIV. K. OHANEKAR SHRI D. S.PRAKASH RAo (AI,.,,",,e) Structural Eneineerina Research CeDtre (CSIR). Ohazilbad SHai S.Ie. OUHA l'IwaJaTA SHRIS. P. SANICAIANARAYANAN (AllerMte) Gannon Dunkerley andCo Lad. MWDbai StDUJ.S.~~ Associated Consultina Services. Mumbai SHRI L It JAIN InpenoDiI capacity SHRI M. P. JABINOH DR B. KAMBSWAIlARAo(Aller".,e) Cenlral Buildinc RCleirch InsdlUle (CSIR), Roorbe CHIU ENoINUR A JOINT SECRBTAILY SUPI'JlIN1'DIDINO ENoINBBR (AI'.....") Public Works [)e.-rament, Mumbai PIIoP S. Ka.1IMA Mool11lY lodi.. IOlbtUIe of TechaololY. Now Delhi SHIU K. K. NAvAIl(Altc,.,..te) DaS.C.MArn NadoDal Couldl for Ce"••'I.d BuildiD, Materiala. Ballabprla MANAOING DIUCTOI Mild.-taD Prefab UlDileCl. New Delhi S... M. KUNDU (AI,.".,.) Stili S. K. NAn1tANI LT-COL Ie. S. CHAaAK SHRIB. V. B. PAl (A'''''''') S... M.G. DANDvA'n (AI.......) ne AuociIIedc...a' CompilitllJd. Mum'" SNRI A. B. PHADa S... D.M.SAvua (AI,.",.,.) n. HiDdUltll CoIIINCdol ColJd. M.....I SHRI Y. R.PHuu. S...S.S. S.1iIA I) SHIISATANDIIKUMAI(Al,.,.tcll) Cea....1Road ReIeIrch IDlIiIUIe (CSIR). New Dellai (A'''''''''' 4 (C~_".,.5) Amend No.1 to IS45' : 2000 ( c.,;,.".".".,.,...) If."....,;". /;I...." SMII A. I. PwAD RAo SHU K. MANI (AI,.".,") Structural &aln••rinl ReMarch C.nIN (CSIR), Chona.' IHI. JC. L Pima N.tlonal Bulldi SHIll. R. OA...IL(A',."....) 1...8. D.lAHAucal StiliU. S.P.VIlMA ~/"""") SHII~RAo StiliG. RAMAICI.HMAN CAl'.",.") SHIll. A. RIDD. Da N.JC. NAVAl (AI,.,,...) ft' Conltructlon Corponlion Lad. New Delhi Nuclear Power Corporation, MUlllbai A.P. En,I'''''''1 Reaearch LabonlOrica, Hydenbad Gammol India LId. Mumbai SHRII. C. SAWHNIY SHI.R. P. MIHIOTIA CAl"",.") anainOl,. India IJd. New Delhi Pao,M.S.SHIm' IDdian Concrole In'lhule,Chonnll SHiI N. K. SINHA SHIIB. T. UNWAUA Minlaary or Surface Traftlporl (Road. Wina), New Delhi Inpenonal capacity Panel for Revision or IS 456, CEO 2:2IP RepNlCnl;lt, National Council for Cement andBuildin.Material., aaUabprh AI.,.,.., 01 ANlL KUMAR SURIV. K. OtlANBlCAR National Council for Comenl and Dulldln, Malerials, BaUabaarb Structural Enaineerinl Rete.rehCentre (CSIR), Ohazilbad Paa. A It JAIN University of Roorkee, Roorke., SHII L K.JAIN InperlOnal capacity StlRIJOI! KURIAN Centr.1 Public Worlcl Department, New Deihl DaS.C.MAm Nallonal Coundl forCemcnllndDuildin. Material., BlUablarh DR A. K. MnTAL Central Public Workl Department, New DeIhl SHRI S. A. RsoDI GAmmon India Lcd, Mumbai DR V. THlRlNBNODAM School of Planninaand Architecture, New Delhi Special Ad-Hoc Group forRevision of IS 456 Convener DR H. C. VISVP.5VAItAVA 'Chandrika', II 15d1 Cross. 63-64 BasI Park Road, Malleswaram. Banaalore..S60003 DR C. IWKUMAR National Council ror Cement and Suildina Materials, Ballabearb S"IU S. A. REDol Gammon India LJd, Murnbai (CED2) 5 II .. • 2 AMENDMENT NO. TO IS 456: 2000 2~Or SE'riMBER ~. tW\U'" PLAI.N AND REINFO~D CONCRETE CODE OF 'PRACTICE ( FIJUrth Revision) , ( Page 13, clause 5.2.1.1, line 1 ) 'Grade rens 3812'. Substitute 'IS 3812 (Part 1)' for ( Page 13, clause 5.2.1.2 and corresponding Note ) following for theexisting: Substitute the . Silica fume conforming to IS 15388 may be used as partreplacement of cement provided uniform blending with the cement is ensured. NOTE - Silica fume is usually used in proportion of content of a mix.' ~ to 10 percent of the cement t Page 13. Note under clause 5.2.1.3, line 5 ) - Substitute 'be' for 'range from being'! . ( Page 25.. clause 10.3.3, line 4 ) - Delete the word 'and'. ( Page 65. clause 34.2.4.2. line 1 ) - Substitute 'on' for 'or'. [ Page 65. clause 34.3.1 (a).. line 2 I - Delete the words direction' . ~extending in each ( Page 66, clause 34.4.3.. line 5 ) - Substitute 'not' for 'no'. ( Page 78,..1nnex A ) - Substitute the following for the existing entries for 153812: 1981: ·/S 1\/0. ,Title IS 3812 (Part 1) : 2003 Specification for pulverized fuel ash : Part I For usc as pozzolana in cement, cement mortar and concrete (secondrevision)' ('Page 79. Annex A ) ._-- Add the following at the end: 41~')1 No. IS 15388 : 2001 2116 815/07-1 Title Specification for silica fume' (p. ... 80, 1-2.1.1, Ilf/oIfIMllabl, ) -Inlert the foUowlftlln the table: • 5.6 ( Pag, 81, TtJbl, 21 )-Insert the followiftl row after the IMt row: '(1) (2) (3) (4) M'S 17.5 13,0 I." ( Pag, 91, TtJbl, 26, eMf No.2, col 2 ) - Subltitute 'OM Short Ed•• DilOOlltlnuou.' lor 'OnIlhoit Ed.. Conti.....' , [PGI,96, G-1.l(c)./olWlIl/G ] -Subltitute 'MuJiII'/o, 'My'um', [Pagl96, G-l.1(d), ,.,"'" ] -Subltitute '31.1I /0' '39.1 I. (CED2) 2 18 456: 2000 Indian Standard PLAIN AND REINFORCED CONCRETE CODE OF PRACTICE ( Fourth Revision ) FOREWORD ThisIndianStandard (Fourth Revision) wasadopted by the Bureau of Indian Standards, afterthedraftfinalized . by theCementandConcrete Sectional Committee hadbeenapproved by theCivilEngineering Division Council. This standardwas first published in 1953 underthe title 'Codeof practice for plainand reinforced concrete for general building construction' and subsequently revised in 1957. The code was further revised in 1964 and published under modified title 'Code of practice for plainand reinforced concrete', thusenlarging the scopeof use of this code to structures otherthan general building construction also. Thethirdrevision was published in 1978, and it includedlimit state approach to design. This is the fourth revision of the standard. This revision was takenup witha viewto keeping abreast withthe rapiddevelopment in the fieldof concrete technology and to bringin furthermodifications/improvements in the lightof experience gained whileusingtheearlierversion of the standard. This revision incorporates a number of important changes. The majorthrustin the revision is on the following lines: a) In recent years. durability of concrete structures have become the cause of concern to all concrete technologists. This has led to the needto codify the durability requirements worldover. In this revision of the code. in order to introduce in-built protection from factors affecting a structure, earlierclause on durability has been elaborated and a detailed clause covering different aspects of design of durable structure has been incorporated. b) Sampling and acceptance criteriafor concrete havebeenrevised. With this revision acceptance criteria has been simplified in line with the provisions given in BS 5328 (P8l1 4):1990 'Concrete: Part 4 Specification for the procedures to be used in sampling, testing and assessing compliance of concrete'. Some of the significant changes incorporated in Section 2 are as follows: a) All the threegrades of ordinary Portland cement, namely 33 grade, 43 gradeand 53 gradeand sulphate resisting Portland cement have been included in the list of types of cementused (in addition to other types of cement). b) The permissible limits for solids in waterhavebeen modified keeping in viewthe durability requirements. c) The clause on admixtures has been modified in view of the availability of new types of admixtures including superplasticizers. d) In Table2 'Grades of Concrete', grades higherthan M 40 have been included. e) It has been recommended that minimum grade of concrete shall be not less than M 20 in reinforced concrete work (see also 6.1.3). f) The formula for estimation of modulus of elasticity of concrete has been revised. g) In the absence of proper correlation between compacting factor, vee-bee time and slump, workability has now been specified only in termsof slump in line withthe provisions in BS 5328(Parts 1 to 4). h) Durability clausehasbeenenlarged to include detailed guidance concerning thefactors affecting durability. The table on 'Environmental Exposure Conditions' has been modified to include 'very severe' and 'extreme' exposure conditions. This clause also covers requirements for shape and size of member, depthof concrete cover, concrete quality, requirement against exposure to aggressive chemical andsulphate attack,minimum cementrequirement andmaximum watercementratio,limitsof chloride content. alkali silica reaction, and importance of compaction, finishing and curing. j) Aclause on -'Quality Assurance Measures' has been incorporated to givedue emphasis to goodpractices of concreting. k) Properlimitshavebeenintroduced on theaccuracy of measuring equipments to ensureaccurate batching of concrete. 2116 BIS/07-:.!. IS 456: 2000 m) The clause on 'Construction Joints' has been modified. n) The clause on 'Inspection' has been modified to give more emphasison quality assurance. The significant changes incorporatedin Section 3 are as follows: a) Requirements for 'Fire Resistance' have been furtherdetailed. h) 'The figure for estimation of modification factor for tension reinforcement used in calculation of basic values of span to effective depth to control the deflection of flexural member has been modified. c) Recommendations regarding effective length of cantilever have been added. d) Recommendations regardingdeflection due to lateral loads have been added. e) Recommendations for adjustmentsof support moments in restrainedslabs have been included. f) In t.he detemination of effective length of compression members.stability index has been introduced to determine sway or no sway conditions. g) Recommendations have been made for lap lengthof hooksfor bars in direct tensionand flexuraltension. h) Recommendations regarding strength of welds have been modified. j) Recommendations regarding cover to reinforcement have been modified. Cover has been specified based on durability requirements for differentexposureconditions. The term 'nominal covert has been introduced. The cover has now been specified based on durability requirement as well as for fire requirements. The significantchange incorporated in Section4 is the modification of the clauseon Walls. The modifiedclause includes design of walls against horizontal shear. In Section 5 on limit state method a new clause has been added for calculation of enhanced shear strength of sections close to supports. Some modifications have also been made in the clause on Torsion. Formula for calculation of crack width has been added (separatelygiven in Annex F). \Vnrking stress method has now been given in Annex B so as to give greater emphasis to limit state design. In thisAnnex, modificanonsregarding torsion and enhanced shear strengthon the same lines as in Section 5 have been made, Whilst the common methods of design and construction have been covered in this code, special systems of design and construction of any plain or reinforcedconcrete structure notcovered by this code may be permitted on production of satisfactory evidence regarding their adequacy and safety by analysis or test or both (see 19). In this code it has been assumed that the design of plain and reinforcedcement concrete work is entrusted to a qualifiedengineerand that theexecutionof cementconcretework iscarriedout underthe directionof a qualified and experienced supervisor. In the formulation of this standard, assistance has been derived from the following publications: BS 5328 : Part 1 : 1991 Concrete: Part 1 Guide to specifyingconcrete, British Standards Institution BS 5328 : Part 2 : 1991 Concrete : Part 2 Methods for specifying concrete mixes, British Standards Institution BS 5328 : Part 3 : 1990 Concrete: Part 3 Specificationfor tbe procedures to be used in producing and transporting concrete. British Standards Institution BS 532R : Part 4 : 1990Concrete; Part 4 Specification for the proced.ures to be used in sampling, testing and assessing complianceof concrete, British Standards Institution BS 8110 : Part 1 : 1985 Structural use of concrete: Part t Code of practice for design and construction, British Standards Institution BS RItO: Part 2 : 1985 Structural use of concrete: Part 2 Code of practice for special circumstances, British Standards Institution ACT 319 ~ 1989 Building code requirements for reinforcedconcrete, AmericanConcrete Institute AS 3600 : 1988Concrete structures. StandardsAssociationof Australia 2 -.... IS 456: 2000 DIN 1045July 1988Structural use of concrete, design and construction. Deutschcs lnsritut fur Normung E.V. CEB..FIP Model code 1990, Comite Euro .. International Du Bclon The composition of the technical committee responsible for the formulation of this standard is given In Annex H. For the purpose of deciding whether a particular requirement of this standard is complied with, the final value, observed or calculated, expressing the result of a test or analysis shall he rounded off in accordance with IS 2: 1960 'Rules for rounding off numerical values (revised)'. The number of significant places retained in the rounded off value should be the same as that of the specified value ill this standard. 3 IS 456: 2000 SECTION 1 GENERAL - 1 SCOPE EL 1.1 This standard deals with the general structuraluse of plain and reinforced concrete. 1.1.1 For the purpose of this standard, plain concrete structures are those where reinforcement, if provided is ignoredfor determination of strengthof the structure. 1.2 Special requirements of structures, such as shells, folded plates, arches.bridges,chimneys,blastresistant structures, hydraulic structures, liquid retaining structures and earthquakeresistant structures,covered in respective standards have not been covered in this standard; these standards shall be used in.conjunction with this standard. E. - e - let. - t; f t1 t, I, H. Hwe Ie( 1 - 2 REFERENCES The Indian Standards listed in Annex A contain provisions which through reference in this text, I, - 'f - constitute provisions of thil standard. At the time of publication, the edition. indicated were valid. All standards are subject to revision and parties to agreements based on this standard are encouraged to investigate the possibility of applying the most recent editions of the standards indicated in Annex A. . K k Ld U - Lw - 3 TERMINOLOGY - For the purpose of this standard, the definitions Biven in IS 4845 and IS 6461 (Parts 1 to 12) shall generally apply. 4 SYMBOLS For the purpose of this standard, the following letter symbols shallhavethe mcanina indicated against each; where other symbols are used. they are explained at the appropriate place: A - Area b - Breadth of beam, or shorter dimension of a rectanguler column bet" Effective width of slab b, Effective width of flanac b., - Breadth of web or rib D - Overall depth of beam or slab or diameter of column; dimension of a rectangular column in the direction under consideration Dr - Thickness of flange DL - Dead load d - Effective depth of beam or slab d' - Depth of compression reinforcement from the highly compressed face Ec - . Modulus of elasticity of concrete ler - lea - Iey - I. I'n - I" ly 10 I. - - 12 - I' - 2 M m n p q" 11 - - - Earthquakeload Modulus of elasticity of steel Eccentricity Characteristic cube compressive stren.th of concrete Modulus of rupture of concrete (flexural tensile aU-oath) Splittin, tensile lU'eftltb of concrete Desip Itren,th Characteriatic ItrenJth of steel Unsupportedhei,ht of wall Effective hei,ht of wall Effective moment of inertia Momentof inertia of the gross section excluding reinforcement Moment of intertiaof cracked section Stiffness of member Constant or coefficient or factor Developmentlength Live load or imposed load Horizontal distancebetweencentresof lateral restraint Length of a column or beam between adequate lateral restraints or the unsupportedlength of a column Effective span of beam or slab or effective length of column Effective length about x-x axis Effective leng~ about y-y axis Clear span, face-to-face of supports for shorter of the two spans at right &lgles Length of shorter lide of slab Lin.th of loftier aide of slab Distance between points of zero I: lnomen.. in a beam Span in the direction in which moments are determined, centre to centre of supports Span transv~se to I" centre to centre of supports 12 for the shorter of the; continuous spans Bendin. moment Modular ratio Number of samples Axial load on a compression member Calculatedmaximumbearingpressure IS 456: 2000 qn - Calculated maximum bearing pressure of soil r - Radius s - Spacing of stirrups or standard deviation T - Torsional moment Ym 8m e ec Partial safety factor for material Percentage reduction in moment Creep strainof concrete G&:hI; Permissible stress in concrete in bending compression a&;e Permissible.stress in concrete indirect compression oftK: - Permissible stress in metal in· direct compression GM: - Permissible stress in steel in compression (J", - Permissible stress in steel in tension a"v - Permissible tensile stress in shear reinforcement t hd - Design bond stress t&; Shear stress in concrete t e• mI&X- Maximum shear stress in concrete with shear reinforcement - Wall thickness V - Shear force W - Total load WL Wind load w - Distributed load per unit area Wd Distributed dead load per unit area WI Distributed imposed loadper unitarea x Z - Depth of neutral axis Modulus of section l - a. 8 Yr - Lever arm Anile or ratio Partial safety factorfor load .. J:! - 'tv - Nominal shear stress , - Diameter of bar IS 456: 2000 SECTION 2 MATERIALS, WORKMANSHIP, INSPECTION AND TESTING have no relation whatsoever with the characteristics guaranteed by the Quality Marking as relevant to that cement. Consumers are, therefore, advised to go by the characteristics as given in the corresponding Indian Standard Specification or seek specialist advise to avoid any problem in concrete making and 5 MATERIALS s.t Cement The cement used shall he any of the following and the type selected should be appropriate for the intended use: a) 33 Grade ordinary Portland cement conforming to IS 269 b) 43 Grade ordinary Portland cement conforming to IS 8112 c) S3 Grade ordinary Portland cement conforming to IS 12269 d) Rapid hardening Portland cement conforming to IS 8041 e) Portland slag cement conforming to IS 4;5 5.2.1.1 Fly ash (pulverized fuel ash) f) Portland pozzolana cement (fly ash based) conforming to IS 1489 (Part 1) g) Portland pozzolana cement (calcined clay based) conforming to IS 1489 (Part 2) Fly ash conforming to Grade 1 of IS 3812 may be used as part replacement of ordinary Portland cement provided uniform blending with cement is ensured. h) Hydrophobic cement conforming to IS 8043 j) Low heat Portland cement conforming to IS 12600 k) Sulphate resisting Portland construction. 5.2 Mineral Admixtures 5.1.1 Pozzolanas Pozzolanic materials conforming to relevant Indian Standards may be used with the permission of the engineer-in-charge, provided uniform blending with cement is ensured. 5.2.1.2 Silicafume Silica fume conforming to a standard approved by the deciding authority may be used as part replacement of cement provided uniform blending with the cement is ensured. cement NOTE-The silica fume (very fine non-crystalline silicon dioxide) isa by-product of the l1UU1ufacture of silicon, ferrosilicon or the like. from quartz and carbon in electric arc furnace. It is usually used inproportion of Sto 10percent of the cement content of a mix, conforming to IS 12330 Other combinations of Portland cement with mineral admixtures (see $.2) of quality conforming with relevant Indian Standards laid down may also be used in the manufacture of concrete provided that there are satisfactory dati on their suitability, such as performance test ~ concrete containing them. 5.1.1 Low heat Portland cement conforming to IS 12600 shall be used with adequate precautionswith regard to removal of formwork, etc. 5.1.1.3 Rice husk ash Rice husk ash giving required performance and uniformity characteristics may be used with the approval of the deciding authority. NOTE-Rice husk esh is produced by burning rice husk and contain largeproportion of silica. To achieve amorphous state, ricehusk ahay beburntat controlledtemperature, It is necessary toevoluat8 the productfroma particularsourcefor performance and unirofmity since it con ran,e from beinl as deleteriousas silt when.~ncorporated in concrete. Waterdemand and dryinl shrinkage ',should be studiedbefore using rice husk. 5.1.Z Hiah alumina cement conforming to IS 6452 or supersulphated cement conforming to IS 6909 may be used only under special circumstances with the prior approval of the engineer-in-charge. Specialistliterature Inay be consu Ited for guidance regarding the use of 5.2.1.4 M'takaoline these types of cements. 5.1.3 The attention of the engineers-in-charge and users of cement is drawn to the fact that quality of various cements mentioned in 5.1 is to be determined on the basis of its conformity to the performance characteristics given in the respective Indian Standard Specification for that cement. Any trade-mark or any trade nameindicating any special features not covered in. the standard or any qualification or other special performance characteristics sometimes claimedl indicatedon the bass or containersor in advertisements alongside the 'Statutory QualityMarking' or otherwise Metakaollne having fineness between 700 to 900 m 2/kg' may be used as pozzolanic material in concrete. NOTE-MetokQoline is obtained by calcination of pure or refined koollntic clay orD temperature between 6500C and 8~O°C, followed by .rindin. to achieve a fineness of 700 to 900 m:llka. The resultiDI material hOI hilh.'pozzoianicity. S.2.2 GroundGranulated Blast Furnace Slag Ground granulated blast furnace slag obtained by grinding granulated blast furnace slag conforming to IS 12089 may be used as part replacement of ordinary 13 IS 456: 2000 Portland cements provided uniform blending with cement is ensured. 5.3 Allre.ates Aggregates shall comply with the requirements of IS 383. As far as possiblepreferenceshall be givento natural aggregates. . 5.3.1 Other types of aggregates such as sial and crushed overbumt brick or tile, which may be found suitable with regard to strength. durability of concrete andfreedom from harmful effects may be usedforplain concrete members. but such aggregates should not contain more than 0.5 percentof sulphates as SO]and should not absorb more than 10 percent of theirown mass of water, 5.3.2 Heavy weight aggreiates Of light weight aggregates such as bloatedclay aggregates and sintered fly ash aggregates may also be used provided the engineer-in-charge is satisfied with the data on the properties of concretemade with them. NOTE-Some of the provisioDI of the code would require modIfication whenthese alPlates areused: speclalilt literatuJe may be consulted for auidance. 5.3.3 Sizt ~f Aggregate Thenominal maximum sizeofcoarse aggregate should be as large as possible within the limits specified but in no case greater than one-fourth of the minimum thickness of the member, provided that the concrete can be placed without difficulty so as to surround all reinforcement thoroughly and fill the comers of the form, For most work, 20 nun alareaate is suitable. Where there is no restriction to the flow of concrete into sections, 40 nun or laraor size may be permitted. Inconcrete elements withthinsections, closelyspaced reinforcement or smallcover, consideration should be liven to the use of 10 mm nominal maximum lize. Plums above 160 nun and up to any reuonable aize may be used in plain concreteworkup to a maximum limit of 20 percent by volume of concrete when specifically permitted by the enaineer-in-charao. The plums shallbedistributed evenly andIhall benotcloser than 1'0 mm from the lurface. 5.3.3.1 For heav.iJy reinforced concrete memben u in the else of ribs of main beams, the nominal maximum aize of the a'lf'late Ihould usually be re.trietedto ~ mm lei. thantheminimum clear eli.tanee between themain bars or S mm lell than the minimum cover to the reinforcement whichever i. Imaller. 5.3.4 Coarse and fine alsrelate Ihall be batched separately. All.in-alar.,lte may be used only where lpecifically permitted by tho enlineer-in-char,e. free from injurious amounts of oils.acids, alkalis, salta, sugar, organic materials or other substances that may be deleterious to concrete or steel. Potable water is generally considered satisfactory for mixina concrete. As a guide the following concentrations represent the maximum pennissible values: a) To neutralize 100 ml sample of water, usir.1 phenolphthalein as an indicator, it should not require more than' ml of 0.02 nonnal NaOH. The details of test are aiven in 8.1 of IS 3025 (Part 22). b) To neutralize 100 ml sample of water, uains mixed indicator, it should not require more than 2' ml of 0.02 nonnal H2SO•. The details of test shall be as given in 8 of IS 3025 (Part 23). c) Permissible limits for solids shall be as liven in Table 1. 5.4.1 In case of doubt regardinl development of strength. the suitability of water for makingconcrete shall be ascertained by the compressive streolth and initial setting timetestsspecified in 5.4.1.1and5.4.1.3. 5.4.1.1 The sample of water taken for teslin, Ihall represent thewaterproposed to beusedfor concreting, due account being paid to seasonal variation. The sample shall not receive any treatment before te_un, otherthanthatenvisaged in theregular supply of water proposed foruseinconcrete. Thesample shallbeltored in a clean container previo~lly rinsed out with limilar water. 5.4.1.2 Averalo 28 days compressive Itten.th of at leastthree l~O nun concrete cubesprepared with water proposed to be used shall not be lell than 90 percent of the average of strenlth of three similar concrete cubes prepared with diltilled water, Th. cube••hall be prepared. cured and tested in accordance with the requirements of IS 516. 5.4.1.3 The initial •• ttinl timeof te.t blockmadewith the appropriate cement and the water propolld to be used .hall not be le•• than 30 min and .hall not dlff. by ± 30 min fromthe initial .etlina time of control telt block prepared with the lame cement ,and diltiJled water. The telt block. ,han be preparedand tilted In accordance with the requirementa of IS 4031 (P.n 5). 5.4.1 The pH valueof water ,hall be not lell than 6. 5.4.3 Sea Water Mixinl or curin, of concrete with .ea waler il not recommended because 'ofPf"Once of harmful.lltl in ... water. Under unavoidable Circumltaneel 1M water may be used formixin.orcuriolin plainconcrete with noembedded steel after hayiJllliven due conllderation toposlible.disadvantapa and precaution. includin, UII 1.4 Water of appropriate cement system. . Waterused for mixin, and cunn'lhall be clean and 14 IS 456 : 2000 Table 1 Permissible Limit for Solids tCtaus« 5.4) n ii) iii) iv) l'crDli~~ible 'Iesred as per 51 Nil, Limit, Mllx Organic Inorganic Sulphates (as SO) Chlorides (as CIl IS ~02~ (Part IS) IS ~025 (Purt Ill) IS ~02'i (Part 24) IS .1025 (Part ~2) 2001ll!!!1 11M10 mg!1 400 mg/l 2IM)() IIIg!1 for concrete 1101 coutaining embedded steel and ~(JO 1IIg/\ I<Jr reinforced concrete work v) Suspended mailer IS 3025 (Part 17) 2 000 1lIg11 5.6.1 All reinforcement shall he free from loose mill scales. loose rust and coats of paints. oil. mud or any other substances which may destroy or reduce hondo Sand blasting or other treatment is recommended to dean reinforcement. 5.4.4 Water found satisfactory for mixing is also suitable for curing concrete. However, water used for curing should not produce any objectionable stain or unsightly deposit \10 the concrete surface. The presence of tannic add or iron compounds is objectionable, 5.6.2 Special precautions like coating (If reinforcement may be required for reinforced concrete clcmenIs in exceptional cases and for rehabilitation of structures. Specialist literature may he referred to in such cases. 5.5 Admixtures 5.5.1 Admixture. if used shall comply with IS 9103. Previous experience with and data (IIi such materials should he considered in relation to the likely standardsof supervisionand workmanshipto the work being specified. 5.6.3 The modulus of elasticity of steel shall be taken as 200 kN/l1llJ1·~. The characteristic yield strength of different steel shall be assumed as the minimum yield stress/0.2 percent proof stress specified in the relevant Indian Standard. 5.5.2 Admixtures should not impair durability (If concrete nor combine with the constituent to form harmful compounds nor increase the risk of corrosion of reinforcement. 13.7 Storage of'Materials 5.5.3 The workability, compressive strength and the slump loss of concrete with and without the usc of admixtures shall be established during the trial mixes before lise of admixtures Storage of materials shall he as described in IS 40K2. 6 CONCRETE 6.1 Grades 5.5.4 The relative density of liquid admixtures shall he checked for cadi drum containing admixtures and compared with till' specified value before acceptance. The concrete shall be in grades designated as per Tanlc 2 5.5.5 The chloride content of admixtures shall be independently tested fill e ach hutcl) before acceptance. 6.1.1 The characteristic strength is defined as the strength of material below which not more than 5 percent of the test results arc expected to fall. 5.5,6 If two or more admi xture s art' used simultaneously in the same concrete mix. Jala should be obtained to assess their interaction and to ensure their compatibility, 6.1.2 Tile minimum grade of concrete for plain and reinforced concrete shall be as per Table 5. 6.1.3 Concrete of grades lower than those given in Table 5 may he used for plain concrete constructions. lean concrete, SImple foundations, foundation for masonry walls and other simple or tcmporury reinforced concrete construction. 5.6 Reinforcement TIll' reinforcement shall be any of the following: a) Mild steel and medium tensile steel bars conforming to IS 432 (Part I). 6.2 Properties of Concrete 6.2.1 h) High strength deformed steel bars conforming to IS 1786. IIIClI'(/.I'(, of Strength with Agi' There is normally a gain of strength beyond 2S days. The quantum of increase depends upon the )!radc and type of cement, curing and cnvuoruucnral conditions, etc. The design should 1)(' h:1S,xl on 2x dav-, charactcristic strength "f com.r. " 'lIlkss there is a evidence II I c) Hard-drawn steel wire fabric conforming to IS 1566. d) Structural steel conforming to Grade A of IS 2062. 15 IS 456: 1000 'Dable2 Gndes of Concnte (Clause 6.1.9.2.2.15.1.1 and 36.1) Group Grade DeI.....IIOIl Spedfted Cba 1Ie eo.,...." S til ISO ami Cube at 210.,." Nlmm2 (I) (2) (3) Ordinary Concrete M 10 M IS 10 IS 20 M20 Slalldllrd Concrete M2S M30 M3S 2S 30 M40 40 45 3S M4S MSO MSS Hi,h Strength Concrete SO SS M60 60 65 70 M6S M70 M7S M80 75 80 NOTES I Inthedesipotion of concrete mixM refersto the mixlUld the number to the specified compnlUive Itrenath of 150 mm size cube lit 28 days.expressed in N/mmJ. 1 Forconcrete of com~ssive strenath areaterthan M55.desip parameters givenin the llalldllrd maynot be applicable and the values may be obtained from specialized literatures and experimcntalresults. justifya higherstrength fora particular structure due to age. 6.2.1.1 For concrete of grade M 30 and above. the rate of increase of compressive strength withageshall be basedon actualinvestigations. 6.2.1.2 Where members are subjected to lowerdirect load duringconstruction, they should be checkedfor stresses resulting from combination of directloadand bending duringconstruction. where Ec is the short tenn static modulus of elasticity in N/mm2• Actual measured values may differ by ± 20 percent from the values obtained from the aboveexpression. 6.2.4 Shrinlcage The total shrinkage of concrete depeRds upon the constituents of concrete, size of the member and environmental conditions. For a givenhumidity and temperature, the total shrinkage of concrete is most influenced by the total amount of waterpresentin the concrete at the time of mixing and, to a lesserextent, by the cementcontent. 6.2.4.1 In the absence of test data, the approximate value of the total shrinkage strain for deslan may be takenas 0.000 3 (for moreinfonnation, see IS 1343). 6.2.S Crtepof Concrete Creep of concrete depends, in addition to the factors listed in 6.2.4, on the stress in the concrete. age at loading and the duration of leading. As long as the stress in concrete does not exceed one-third of its characteristic compressive strength, creep may be assumed to be proportional to the stress. 6.1.5.1 Intheabsence ofexperimental data and detailed information on theeffectof thevariables, the ultimate creep strain may be estimated from the following values ofcreep coefficient (that is.ultimate creep strain! elastic strain at the age of loading); for long span structure, it is advisable to determine actual creep strain, likelyto take place: 6.2.2 Tensile Strength of Concrete The flexural and splitting tensile strengths shall be obtained as described in IS 516 and IS 5816 respectively. When the designer wishes to use an estimateof the tensilestrength from the compressive strength, the following formula may be used: Flexural strength, fer Creep Coefficient I year 1.1 2.2 1.6 NOTE-The ultill1lle creep 1UIin. eatimlled as described above does not include the elastic IItI'lIin. 6.2.6 Thermal Expansion The coefficient of thermal expansion depends on IllltUI'e of cement, the aggregate,. the cement content, the relative humidity and the size of sections. The value of coefficient of thermal expansion for concrete with different aggregates may be takenas below: = 0.7..[l; N/mm2 where f", is thecharacteristic cubecompressive strength of concretein N/mm 2• 6.2.3 Elastic Deformation The modulus of elasticity is primarily influenced by the elastic properties of the aggregate and to a lesser extent by the conditions of curing avet age of the concrete, the mix proportions and the type of cement. The modulus of elasticity is normally related to the compressive strengthof concrete. 6.2.3.1 The modulus of elasticity of concrete can be assumed as follows: " Ageat Loading 7 days 28 days Type ofAggregate Quartzite Sandstone Granite Basalt Limestone Coefficient ofThermal .Expansionfor Concrrte/"C 1.2 to 1.3 x 10'5 0.9 to 1.2 x 10" . 0.7 to 0.95 x 10" 0.8 to 0.95 x 10" 0.6lQ,.o.9 x 10'5 ..1 '." 16 IS 456: 2000 7 WORKABILITY OF CONCRETE be compacted with the means available. Suggested ranges of workabihty of concrete measured in accordance with IS J 199 are given below: 7.1 The concrete mix proportions chosen should be such that the concrete is of adequate workability for the placing conditions of the concrete and can properly Placing Conditions (I) Blindingconcrete; Shallow sections; Pavements using pavers Mass concrete: Lightly reinforced sections in slabs, beams, walls,columns: Degree oj· Workllbi lity Slump (2) (3) Very low See 7.J.l Low 25-75 Medium 50-100 (mm) Floors; Hand placed pavements; Canal lining; Strip footings Heavily reinforced sections in slabs. beams, walls. columns; Slipform work; Pumped concrete Trench fill; In-situ piling . Trernie concrete 75-100 Iligh 100-150 Very high See 7.1.2 NOTE-For most of the placing conditions, mtcrnul vibrators (needle vihrators) are suitable. The diameter of the needle shall be determined based on the density and spacing of reinforcement bars and thickness of sections. Fur tremie concrete, vibrators are not required to be used (s,e also l:t~~). a suitably low permeability is achieved by having an adequate cement content sufficiently low free water/ cement ratio, by ensuring complete compaction of the concrete. and by adequatecuring. 7.1.1 In the 'very low' category ofworkability where strict control is necessary, for example pavement quality concrete, measurement of workability hy determination of compacting factor will he more appropriate than slump (see IS 1199) and a value of compacting factor of 0.75 to 0.80 is suggested. The factors influencing durability include: a) the environment; 7.1.2 In the 'very high' category of workability, measurement of workability hy determinationof flow will be appropriate (see IS 9103). h) the cover to embedded steel; c) the type and quality of constituent materials; 8 DURABILITY OF CONCRETE 8.1. General d) the cement content and water/cement ratio of A durable concrete is one that performs satisfactorily in the working environment during its anticipated exposure conditions during service. The materialsand e) workmanship, to obtain full compaction and efficient curing; and the concrete; f) mix proportions specified and used should be such as to maintain its integrity and, if applicable, to protect embedded metal from corrosion. 8.1.1 One of the main characteristics influencing the durability of concrete is its permeability to the ingress of water, oxygen, carbon dioxide. chloride, sulphate and otherpotentially deleterious substances. Impermeability is governed by the constituentsand workmanship used in making theconcrete. With normal-weight aggregates 2116 818/07-4.. the shape and size of the member. The degree of exposure anticipated for the concrete during its service life together with other relevant factors relating to mix composition. workmanship. design and detailing should be considered. The concretemix to provideadequatedurability under these conditions should be. chosen taking account of the accuracy of current testing regimes for control and compliance as described in this standard. 17 IS 456: 2000 8.2 Requirements for DurabUity 8.2.1 Shapeand Size ofMember The shape or design details of exposed structures should be such as to promote good drainage of water and to avoid standing pools and rundown of water. Care should also betaken to minimize any cracks that may collect or transmit water. Adequate curing is essential to avoid the harmful effects of early loss of rnoisture (see 13.5).Member profiles and their intersections with othermembers shall be designed and detailed in a way to ensure easy flow of concrete and proper compaction during concreting. Concrete is more vulnerable to deterioration due to chemical or climatic attack when it is in thin sections, in sections under hydrostatic pressure from one side only, in partially immersed sections and At comers and edges of elements. The life of the structure can be lengthened by providing extra cover to steel, by chamfering the corners or by using circular crosssections or by using surface coatings which prevent or reduce the ingress of water, carbon dioxide or aggressive chemicals, 8.2.2 Exposure Conditions 8.2.2.1 General environment general environment to which the concrete will be exposed during its working life is classified into five levels of severity, that is, mild, moderate, severe, very severe and extreme as described in Table 3. The . Table 3 Environmental Exposure Conditions (Clauses 8.2.2.1 and 35.3.2) SI No. (1) Environment (2) Exposure Conditions (3) i) Mild Concrete surfaces protected against weatheror aggressiveconditions, except ii) Moderate Concrete surfaces sheltered from severe rain or freezingwhilst wet Concrete exposedto condensation al'd min Concrete continuously under water Concrete in contactor bt!ried undernonaggressive soil/ground \Yater Concrete surfaces sheltered from saturated salt air in coastal area Concrete surfaces exposed to severe rain, alternate wettinl and drying or occasionalfreezing whilst wet or severe condensation. Concrete ~letely immersed in seawater Concl1'tc exposed to coosual environment COncrelC surfaces exposed to sea water spray. corrosive fumes orsevere freezin, conditions whilst wet Concrete in contact witb or buried under aaressive lub-loiVaround water Surface of members in tidal zone Memben in direct contact with liquldl solidaggressive chemicals those situated in ccestal area. iii) Severe iv) Very severe v) Extreme 8.2.2.2 Abrasive Specialist literatures may be referred to for durability requirements of concrete surfaces exposed to abrasive action, forexample, in case ofmachinery andmetal t)'fes. 8.2.2.3 Freezing and thawing Where freezing and thawing actions under wet conditions exist. enhanced durability can be obtained by the useof suitable airentraining admixtures. When concrete lower than grade M 50 is used under these conditions, the mean total air content by volume of the fresh concrete at the time of delivery into the construction should be: Nominal Maximum Size Aggregate Entrained Air Percentage (mm) 20 40 S±l 4±t Since air entrainment reduces the strength, suitable adjustments may be made in the mix design for achieving required strength. 8.1.1.4 Exposure to sulphate attack Table 4 givesrecommendations for the type of cement, maximum free water/cement ratio and minimum cement content, which are required at different sulphate concentrations in near-neutral ground water having pH of6 to 9. For the very high sulphate concentrations in Class S conditions, some form of liningsuch as polyethylene or polychloroprene sheet; or surface coating based on asphalt, chlorinated rubber, epoxy; or polyurethane materials should also be used to prevent access by the sulphate solution. 8.2.3 Requirement of Concrete Cover 8.1.3.1 The protection of the steel in concrete against corrosion depends upon an adequate thickness of good quality concrete. 8.2.3.2 The nominal coverto the reinforcement shall be provided as per 26.4. 8.%.4 Concrete Mix Proportions 8.1.4.1 General The free water-cement ratio is an important factor in governing the durability of concrete andshould always be the lowestvalue. Appropriate valuesfor minimum cementcontentand the maximum free weler-cemenl ratio are given in Table S for different exposure conditions. The minimum cement content and maximum water-cement ratio apply to 20 mm nominal maximum size aggresate. For othersizesof aggregate they should be changed 81 given in Table6. 18 IS 456: 2000 8.2.4.2 Maximum cementcontent Cement content not including fly ash and ground granulated blast furnace slag in excess of 450 kglml should not be used unless special consideration has been given in design to the increased risk of cracking due to drying shrinkage in.thin sections, or to early thermal cracking and to the increased risk of damage due to alkali silica reactions. Table 4 Requirements for Concrete Exposed to Sulphate Attack (Clauses 8.2.2.4 and 9.1.2) Concentration of SuJpbates, Expressed u SOJ ClaVi SI No. Type of Cement .... ... 1..- ~oil , Total SOl SOlin 2:1 Water: Dense, ruDy Compacted Concrete. Made wltb 20 mm Nominal Maximum Size Allre.ate. ComplyIDl witb IS 383 In Ground Water # SoilExtract Minimum Cement Content kllm J Percent gil gil (3.) (4) (5) Traces Less than « 1.0 Less than n.3 1.0 to 0.3 to 1.9 1.2 (2) (I) 1) 0.2) (6) (7) , Maximum Face WaterCement Ratio (8) 280 0.5S Ordinary Portland cement or Portlandslag cementor Portland pozzolana cement 330 0.50 Supersulphated cement or sulphateresisting Portlandcement 310 o.so Supersulphated cement or sulphateresisting Portland cement Portland pozzolana cement or Portland slag cement 330 0.50 350 0.45 370 O,4S 4(X) 0.40 Ordinary Portland cement or Portland slag cement or Portlandpozzolana cement ii) 2 iii) 0.2 to 0.5 0.5 to 1.0 iv) 4 10to 2.0 1.91U 3.1 11 [0 S,O 1.110 2.5 2.5 to 50 Supersulphatcd or sulphate resisting Portland cement 5 v) More thin 2.0 More chan Morethan 5.0 5.0 Sulphateresisting,. Portland cement supersulphated c;eanent with protectivecoatings or NOTES 1 2 3 4 5 6 7 Cement content given in this table is Irrespective of grades of cement. Use of supersulphated cement is generally restricted where the prevailingtemperatureis above 40 f'C. Supersutpbated cement gives an acceptable life providedthat the concrete is dense and prepared with a water-cementratio of 0.4 or less, in mineral acids, down to pH 3.~. The cement contents given in col 6 of this table are the minimum recommended. For SO, contents near the upper limit of any class. cement contents above these minimum are advised. For severe conditions. such ~ thin sections under hydrostatic pressureon one side only and sections panty immersed.considerations should be given to a further reduction of water-cement ratio. Portland slag cement conforming to IS 45.5 with slag content more than 50 percentexhibits better sulphate resisting properties. Where chl()ride is encountered along with sulphates in soil or ground water.ordinary Portlandcement with C 1A content from ~ to 8 percent shall be desirable to he used in concrete, insteadof sulphate resistingcement.Alternatively. Portland ~lllg erment conforming to IS 4~~ having more than ~o percentslag Of a blendof ordinaryPortlandcementand slag may beused providedsutlicient information is available on performance of.such blended cements in these conditions. 19 IS 456: 2000 expansionand disruption of concrete. To prevent this, the total water-soluble sulphatecontent of the concrete mix.expressed as SOl' should notexceed 4 percent by mass of the cement in the mix. The sulphate content should be calculated as the total from the various constituents of the mix. The 4 percentlimitdoes not apply to concrete made 8.2.5 Mix Constituents 8.2.5.1 General For concrete to be durable, carefulselectionof the mix and materials is necessary, so that deleterious constituents do not exceed the limits. 8.2.5.1 Chlorides in concrete with supersulphated cement complying withIS 6909. Whenever there is chloride in concrete there is an increased risk of corrosion of embedded metal. The higher the chloridecontent, or if subsequently exposed to warm moist conditions. the greater the risk of corrosion. All constituents may contain chlorides and . concrete may be contaminated by chlorides from the external environment. To minimize the chances of deterioration of concrete from harmful chemical salts, the levels of such harmful salts in concrete coming from concrete materials, that is, cement, aggregates water and admixtures. as well as by diffusion from the environment should be limited. The total amount of chloride content (as Cl) in the concrete at the time of placing shall be as given in Table 7. 8.2.5.4 Alkali-aggregate reaction Some aggregates containing particular varieties of silica may be susceptible to attack by alkalis (N~O and ~O) originating from cement or other sources, producing an expansive reaction which can cause cracking and disruption of concrete. Damage to concrete from this reaction will normally only occur when all the following are present together: a) A high moisture level, within the concrete; b) A cement with high alkali content, or another source of alkali; c) Aggregate containing an alkali reactive constituent. The total acid soluble chloride content should be calculated from the mix proportions and the measured chloridecontents of each of the constituents. Wherever possible, the total chloride content of the concrete should be determined, Where the service records of particular cementl aggregatecombination are wellestablished,and do not include any instances of cracking due to alkaliaggregate reaction, no further precautions should be necessary. When the materials are unfamiliar, precautions should take one or more of the following forms: a) Use of non-reactive aggregate from alternate sources. 8.2.5.3 Sulphates in concrete Sulphates are present in most cements and in some aggregates; excessive amounts of water-soluble sulphatefrom theseor other mix constituentscan cause Table 5 Minimum Cement Content, Maximum Water-Cement Ratio and Minimum Grade of Concrete for DifTerent Exposures with Normal Weight Aggregates of 20 mm Nominal Maximum Size (Clause» 6.1.2, 8.2.4.1 and 9.1.2) SI No. t;xposure Reinforced Concrete Plain Concrete ~ Minimum Cement Content .... Maximum FreeWater· Cement Ratio "Minimum Grade of Concrete ... Minimum Gradeof Concrete (6) (7) (8) 300 O.5~ M20 M25 MJO M3S M40 Content (3) (4) 0.60 (~) i) Mild 220 iii) Moderate Severe 240 0.60 MIS 300 O.SO iii) 2S0 O.SO M20 320 O.4~ iv) Very severe 260 0.45 M20 340 0.45 Extreme ~80 0.40 M2~ 360 0.40 v) ... Maxirnum FreeWaterCement Ratio kgln}l kglm' (2) -- Minimum Cement NC)T&, I Celnentcontent prescribed in this table is irrapeetive of the grDdes of cementand it is inclusive of additions mentioned in 5.2. The additions such DIfly ashor around granulated blastfurnace slag mayhe takeninto ICcount in the concrete composition with respecllO the cementcontentand water-cement ratio if the suitability is established and as lonl as the maximum 81nounts cakcn into ac&.~unt do not exceedthe limil or pozzolona and alae specified in IS 1489 (Part I) and IS 4S~ respectively. 2 Minimum grade·for plainconcrete undermild exposu~ condition it nolspecified. 20 1S4S6:2000 Table 6 Adjustments to Minimum Cement Contents for Allregates Other Than 20 mm Nominal Maximum Size evaporation may cause seriousconcentrations of salts with subsequent deterioration, even where the original .salt content of the soil or water is not high. (Clause 8.2.4.1) SI No. Nominal Maximum Adjustments to Minimum CemeDt Contents In 1able 5 Aarepte Size k&lm:mm (I) (2) (3) i) ii) iii) 10 20 +40 40 -30 NOTE - Guidance feaarding requirements for conaete exposed in 1~4. 10 sulphnte anaek is liven 8.1.6.2 Drainage At sites where alkali concentrations are high or may become very high.the groundwatershould be lowered by drainage so that it will not come into direct contact with the concrete. Additional protection may be obtained by the use of chemically resistant stone facing or a layer of plaster of Paris covered with suitable fabric, such as jute thoroughly impregnated with bituminous material. o Table 7 Limits of Chloride Content or Concrete (Clause 8.2.5.2) SI Type or Use 01Concrete Maximum Total Acid Soluble No. 8.2.7 Compaction; Finishing and Curing Chloride ConteDt Exp~cd Adequate compaction without segregation should be ensured by providing suitable workability and by employing appropriate placing and compacting equipment and procedures. Full compaction is particularly important in the vicinity of construction and movement joints and of embedded water bars and reinforcement. as klhnJor CODcrete (I) i) (2) Concretecontaining metal and (3) 0.4 steam cured at elevated tempe- ii) iii) ratureand pre-stressed concrete Reinforced concrete or plain concrete containingembedded metal Concrete not containing embedded metalor any material requiring protection from chloride 0.6 Good finishing practices are essential for durable concrete. J.O Overworking the surface and the addition of waterl cement to aid in finishing should be avoided; the resulting laitance will have impaired strength and durability and will be particularly vulnerable to freezing and thawing under wet conditions. b) Usc of low alkali ordinary Portland cement having total alkali content not more than 0.6 percent(as Na20 equivalent). Furtheradvantagecan be obtainedby useof fly It is essential to use proper and adequate curing techniques to reduce the permeability of the concrete and enhance its durability by extending the hydration of the cement, particularly in its surface zone ash (Grade I) conforming to IS 3812 or granulated blastfurnace slag conforming to IS 12089 as part replacement of ordinary Portland cement (having total alkali content as Na20 equivalent not more than 0.6 percent), provided fly· ash content is at least 20 percent or slag content is at least 50 percent. isee 13.5). 8.2.8 Concrete in Sea-water Concrete i~ sea-water or exposed directly along the sea-coast shall be at least M 20 Grade in the case of plain concrete and M 30 in case of reinforced concrete. The use of slag or pozzolana cement is advantageous under such conditions. c) Measures to reduce the degree of saturation of the concrete during service such as use of impermeable membranes, d) Limiting the cement content in the concrete mix and thereby limiting total alkali content in the concrete mix. For more guidance specialist literatures may be referred. 8.2.8.1 SPecial attention shall be given to the design of themixto obtainthe densestpossibleconcrete; slag. broken brick. soft limestone, soft sandstone, or other porous or weak aggregatesshall not be used. 8.2.8.2 As far as possible, preferenceshall be givento precast members unreinforced, well-cured and hardened. without sharp corners, and having trowelsmooth finished surfaces free from crazing. cracks or other defects; plasteringshould be avoided. 8.2.8.3 No construction joints shall be allowed within 600 mm below low water-level or within 600 mm of the upper and lower planes of wave action. Where 8.2.6 Concretein Aggressive Soils and Water 8.2.6.1 General The destructive action of aggressive waters on concrete is progressivee The rate of deterioration decreases as the concrete is made stronger and more impermeable, and increasesas the salt contentof the waterincreases. Where structures are only partially immersed or are in contactwithaggressive soilsor waters on onesideonly, 21 IS 456: 1000 a) Type of aggregate, unusually severeconditionsor abrasionare anticipated, suchparts of the workshall be protectedby bituminous or silico-fluoridecoatings or stone facingbeddedwith bitumen. 8.2.8.4 In reinforcedconcrete structures,care shall he taken to protect the reinforcement from exposure to saline atmosphereduring storage, fabricationand use. It may be achieved by treating the surface of reinforcement with cement wash or by suitable methods. 9 CONCRETE MIX PROPORTIONING 9.1 Mix Proportion The mix proportions shall be selected to ensure the workabilityof the freshconcrete and when concrete is hardened, it shall have the requiredstrength,durability and surface finish. 9.1.1 The determinationof the proportionsof cement, aggregates and water to attain the required strengths shall he made as follows: a) By designing the concrete mix; such concrete shall be called 'Design mix concrete', or b) By adopting nominal concrete mix: such concreteshall becalled 'Nominal mixconcrete'. b) Maximum cement content. and c) Whether an admixture shall or shall not be used and the type of admixture and the condition of use. 9.2 Design Mix Concrete 9.2.1 As the guarantor of quality of concrete used in theconstruction, theconstructor shall carry outthemix design and the mix so designed (not the method of design) shall be approved by the employer within the limitations of parameters and other stipulations laid down by this standard. 9.2.2 The mix shall be designed to produce the grade of concrete having the required workability and a characteristic strengthnot less than appropriate values given in Table2. The target mean strength of concrete mix should be equal to the characteristicstrength plus 1.65 times the standard deviation. 9.2.3 Mix design done earlier not prior to one year may be considered adequate for later work provided there is. no change in source and the quality of the materials, 9.2.4 Standard Deviation Design mix concrete is preferred to nominal mix. If design mix concrete cannot be used for any reason on the work for grades of M 20 or lower) nominal mixes may be usedwiththe permission of engineer-in-charge. which, however. is likely to involve a higher cement The standard deviationfor each gradeof concrete shall be calculated, separately. 9.2.4.1 Standard deviation blued on test strength of sample a) Number of test results of sample,s'-The total number of test strength of samples required to constitute an acceptable record far calculation of standard deviation shall be not less than 30. Attempts should be made to obtain the 30 , samples, as early as possible, whena mix is used for the first time. content. 9.1.2 Information Required In specifying a particular grade of concrete, the following informationshall be included: a) Type of mix, that is, design mix concrete Of nominal mix concrete: h) Grade designation; c) Type of cement; d) Maximum nominal size of aggregate; b) In case of significant changes in concrete- When significant changes are made in the production of concrete batches (for example changes in the materials used, mix design, equipment or technical control). the standard deviation value shan be separately calculated for such batches of concrete. e) Minimum cement cont.ent (for design mix concrete); f) g) h) j) k) Maximum water-cement ratio; Workability; Mix proportion (for nominal mix concrete); Exposure conditions as per Tables 4 and 5; Maximum temperature of concrete at the time of placing; c) Standard deviation to be brough: up to date- The calculation of the standard deviation shall be broughtup to date after every change of mix design. 9.2.4.2 Assumed standard deviation Where sufficient test results for a particular grade of concrete are not available. the value of standard deviation given inTable 8 may be assumed for design of mix in the first instance. As soon as the results of samples are available, actual calculated standard deviationshall be used and the mix designed properly. m) Method of placing; and n) Degree of supervision. 9.1.2.1 In appropriate circumstances. the following additional information may be specified: 22 IS 456: 2000 However, when adequate past records for a similar grade existandjustifyto the designer a valueof st,Uldard deviation different from that showninTable 8, it shall bepermissible to use that value. 10 PRODUCTION OF CONCRETE 10.1 Quality Assurance Measures 10.1.1 In order that the properties of the completed structure be consistent with the requirements and the assumptions made during the planning and the design, adequate quality assurance measures shall be taken. The construction should result in satisfactory strength, serviceability and long term durability so as to lower the overall life-cycle cost. Quality assurance in construction activity relates to proper design, usc of adequate materials and components to be supplied by the producers, proper workmanship in the execution of works by the contractor and ultimately proper care during the use of structure including timely maintenance and repair by the owner. Table 8 Assumed Standard Jleviation (Clau~'e 9.2.4.2 and Tub/£' 11) Grade of Concrete StKndard Deviation N/narn z AS5Uftl,d MIO MIS l5 M20 M2S 4.0 MJO MJS M40 M4S M SO 5.0 10.J.2 Quality assurance measures are both technical and organizational. Some common cases should be specified in a general Quality Assurance Plan which shall identify the key elements necessary to provide fitness of the structure and the means by which they are to be provided and measured with the overall purpose to provide confidence that the realized project will work satisfactorily in service fulfilling intended needs. Thejob of quality control and quality assurance would involve quality audit of both the inputs as well as the outputs. Inputs are in the form of materials for concrete: workmanship in all stages of hatching. mixing, transportation, placing, compaction and curing: and the related plant, machinery and equipments: resulting in the output in the form of concrete in place. To ensure proper performance, it is necessary that each step in concreting which wi11 be NOTE--The above values correspond to the site control having properstorageof cement;weighhatchingof all material»; controlled addition of water; regular checking of all ,nate.-juls. ag~rcgate &J'adings and moisture content; and periodical checking of work3hility and strength. W~rc there i~ deviation from th~ above the values given in the abnve tnble shall he inc.:fea~cd hy I N/nun! . 9.3 Nominal Mix Concrete Nominal mix concrete may be used for concrete of M 20 or lower. The proportions of ruutcnals for nominal mix concrete shall be in accordance with 1:1ble 9. 9.3.1 The cement 'content of the mix specified in Table 9 for any nominal mix shall be proportionately increased if the quantity of water in a nux has to he increasedto overcor..e the difficultiesof placementand compaction, so that the water-cement ratio as specified is not exceeded. covered by the next step is inspected as the work proceeds (see also 17). Table «) Proportions for Nominal Mix Concrete (Clausrs 9.3 lind Grade of Concrete 9.~.l) Total Quantity of Dry Aggre- Preportion of Fine gates by i\lass per SO kg of Cement, to be Taken as the SUID of the Individual M1I$..'ies of Ftnt aod Coarse Al:gregH1es, kg, A~gregate to ~oarse Quantity of Wat~r per SO kg of Cement, Max Axgre"ate (hyl\1a'tt) I MtlX (I) (2) M5 ROO M7.~ 625 M 10 480 M 15 330 32 M20 2~O 30 (4) Generally 1:2 but subject to an upper limit of I: 11 and a lowerlimit of 1:21/1. '1 60 45 34 NOTE-11le proportion of the fineto coarse aggregates should be adjustedfromupperlimit 10 lowerlimit progressively as the ~rading of fine agl~gates becomes finer and the maximum size of coarse a~gregate becomes larger, Graded coarse aggregate shall be used. Examplt For M Avera,,, ,radina of fine aggregate (that is. Zone II of Table 4 of IS ~83). the proportions shall be L 1'1" 1:1 and l:2'/:! for maximum sizeof ngg~gntes 10 mm, 20 mm and40 mm respectively, 23 IS 456: 2000 10.1.3 Each party involved in the realization of a project should establish and implement a Quality Assurance Plan. for its participation in the project. Supplier's and subcontractor's activities shall be covered in the plan. The individual QualityAssurance Plans shall tit into the general QualityAssurancePlan. A Quality Assurance Plan shall define the tasks and responsibilities of all persons involved. adequate control and checking procedures,and the organization and maintaining adequate documentation of the building process and its results. Such documentation should generally include: a) test reports and manufacturer's certificate for materials. concrete mix design details; b) pour cards for site organization and clearance for concrete placement; c) record of site inspectionof workmanship, field tests; d) non-conformance reports. change orders; e) quality control charts; and 1) statistical analysis. NOTE-Quahty controt charts are recommended whereverthe concrete is in continuousproductionover considerable period. 10.2 Batching Toavoidconfusionand error in batching,consideration should be given to using the smallest practicalnumber of different concrete mixes on any site or in anyone plant. In hatching concrete.thequantityof bothcement and aggregateshall be determinedby mass;admixture. if solid. by mass; liquid admixture may however be measured in volume or mass; water shall be weighed OJ' measured by volume in a calibrated tank (set' also IS 4925). Ready-mixed concrete supplied by ready-mixed concreteplantshall be preferred. Forlargeand medium project sites the concrete shall be sourced from readymixed concrete plants or from on site or off site hatching and mixing plants (see IS 4926). 10.2.1 Except where itcan he shown to the satisfaction of the engineer-in-charge that supply of properly gradedaggregateof uniformqualitycan be maintained over a period of work. the grading of aggregateshould be controlled by obtaining the coarse aggregate in different sizes and blending them in the right proportions when required. the different sizes being stocked in separate stock-piles. The material should be stock-piledfor severalhours preferablya day before use. The grading of coarse and fine aggregate should be checked as frequently a.s possible. the frequency for a given job being determined by the engineer-incharge to ensure that the specified grading is maintained. 10.2.2 The accuracy of the measuringequipmentshall be within ± 2 percent of the quantity of cement being mea.sured and within ± 3 pereent of the quantity of aggregate. admixturesand water being measured. 10.2.3 ProportionflYpe andgradingof aggregates shall be made by trial in such a way so as to obtain densest possible concrete. All ingredients of the concrete should be used by mass only. 10.2.4 Volume batching may be allowed only where weigh-batching is not practical and provided accurate bulk densities of materials to be actually used in concrete haveearlier been established. Allowancefor bulking shall be made in accordance with IS 2386 (Part 3). The mass volume relationship should be checked a.s frequently as necessary. the frequency for the givenjob being determined by engineer-in-charge 10 ensure that the specified grading is maintained, 10.2.S It is important to maintain the water-cement ratioconstant at its correct value.To this end. determination of moisture contents in both fine and coarse aggregatesshall bemade as frequentlyas possible. the frequency for a given job being determined by the engineer-in-charge according to weather conditions. The amount of the added water shall be adjusted to compensate for any observed variations in the moisture contents. For the determination of moisture content in the aggregates.IS 2386 (Part 3) may be referred to. To allow for the variation in mass of aggregate due to variation in theirmoisture content,suitableadjustments in the massesof aggregatesshall also be made. In the absence of exact data. only in the case of nominal mixes. the amount of surface water may be estimated from the values given in Table 10. . 24 Table 10 Surface Water Carried by Aggregate (Clause 10.2.5) Approximate Quantity of Surface Water .. (3) (4) 120 Modernlel)' wet sand 7.5 5.0 iii) Moistsand 2.5 40 IV) "Moist gravelor crushed rock 1.25-2,5 (I) (2) i) Very wet sand ii) II 80 20-40 Courserthe oggregllte. less the wllterit will corry. 10.2.6 No substitutionsin materials used on the work or alterations in the established proportions.except as permitted in 10.2.4 and 10.2.S shall be made without additional tests to show that the quality and strength of concrete are satisfactory. 10.3 Mixing Concrete shan be mixed in a mechanical mixer. The mixer should comply with IS 179" and IS 12119. The mixersshall befitted with watermeasuring(metering) devices. The mixingshall be continueduntil there is a uniform distribution of the materials and the mass is 18456: 1000 ubifortn in colour and consistenc.y. If there is .e,re,ation alter unloading from the mixer, the COhcrete should be remixed. 10.3.1 Por guidance, the mixing timeshall be at least 2 min. Por other types of more efficient mixers, manufacturers recommendations shalJ be followed; for hydrophobic cement it may be decided by the engineer-in-charge. 10.3.2 Workability should be checked at frequent intervals (Itt IS 1199). 10.3.3 Dosages of retarders, plasticisers and superplasticisers shall be restricted to O.S, 1.0and2.0 percent respectively by weight of cementitious materials and unless a higher value is agreed upon between the! Itllftufacturer and the constructor based on performance test. 11.3 Strlpplnl11me Fonns shall not be released until the concrete has achieved a strength of at leasttwice the stressto which the concrete may be subjected at the time of removal of fonnwork. The strength referred to shall be that of concrete using the same cement and aggregates and admixture, if any, withthesameproportions andcured under conditions of temperature and moisture similar to those existing on the work. 11.3.1 Whilethe above criteriaof strength shall be the guiding factor for removal of formwork, in normal circumstances where ambient temperature doesnotfall below ISOC and where ordinaryPortland cement is used andadequate curingis done,following striWng period maydeemto satisfy the guideline given in 11.3: Type of Formwor/c 11 FORMWORK 11.1 General The formwork shall be designed and constructed so as to remain sufficiently rigid during placing and compaction of concrete, andshall be suchas to prevent loss of slurry from the concrete. For further details regarding design, detailing, etc,reference may be made to IS 14687. The tolerances on the shapes, lines and dimensions shown in the drawing shall be within the limitsgiven below: a) Deviation from specified + 12 dimensions of cross-section _ 6 mm of columns aad beams b) Deviation from dimensions offootinss 1) Dimensio. in plan +50 mm a) b) c) d) e) -12 2) Eccentricity 3) Thickness 0.02 times the widthofthefooting in the direction of deviation butnotmore than SOmm ± o.os times the specified thickness Thesetolerances applyto concrete dimensions only, and notto positioniolof vertical reinforcing steel ordowels. 11.2 aeanm._ TnatmeDt 01Formwork All rubbish, particularly, chippinss, shavings and sawduat sball beremoved from the interior ofthefonns before the concrete is placed. The face of formwork incontactwith the concrete shallbe cleaned andtreated with form release agent. Release agents should be applied soas to providea thin unifonn coating to the fonns withoutcoatingthe reinforcement. 2118 818/07-5 Minimum Period Before Striking Formwork Vertical fonnwork to columns, 16-24 h walls, beams Soffitformwork to slabs 3 days (Props to be refixed immediately afterremoval of formwork) 7 days Soffit fonnwork to beams (Props to be refixed immediately afterremoval of formwork) Props to slabs: 7 days 1) Spanning up to 4.5 m 14days 2) Spanning over4.S m Props to beams and arches: 14 days 1) Spanning up to 6 m 21 days 2) Spanning over 6 m For other cements and lower temperature, the stripping time recommended above may be suitably modified. 11.3.2 The'number of propsleft under, theirsizesand disposition shall be such as to be able to safely carry the full dead load of the slab, beam or arch as the case may be tOlether with any live load likely to occur during curingor further construction. 11.3.3 Where theshapeof theelementis suchthat the formwork has re-entrant angles, theformwork shall be removed as soonas possible afterthe concretehas set, to avoid shrinkage cracking occurring due to the restraint imposed. 11 ASSEMBLY OF REINFORCEMENT 12.1 Reinforcement shall be bent and fixed in accordance with procedure specified in IS 2502. The highstrength defonnedsteelbarsshould notbere-bent 2S IS 456: 2000 or straightcned without the approval of engineer-incharge. Bar bending schedules shall be prepared for all reinforcement work. J2.2 All reinforcement shall be placed and maintained in the position shown in the drawings by providing proper cover blocks, spacers, supporting bars, etc. 12.2.1 Crossing bars should not be lack-welded for assembly of reinforcement unless permitted by engineer-in-charge. 12.~~ Placing of Relnforcement Rough handling, shock loading (prior to embedment) and the droppingof reinforcementfroma heightshould be avoided. Reinforcement should he secured against displacement outside the specified limits. 12.3.1 Tolerances on Placing (~f Reinforcement Unless otherwise specified by engineer-in-charge, the reinforcement shall he placed within the following tolerances: a) for effective depth 200 nun or less ± 10 nun b) for effective depth more than 200 mm ± 15 mm t2.3~2 Tolerancefor Cover Unless specified otherwise, actual concrete cover should not deviate from the required nominal cover by +10 0 mrn, Nominal cover as given in 26.4.1 should be specified to all steel reinforcement including links. Spacers between the links (or the bars where no links exist) and the formwork should be of the same nominal size as the nominal cover. Spacers, chairs and other supports detailed on drawings, together with such other supports as may he necessary, should be used to maintain the specitied nominal cover to the steel reinforcement. Spacers or chairs should be placed at a maximum spacing of I m and closer spacing may sometimes be necessary. steel bars are bent. aside at construction joints ana afterwards bent back into their original positions. care should be taken to ensure that at no time is the radius of the bend Jess than 4 bar diameters for plain mild steel or 6 bar diameters for deformed bars, Care shall also be taken when bending hack bars, to ensure that the concrete around the bar is not damaged beyond the band. 12.6 Reinforcement should be placed and tied in such a way that concrete placement be possible without segregation of the mix. Reinforcement placingshould allow compaction by immersion vibrator. Within the concrete mass, different types of metal in cont.act should be avoided to ensure that bimetal corrosiondoes not t.ake place, 13 TRANSPORTING, PLACING, COMPACTI'()N AND CURING 1.3.1 Transporting and Handling After mixing, concrete shall be transported to the formwork as rapidly as possibleby methods which will prevent the segregation Of Jossof any of the ingredients or ingress of foreign matter or water and maintaining (he required workability 13.1.1 During hoi Of cold weather. concrete shall be transportedin deep containers. Other suitable methods to reduce the loss of water hy evaporation in hot weather and heat loss in cold weather may also be adopted. 13.2 Placing TIle concrete shall he deposited as nearly as practicable in its final position to avoid rehandling. The concrete shall he placed and compacted hefore initial setting of concrete commences and should not be subsequently disturbed. Methods of placing should be such as to preclude scgreg.rtion. Care should be taken to avoid displacement of reinforcement or movement of Iorrnwork . As a general guidance, the maxi . . mum permissible free fall of concrete may be taken as 1.5 Ill. 13.3 COInpaction Concrete should he thoroughly compacted and fully worked around the reinforcement, around embedded Spacers, cover blocks should he of concrete of same strength or PVC. fixtures and into corners of the fonnwork. 1.2.4 Welded Joints or Mechanical Connections 13.3.1 Concrete shall be compacted using mechanical vibrators complying with IS 2505, IS 2506. IS 2514 and IS 4656. Over vibration and under vibration of concreteare harmful and should beavoided. Vibration of very wet mixes should also he avoided. Welded joints or mechanical connections in reinforcement may be usedbut in allcasesof important connections, tests shall he made to prove that thejoints are of the full strength of bars connected. Welding of reinforcements shall be done in accordance with the recommendations of IS 2751 and IS 94 J7. 12.5 Where reinforcement bars upto 12 mm for high strength deformed steel bars and up to 16mm for mild Whenever vibration has to be applied externally, the design of formwork and the disposition of vibrators should receive specialconsideration to ensure efficient compaction and to avoid surface blemishes. 26 IS 456: 2000 13.4 ConstMlttion Joints and Cold Joints of ordinary Portland Cementand at least 10 days where Joints are a common source of weaknessand, therefore, it is desirable to avoid them. If this is not possible. their number shall be minimized. Concreting shall be carried out continuously up to construction joints, the position and arrangement of which shall be indicated by the designer. Construction joints should compJywithlS 11817. Construction joints shall be placed at accessible locations to permit cleaning out of laitance, cement slurry and unsound concrete, in order to create rough/ unevensurface. It is recommendedto clean out laitance and cement slurry hy using wire brush on the surface of joint immediately after initial setting of concrete and to clean out the same immediately thereafter. The prepared surface should be in a clean saturated surface dry condition when fresh concrete is placed. against it. mineral admixturesor blendedcements are used. The period of curing shall not be less than J0 days for In the case of construction joints at locations where the previous pour has been cast against shuttering the recommended method of obtaininga rough surface for the previously poured concrete is to expose the aggregate with ,1 high pressure water Jet or any other appropriate means. Fresh concrete should be thoroughly vibrated near construction joints so that mortarfrom the new concrete flows between large aggregates and develop proper bond with old concrete. Where high shear resistance IS required at the construct ion joints. shear keys "lay he provided. Sprayed curing membranes and release agents should be thoroughly removed from joint surfaces. 13.5 (:urin~ concrete exposed to dry and hot weather conditions. In the case of concrete where mineral admixtures or blended cements are used, it is recommended that above minimum periods may be extended to 14 days. 13.5.2 Membrane (.'. uring Approved curing compounds may be used in lieu of moist curing with the permission of the engineer..incharge. Such compounds shall beappliedtoall exposed surfaces of the concrete as soon as possible after the concrete has set. Impermeable membranes such as polyethylene sheeting covering closely the concrete surface may also be used to provide effective barrier against evaporation. 13.5.3 For the concrete containing Portland pozzolana cement, Portland slag cement or mineral admixture, period of curing may be increased. 13.6 Supervision It is exceedingly difficult and costly to alter concrete once placed. Hence, constant and strict supervision of all the items of the construction is necessary during the progress of the work, including the proportioning and mixing of the concrete. Supervision is also of extreme importance to check the reinforcement and its placing before being covered. 13.6.1 Before any important operation. such as concreting or stripping of the fonnwork is started, adequate notice shall be gi yen to the construction supervisor. Curing is the process of preventing the Joss of moisture 14 CONCRETING UNDER SPECIAL from the concrete whilst maintaining a satisfactory . (~ONDITIONS temperature regime. The prevention of moisture loss from the concrete is panicularly important if the water- 14.1 Work in Extreme Weather Conditions cement ratio IS low, if the cement has a high rate of During hot or cold weather, the concreting should be strength development, if the concrete contains done as per the procedure set out in IS 7861 granulated blast furnace slag or pulverised fuel ash. (Part 1) or IS 7861 (Part 2). TIlecuringregime should also prevent the. development 14.2 Under-Water Con~retinl of high temperature gradients within the concrete. The rate of strength development at early ages of 14.ZL 1 When it is necessary to deposit concrete under concrete made with supersulphated cement is significantly reduced at" lower temperatures. Supersulphated cement concrete is seriously affected by inadequate curing and the surface has to be kept moist for at least seven days. water, the methods. equipment, materials and proportions of the mix to be used shall be submitted to and approved by the engineer-in-charge before the work is started. 13.5.1 Moist Curing Exposed surfaces of concrete shall be kept continuously in a damp Of wet condition by pending or by covering with a layer of sacking, canvas, hessian or similar materials and kept constantly wet for at least seven days from the date of placing concrete in case 14.2.2 Under-water concrete should have a slump recommended in 7.1. The water-cement ratio shall not exceed 0 6 and may need to be smaller, depending on the grade of concrete or the type of chemical attack. For aggregates of 40 rom maximum particle size, the cement content shall be at least 350 kg/m' of concrete. 14.1.3 Coffer-dams or forms shall be sufficiently tight 27 IS 456: 2000 to ensure still water if practicable. and in any cue to reducethe flowof waterto less than 3 m1min throup the space into which concrete is to be deposited. Coffer-dams or fonns instillwatershallbesufficiently tight to prevent loss of mortar through the walls. De-watering by pumping shall not be done while concreteis being placedor until 24 h thereafter. 14.2.4 Concrete cast underwatershouldnotfallfreely through the water. Otherwise it may be leached and become segregated. Concrete shall be deposited continuously until it is broughtto the required height. While depositing. the top surface shallbe kept asnearly level as possibleand the fonnation of seams avoided. The methods to be used fordepositing concrete under water shall be one of the following: a) Tremie-Theconcrete isplacedthroup vertical pipes the lowerend of whichis always inserted sufficiently deep into the concrete which has been placed previously but has not set. The concrete emerging from the pipe pushes the material that has already beenplacedto theside and upwards and thusdoes not come intodirect contact with water. When concrete is to be deposited under water by means oftremie, the top sectionof the tremie shall be a hopperlarge enoughto holdoneentire batch of the mix or the entire contents the transporting bucket, if any. Thetremie pipeshall be not less than 200 mm in diameterand shall be largeenoughto allowa freeflowof concrete and strong enough to withstand the external pressureof the water in which it is suspended, evenif a panial vacuum develops inside the pipe. Preferably, flanged steel pipe of adequate strength for the job should be used. A separate lifting device shall be provided for each tremie pipe with its hopper at the upper end. Unless the lower end of the pipe is equipped with an approved automatic check valve, the upperend of pipe shall be plugged with a wadding of the gunny sackingor other approved material beforedelivering the concreteto the tromie pipe throughthe hopper, so that whenthe concrete is forceddownfromthe hopperto the pipe, it will force the plug (and along with it any water in the pipe) down the pipe and out of the bottom end. thus establishing a continuous stream of concrete. It will be necessary to raiseslowly the tremie in order to cause a uniform flow of the concrete, but the tremieshall not beemptied10 that water entersthe pipe. At all timesafter the placing of concrete is started and until all the concrete is placed, the lowerend of the ttemie pipeshall be below the topsurface of the plastic concrete. This.will cause the concrete to build up from below insteadof flowing out over the the 28 .urface, and thus avoid formetion of laitance layors. If tho cluqo in tho tremie is 10lt while depositin,. tho tromio shall bo naised Ilxlve d1e concrete surface, and unloss _04 by I c~k valvo, it shall be rc-plulled at tho topend, as•• the beginninl. before refl11inl for dcpositin, concrete. b) Direct plactment with pumps-As in the case of the tremie method, tho vertical end pieceof the pipe lineisalways inserted sufficiently deep into the previoosly castconcreteand shouldnot move to tlte side during pumping. c) Dmpbouom bucket -The topof thebucketshall bo covered with acanvas flap. The bottom doors shall open freely downwvd and outward when tripped. Thebucket shall bo (diedcompletely and lowered slowly to avoid backwaah. The bottom doors shall not be opened until tho bucketrests on the surface upon which the concreto is to be deposited and when dtscharged, shall be withdrawn slowly until well above the concrete, d) Bags - Bags of at least 0.028 m] capacity of jute or other coarse cloth shall be filled about two-thirds fullof concrete, the spareend turned underso that baa is square ended and securely tied. They shall be placed carefully in header and stretcher courses so that the whole mass is interlocked. Bagsusedfor thispurpose shall be free from deleterious materials. e) Grouting-A series of round cages made from SO mm mesh of 6 mm steel and extending over the full heisht to be concreted shall be prepared andlaid vortically over thearea to be concreted so that tho distance between centres of thecases and also to the faces of the concrete shall not exceedone metre. Stone aggregate of not less than SO mmnormorethan200mm size shall be deposited outside the stool cages over the full areaandheightto be concreted with due care to preventdisplacement of the cages. A stable 1:2 cement-sand grout with a watercementratio of not loss than 0.6 and not marc than 0.8shall be prepared ina mechanical mixer andsentdownunderpressure (about0.2N/inm2) throulh 38 to 50nundiameter pipes tenninating intosteelcages,about SO mmabovethe bottom of the concrete. As the &rautio, proceeds, the pipe shall be raised aradually up to a heiaht of notmorethan6000 nun above its starlin, level after which it may be withdrawn and pl,acod into the noxt cale for further groutiol by the same procedure. After IfOUtinl the whole area for a heisht of about 600 mm, the same operation shall be repeated, if necessary. for the next layer of L~ 600 mm and so on. The amount of grout to be sent down shall be sufficient to fillallthevoidswhich may be either asc~rtained or assumed as 55 percent of the volume to be concreted. 14.2.5 To minimizethe formulation of laitance, great care shall be exercised not to disturb the concrete as far as possible while it is being deposited. 15 SAMPLING AND STRENGTH OF DESIGNED CONCRETE MIX 15.1 General Samples from fresh concrete shall be taken as per IS 1199and cubes shall be made, cured and tested at 28 days in accordancewith IS S16. 15.1.1 In order to get a relatively quicker idea of the quality of concrete, optional tests on beams for modulus of rupture at 72 ± 2 h or at 7 days, or compressive strength tests at 7 days may be carried out in addition to 28 days compressive strength test. For this purpose the valuesshould be arrived at based on actualtesting. In all cases,the 28 dayscompressive strengthspecifiedinTable2 shallalone be thecriterion for acceptanceor rejection of the concrete. 456: 1000 for testing at 28 days. Additional samples may be required for variouspurposessuch as to determine the strengthof concreteat 7 days or at the time of striking the formwork, or to determine the duration of curing. or to check the testing error. Additional samples may also be required for testing samples cured by accelerated methods as described in IS 9103. The specimen shall be tested as described in IS S16. 15.4 Test Results of Sample The test results of the sample shall be the average of the strength of three specimens. The individual variation should not be more than ±lS percent of the average. If more, the test result.~ of the sample are invalid. 16 ACCEPTANCE CRITERIA 16.1 Compressive Streoath The concrete shall be deemed to comply with the strength requirements when both the following condition are met: a) The mean strength determined from any group of four consecutive test results compiles with the appropriate limits in col 2 of Table 11. b) Any individual test result complies with the appropriate limits in col 3 of Table I). 15.1 Frequency of Sampling 16.2 Flexural Strength 15.2.1 Sampling Procedure A random sampling procedure shall be adopted to ensurethateach concretebatchshallhavea reasonable chance of being tested that is, the sampling should be spread over the entire period of concreting and cover all mixing units. . When both the following conditions are met" the concrete complies with the specified flexural strength. a) The mean strengthdetermined from any group of four consecutive test results exceeds the specified characteristic strength by at least 0.3 N/mn12• 15.2.2 Frequency b) The strengthdetermined from any test result is not less than thespecified characteristicstrength The minimum frequency of sampling of concrete of each grade shall be iD accordance with the following: Quantity of Concrete in the Number ofSamples Work, m' I· 5 6 - IS 16 - 30 31 - 50 51 and above 1 2 3 4 4 plus one additional sample for each additional 50 m' or part thereof NOm-At leost one sample shall be taken from each shift. Whereconcrete is produced at continuous production unit, such as ready-mixed concrete plant,frequency of'sampling lnay be agreeduponmutually by suppliers and purchasers. 15.3 Test Specimen Three test specimens shall be made for each sample less 0.3 N/mm1• 16.3 Quantity of Concrete Represented by Strength Teat Results The quantity of concrete represented by a group of four consecutive test results shall include the batches from which .the first and last samples were taken together with all intervening batches. For the individual test result requirements given in col 2 of Table II or in item (b) of 16.2, only the particular batchfromwhichthe samplewastakenshall be at risk. Where the mean rate of sampling is not specified the maximum quantity of concrete that four consecutive test results represent shall be limited to 60 m'. 16.4 If the concreteis deemednot to complypersuant to 16.3. the structural adequacy of the parts affected shall be investigated (see 17) and any consequential action as needed shall be taken. 29 IS 456: 2000 16.5 Concrete of each grade shall be assessed separately. 16.6 Concrete is liable to be rejected if it is porous or honey-combed. its placing has been interrupted without providing a proper construction joint. the reinforcement has been displaced beyond the tolerances specified. or construction tolerances have not been met. However. the hardened concrete may be accepted after carrying out suitable remedial measures to the satisfactionof the engineerin-charge. e) there is a system to verify that the quality is satisfactory in individual parts of the structure, especiallythe critical ones. 17.2 Immediately after stripping the forrnwork, all concreteshallbecarefully inspectedandanydefective work or small defects either removed or made good before concrete has thoroughly hardened. 17.3 Testing 17 INSPECTION AND TESTING OF STRU<"'""TURES In case of doubt regardingthe grade of concrete used, either due to poor workmanship or basedon results of cube strength tests, compressive strength tests of concreteon the basisof 17.4 and/orloadtest (see 17.6) may be carried out. 17.1 Inspection 17.4 Core Test To ensure that the construction complies with the design an inspection procedure should be set up covering materials, records. workmanship and construction. 17.1.1 Tests should be made on reinforcement and theconstituent materials ofconcretein accordance with the relevant standards. Where applicable, use should be made of suitable quality assuranceschemes. 17.4.1 The points from which cores are to be taken and the number of cores required shall be at the discretion of the engineer-in-charge and shall be representative of the whole of concrete concerned. In no case. however. shall fewer than three cores be tested. 17.4.2 Cores shallbe preparedand tested asdescribed in IS 516. 17.1.2 Care should be taken to see that: 17.4.3 Concrete in the member represented by a core test shall be considered acceptable if the average equivalent cube strengthof the cores isequal to at least 85percentof thecubestrengthof the gradeof concrete specifiedfor the correspondingage and no individual core has a strengthless than 7S percent. a) design and detail are capable of beingexecuted to a suitable standard, with due allowance for dimensional tolerances; b) there are clear instructions on inspection standards; c) there are clear instructions on permissible deviations; d) clements critical to workmanship, structural performance. durability and appearance are identified; and 17.5 In case the core test results do not satisfy the requirement.s of 17.4.3 or where such tests have not been done, load test (17.6) may be resorted to. 17.6 Load Tests for Flexural Member 17.6.1 Load tests should be carried out as soon as Table 11 Characteristic Compressive Strength Compliance Requirement (Claus~s Sp«lfted (;rade II) M I~ 16.1 and 16.3) Mean of the Group of 4 Non-Onrlapplnl Individual Test Results In N1mmJ Consecutive nsf Results In NfmmJ (2) (3) 4! 1... + 0.825 x established standarddeviation (rounded off to neaJal 0.5 Nlmm1) or f.. +3NlmmJ. whicheveris greater M 20 or above ~ .f.., + 0.82S )( established ~ f",~ N/mm1 standarddeviation (rounded off to nealat O.~ N/mmJ ) or L.. + 4 N/..mr. whichever is~ter NOTE-In the absence of established valueof standard deviation. the valuesJiven in Table8 l114y be assumed.and llttempt shouldbe l1llIde 10 obtain resultsof 30 samples lIS early lIS poasible to ambUsh die valueof standarddeviation. 30 IS 45(i : 200() possible after expiry of 28 days from the lillie of placing of concrete. not apply. 17.7 Members (1thcr Than Flexural Members 17.6.2 The structure should he subjected to a load equal to full dead load of the structure plus 1.25 tillll'S the imposed load tor a period of 24 h and then the unposed load shall he removed, Memher-, other than flexural members should he preferably investigated hy analysis. NOTE--·-Dc:ad load includes self weight of the structural members pili" weight of finishes and walls or partition». If any ~l'\ considered in the design . Non-destructive tests arc used to obtain estimation of the properties of concrete in the structure. TIle methods 17.H Non-destructive Tests adopted include ultrasonic pulse velocity (sec IS J 33) I (Pari I) J and rebound hammer [IS 13311 (Pari 2) L pr n be pc net rat i()n, pull 0 utand mat lJ r i t y. Nondcstructi vc tests provide alternatives to core tests for cstirnatiug the strength of concrete in a structure. or 17.6.3 The deflection due to iTJIPOSl~d load only shall he recorded. If within 24 h of removal of the imposed load. the structure docs not recover at least 75 percent of the deflection under superimposed load, the test may be repealed after a lapse of 72 h. If the rl~CO\'CI"y is Ics~ than XO percent . the structure shall be dc.eln~d 1o he unacceptable. .7.()...l l Ir the maximum deflection in during. 24 h under load i~ less than 111111. 4()/'~/1.). can xupplcmcut the data obtained 1'1"0111 a limited n UIII her of cores. These methods art' based on mcusur ing a concrete properly thaI bears sonic rl~latic .nship to strength, The accuracy of these methods, in part. is determined by the degree of correlation h('l\\.'t'l'tl ~fn.. nc~th Hnd Ihe physical quality 1I1CtlSUrl,d h) th~' nun destruct i vc texts. shown where I is the effective span in m; and 1.), the overall depth of tlk' ~cclj()n in 111111, it i\ not ncccxs.n y fOI the teL·O\CI V 10 he measured and the recovery provi ,ion", of t 7.tl.~' ...,-hall Anv of th\..~"i~ mcthodx tna~' he .uloptcd. in which cusc the cnll'ria ~h~lll he agreed upon prior to h'sling . ~H'n. 'I'I~IIH.'l" 11 IS 456: 1000 SECTION 3 GENERAL DESIGN CONSIDERATION be taken from Table 18 for the limit state of collapse. 18 BASES FOR DESIGN 18.1 Aim of DesigD The aim of design is the achievementof an acceptable probabilitythat structuresbeingdesignedwillperform satisfactorily during their intended life. With an appropriate degree of safety, they should sustain all the loads and deformationsof normal construction and use and have adequate durability and adequate resistance to the effects of misuse and fire. 18.2 Methods of Design 18.2.1Structureand structuralelementsshall nonnally be designed by Limit State Method. Account should be taken of accepted theories, experiment and experience and the need to design for durability. Calculations alonedo not producesafe,serviceable and durable structures. Suitablematerials,qualitycontrol. adequate detailing and good supervision are equally important. 18.2.2 Where the Limit State Method can not be conveniently adopted, Working Stress Method (see Annex B) may be used. 18.3 DurabWty, Workmanship aDd ~terlall It is assumed that the quality of concrete, steel and other materials and of the workmanship, as verified by inspections, is adequate fot safety. serviceability and durability. 18.4 DesllDProcess Design. including design for durability, construction and use in service should be considered as a whole. The realization of design objectives requires compliance with clearly defined standards for materials, production, workmanship and also maintenance and use of structure in service. 19 LOADSAND'ORCES 19.1 General In structural design, account shallbe taken of the dead. imposed and wind loads and forces such as those caused by earthquake. and effects due to shrinkage, creep, temperature, etc, where applicable. 18.2.3Design Basedon Experimental Basis Designs based on experimental investigations on models or full size structure or element may be accepted if they satisfy the primary requirements of 18.1 and subject to experimental details and the analysis connected therewith being approved by the engineer-in-charge. 18.2.3.1 Where .the design is based on experimental investigation on full sizestructureor element,loadtests shall be carried out to ensure the following: a) The structure shall satisfy the requirements for deflection (see 23.2) and cracking (see 35.3.2) when subjected to a load for 24 h equal to the characteristic load multiplied by ) .33 Yr' where "(rshall be taken fromTable 18,for thelimitstate of serviceability. If within 24 h of the removal of the load, the structure does not show a recovery of at least 7S percent of the maximum deflection shown during the24h under. the load, the test loading should be repeated after a lapse of 72 h.The recovery afterthe secondtestshould beat least 7S percentof the maximumdeflection shown during the second test. 19.2 Dead Loads Dead loads shall be calculated on the basis of unit weights which shall be established takina into considerationthe materialsspecifiedfor construction. 19.2.1Alternatively, the dead loads may becalculated on the basis of unit weights of materials liven in IS 875 (Part 1). Unless more accurate calculations are warranted, the unit weights of plain concrete and reinforced concrete made with sand and gravel or crushed natural stone aggregate may be taken as 24 kN/m:\ and 25 kN/m3 respectively. 19.3 Imposed Loads, WIndLoadsandSnow LoIds Imposed loads. wind loads and snow loads shall be assumed in accordance with IS 87S (Part 2), IS 87S (Part 3) and IS 875 (Part 4) respectively. 19.4 Earthquake Forces The earthquake forces shall be calculated accordance with IS 1893. In 19.5 Shrlnkap, enep and Temperature Elfeets If the effects of shrinkagc, creep and temperature are liableto affectmaterially the safety andserviceability of the structure. these shall be taken into account in the calculations (see 6.2.4, 6.Z.5 and 6.2.6) and IS 875(Part 5). 19.5.1 In ordinarybuildinp, such• lowrisedwellinp whose lateral dimension do Dot exceed 45 m, the NOTE-If the maximum deflection in mm, shown duriftl 24 h under load is lessthan40 12/D where I is theeffectivespan in m; and D is the overall depth of the section in rom, it i. not necessary for the ~ to be measured. b) The structure shall have adequate strenath to sustainfor 24 h, a total load equal to the characteristic load multiplied by 1.331, where Y, shall 32 IS 456: 2000 effects due to temperature fluctuations and shrinkage and creep can be ignored in design calculations. 20.2 Sliding The structure shall have a factor against sliding of not less than 1.4underthe most adverse combination of the appliedcharacteristic forces. In thiscase only0.9 times the characteristic dead load shall be taken into account. 19.6 Other Forces and Effects In addition, account shall be taken of the following forces and effects if they are liable to affect materially the safety and serviceability of the structure: 20.3 Probable Variation in Dead Load To ensure stability at all times, account shall be taken of probable variations in dead loadduringconstruction, repairor other temporarymeasures. Wind and seismic loading shall be treated as imposed loading. a) Foundation movement (see IS 1904), b) Elastic axial shortening, c) Soil and fluid pressures [see IS 875 (Part 5)], 20.4 Moment Connection In designing the framework of a building provisions shall be made by adequate moment connections or by it system of bracings to effectively transmit all the horizontal forces to the foundations. d) Vibration, e) Fatigue. o Impact [see IS 875 (Part 5)], g) Erection loads (see IS 875 (Part 2)], and h) Stressconcentrationeffect due to point loadand the like. 20.5 Lateral Sway LInder transient wind load the lateral sway at the top should not exceed HI500, where 11 is the total height of the building, For seismic loading, reference should he made to IS J 893. 19.7 Combination of Loads The combination of loads shall be as given in IS 875 (Part S). 21 FIRE RESISTANCE 19.8 Dead Load Counteracting Other Loads and Fon:es 21.1 Astructure Of structural element required to have fire resistance should be designed to possess an appropriate degreeof resistanceto flame penetration; heat transmission and failure. The fire resistance of a structural clement is expressed in terms of time in hours in accordance with IS 1641. Fire resistance of concrete elements depends upon details of member size. cover to steel reinforcement detailing and type of aggregate (normal weight or light weight) used in concrete. General requirements for fire protection are given in IS 1642. When dead load counteracts the effects due to other loads and forces in structural member or joint, special care shall be exercised by the designer to ensure adequate safety for possible stress reversal. 19.9 Deslgn Load Design load is the load to be taken for use in the appropriate method of design; it is the characteristic loadin case of workingstressmethodandcharacteristic load with appropriate partial safety factors for limit state design. 21.2 Minimum requirements of concrete cover and member dimensions for normal-weight aggregate concrete members so its to have the required fire resistance shall be in accordance with 26.4.3 and Fig.l respectively. 20 STABILITY OF THE STRlJCTlJRE ZO.1 Overturnina The stability of a structure as a whole against overturning shall be ensured so that the restoring moment shan be not less than the sum of 1.2times the maximumoverturning momentdue to thecharacteristic dead load and 1.4 times the maximum overturning moment due to the characteristic imposed loads. In cases where dead load providesthe restoring moment, only 0.9 times the characteristic dead load shall be considered. Restoring moment due to imposed loads shall be ignored. 20.1.1 The anchorages or counterweights provided for overhanging members (during construction and service) should be such that static equilibrium should remain, even when overturning moment is 21.3 The reinforcement detailing should reflect the changing pattern of the structural section and ensure that both .individual clements and the structure as a whole contain adequate support. tics, bonds and anchoragesfor the required tire resistance.. 21.3.1 Additionalmeasuressuch as application of fire resistant finishes. provision of fire resistant false ceilings and sacrificial steel in tensile zone, should he adopted in case the nominal cover required exceeds 40 mm for beams and 35 mm for slabs, to give protection against spelling. 21.4 Specialist literature may be referred to for determining fireresistance of the structureswhichhave not been covered in Fig. 1 or Table 16A. doubled. 2116 el5/07---6 33 IS 456: 2000 BEAMS -Pw~· SOLID SLAB RIB I WAFFEL SLAB SLABS ~ : " ..: ".. b .t': ~ f ONE FACE EXPOSE -IbJ... FULL V EXPOSED COLUMNS --_....._. __....... ------_._-- - Column Dimension tb fir DJ Fire Resis- MilJimum tllme " 0.5 I 1.5 2 3 4 Rib Width Minimum Thickness Width b /11 Slabs bw ofFloors D mm mill mID 200 200 200 125 125 12S 125 75 /team ZOO 240 280 ISO 175 95 110 125 150 170 ... ... ... Fully Exposed 50% One EXPOliCd Face Bxposed IIIID 111m mm 150 200 250 m 160 2(X) 140 175 ~on 200 160 400 450 .100 200 240 350 - Minimum Wall Thicknt.u 1'<0.4% .... 04%sp.sl% 1'>1% mm mm tOO 150 120 ISO 100 120 140 160 200 240 mm 100 100 100 100 150 180 NOTES 1 These minimum dimensions relatespecifically to the covers givenin Teble 16A. :z p is the percentage of steel reinforcement. FlO. 1 MINIMUM DIMENSIONS OF REINFURCED CONCRE'1ll MEMBERS FOR FIRE RESiSTANCE 22 ANALYSIS 22.2 Effective Span 22.1 General Unless otherwise specified, the effective span of a member shall be as follows: a} Simply Supported Beam or Slab-The effective spanof a member thatis notbuiltintegrally with its supports shall be takenas clearspan plus the effective depth ofslaborbeam or centre to centre of supports. whichever is less. All structures may be analyzed by the linear clastic theory to calculate internal actions produced by design loads. In lieu of rigorous elastic analysis, a simplified analysis as given in 22.4 for frames and as givenin 22.5forcontinuous beams may be adopted. 34 IS 456: 2000 b) Continuous Beam or Slab - In the case of continuous beam or slab. jf the width of the support is less than 1/12 of the clear span, the effective span shall be as in 22.2 (a). If the supports are wider than 1/12 of the clear span or 600 mm whichever is less, the effective span shall be taken as under: 22.4.1 Arrangement oflmposed Load a) Consideration may be limited to combinations of: 1) Design dead load on all spans with full design imposed load on two adjacent spans; and 2) Design dead load on all spans with full design imposed load on alternate spans. 1) For end span with one end fixed and the other continuous or for intermediate spans. the effective span shall be the clear span between supports; b) When design imposed load does not exceed three-fourths of the design dead toad, the load arrangement may be designdead load and design imposed load on all the spans. 2) For end span with one end free and the other continuous, the effective span shall be equal to the clear span plus half the effectivedepth of the beam or slab or the clear span plus half the width of the discontinuous support, whichever is less; NOTE ----. For beams and slabs continuous over support 22.4.1Ca) rna)' be assumed, 22.4.2 Substitute Frame For determining the moments and shears at any floor or roof level due to gravity loads, the beams at that level together with columns above and below with their far ends Ii xed may be considered to constitute the frame. 3) In the case of spans with roller or rocket bearings. the effective span shall always he the distance between the centres ofbearings. c) Cantilever- The effectivelengthof a cantilever shall he taken as its length to the face of the support plus half the effective depth except where it forms the end of a continuous beam where the length to the centre of support shall be taken. 22.4.2.1 Where side sway consideration becomes critical due to unsymmctry in geometry or loading, rigorous analysis ITIay be required. 22.4.3 For lateral loads, simplified methods may be used to obtain the moments and shears for structures that arc svmmetrical. For unsymmetrical or very tall structures. more rigorous methods should be used. d) Frames - In the analysis of a continuous Irarne, centre to centre distance shall he used. 22.3 Stiffness 22.5 Moment and Shear Coefficientfi for Continuous Beams 22.3.1 Relative Stiffness 22.5.1 Unless more exact estimates are made. for beams of uni form cross-section which support substantially uniformly distributed loads over three or IlH ire :'\1 ',UlS which do notdiffer by more-than 15percent of the longest, the bending moments and shear forces used in design may be obtained using the coefficients given in Table 1.2 and Table 13 respectively. The relative stiffness of the members may be based on the moment of inertia of the section determined on the basis of anyone of the following definitions: a) Gross section - The cross-section of the memberignoringreinforcement: b) Transformed section - 'The concrete crosssection plus the area of rc intor ccmcrn transformed on the basis of modular ratio (St'l' B-I.3); or For moments at supports where two unequal spans meet or j n case where the spans are not equally loaded, the average of ttlc two values for the negative moment at the Stlppt ut may he taken for design. c) Cracked section _.- The area of concrete in compression plus the area of reinforcement transformed on the basis of modular rutin. Where coeflicients given in Table 12 are used for calculationof bending moments,redistributionreferred to in 22.7 shall not be permitted. The assumptions made shall be consistent for (111 the members of the structure throughout any analysis. 22.5.2 Beamsand Slabs Over Free End Supports Where a member is built into a masonry wall which develops nnly partial restraint. the member shall be designed to resist a negative moment at t.he face of the support of W1/24 where W is the total design load and l is the effective span, or such other restraining moment as may be shown to he applicable, For such a condition shear coefficient given in Table 13 at the end support may be increased hy 0.05. 22.3.2 For deflection calculations, appropriate values of moment of inertia as specified in Annex C shGUIU be used. 22.4 Structural Frames The simplifying assumptions as given in 22.4.1 to 22..4.3 may be used in the analysis of frames. 35 IS 456 : 2000 Table 11 Bending Moment Coefficients (Clause 22.5.1) .. Type of Load Span Moments "." Near Middle of End Span (1) Dead load nodimposed load (fixed) Imposed load (not , t"t At Middle of Interior Span At Support Next to the End Support Supports (2) (:l) (4) (5) 1 +12 I +16 1 10 +- I 12 +- fixed) Support Moments , ; At Other Interior I 10 I 12 1 9 1 9 NOTE- For obtainingthe bendingmoment, the coefficient shall be multiplied by the total design load and effectivespan. Table 13 Shear for Coefficients iClauses 22.5.1 and 22.5.2) Type 01Load At End Support At Support Next to the End Support At AllOther Interior Supports t"t &;ter Side InnerSide (2) (3) (4) (~) Dead loud and imposed load (fixed) 0.4 0.6 0.55 0.5 Imposed load (not 0.45 0.6 0.6 0.6 (I) fixed) NOTE- For obtainingthe shear force. the coefficientshall be multiplied by the total designload. 22.6 Critical Sections for Moment and Shear 23 BEAMS 22.6.1 For monolithic construction, the moments computed at the face of the supports shall be used in the design of the members at those sections. For non.. monolithic construction thedesignof the membershall be done keeping in view 22.2. 23.0 Effective Depth Effectivedepth of a beam is the distance between the centroid of the area of tension reinforcement and the maximum compression fibre, excluding the thickness of finishing material not placed monolithically with themember andthethickness of any concrete provided to allow for wear. This will not apply to deep beams. 22.6.2 Critical Section/or Shear The shears computed at the face of the support shall be used in the design of the member at that section except as in 22.6.2.1. 23.1 T-Beams and L·Beams 23.1.1 General 22.6.Z.1 When the reaction in the direction of the applied shear introduces compression into the end region of the member, sections located at a distance Jess than d from the face of the support may be designed for the same shear as that computed at distance d (see Fig. 2). A slab which is assumed to act as a compression flange of a T-beam or L-beam shall satisfy the following: a) The slab shall be cast integrally with the web, or the web and the slab shall be effectively bonded together in any other manner; and b) If the main reinforcement of the slab is parallel to the beam, transverse reinforcement shall be provided as in Fig. 3; such reinforcement shall not be less than 60 percent of the main reinforcementat mid span of the slab. N()TE-The above clauses are applicablefor beamsgenerally carryinguniformly distributedloudor wherethe principal load is located furtherthan "2d (ruin the face of the support. 22.7 Redistribution of Moments Redistribution ofmoments may be done in accordance with 37.1.1 for limit state method and in accordance with8-1.2 forworking stressmethod. However, where simplified analysis using coefficients is adopted, redistribution of moments shall not be done. 23.1.2 Effective Width of Flang, In the absence of more accurate determination. the effective widthof flange may be takenas thefollowing 36 IS 456: 2000 d (0) (b) t FIG. 2 TYPICAL SUPPORT CONOmONS FOR LOCATING FACI'ORED SHEAR FORCE but in no case greater than the breadthof the webplus halfthesumof thecleardistances to theadjacent beams on either side. a) ForT-beams,h, =~ +b", + 6D, b) For L-beams, b, I =~ + bw + 3 D, 12 structureor finishes or partitions. Thedeflectionshall generally be limitedto the following: a) The final deflection due to all loads including the effects of temperature, creep and shrinkage and measured from the as-cast level of the supports of floors, roofs and all other horizontal members, shouldnotnormally exceedspanl2S0. b) The deflection including the effects of temperature, creepandshrinkage occurring after erection of partitions and the application of finishes should not normally exceed span/3S0 or 20 mm whichever is less. c) For isolated beams, the effective flange width shallbe obtainedas belowbut in nocasegreater than the actual width: T - beam,b, .~I)o + b.. .:JL b +4 23.2.1 The verticaldeflectionlimits may. generallybe assumed to be satisfiedprovidedthat the spanto depth ratiosare notgreater thanthe valuesobtainedas below: a) Basic values of span to effective depth ratios for spans up to 10m: · O.S In b L - beam, b '=~+ w ...!l. +4 b Cantilever 7 Simplysupported 20 Continuous 26 b) For spans above 10 m, the values in (a) may be multiplied by 10/span in metres, except for cantileverin whichcase deflection calculations should be made. c) Depending on the area and the stress of steelfor tensionreinforcement, the valuesin (a) or (b) shall be modifiedby multiplying withthe modification factor obtainedas per Fig. 4. d) Depending on the area of compression reinforcement, the value of span to depth ratio be further modified by multiplying with the modification factor obtainedas per Fig. S. where b, In =effective width of flange, =distance betweenpoints of zero moments in the beam, b", = breadth of the web, Dr =thickness of flange, and b = actual width of the flange. NOTE - Por continuous beams and frame., ",,' may be assumed lUI 0.7 time.the effective span. 23.2 Control of Defledlon The deflection of • structure or part thereof shall not adversely affect the appearance or efficiency of the 37 IS 456 : 2000 BEAM I I I I I I T-+----+-+----+--I I Xl t--~- SECTION XX FIG. 3 TRANSVERSE REINFORCEMENT IN FLANGB OFT-BEAM WHEN MAIN REINFORCEMENT Of SLABIS PARAIJ.EL TOTHE BEAM e) For flanged beams, the values of (a) or (b) be modified as per Fig. 6 and the reinforcement percentage foruseinFig.4 and 5 shouldbebased 2·0 \ ',6 \\ \ \ \' \ ~ NOTE-When deflections are required to be calculated, the method given in Annex C may be used. r-, " r-, \ \ -, <, r-, I<, ........ \ on area of sectionequal to b,d. I'-... r-, <, <, 10.",. r--- r---- r-.... I"'-- -.. ~ ~ f•• '45 r--r-- I-- f--... ~ I-... f""90 fu240 h·290 - , I Note: f. IS STEEL STRESS OF SERVICE ,LOADS IN N/mm2 I o 0'4 0,' " ',2 1'6 2·0 2" PERCENTAGE TENSION REINFORCEMENT I. .0.58 f. • ArMof CI'OII' _tion ohteel required ., AreaofCmll • aection of steel provided Flo. 4 MODIACATJON FAcroR FOR TENSION REINFORCEMENT 38 2'8 )0 18456: 2000 .-.-. ~ ~ ~ ~ 100""" ~ L/ V V / ,/ 0-50 '-00 1-50 2-00 2-50 PERCENTAGE COMPRESSION REINFORCEMENT FIG.5 MOOIHCATION FACTOR FOR COMPRESSION REtNPoRCBMENT 1'100 a: 1/ 0095 / e~ e-sc /" &L z 0.85 Q / t ~ 0·80 a: 0·75 0.70 FIG. 6 / o 0'2 0'4 0·8 0'8 1·0 RATIO OF WEB WIDTH TO FLANGE WIDTH REDUCTION FACTORS FOR RA'110S OF' SPAN TO EJ-rEcnVE DEPTH FOR FLANGED BEAMS NOTBS 1 For slabsspanninl in two directions,the shorterof the two spans should be used for calculating the span to etTective depth ratios. 2 For two-wavslabsof shorter spans(up to 3.~ m) with mild stoel reinforcement, the span to overall depth ratios given below may generally be assumed 10 satisfy vertical deflectionlimits for loading class up to 3 kN/mJ• Simplysupportedslabs 3S Continuous slabs 40 23.3 Slenderness Limit'! for Beams to Ensure Lateral Stability A simply supported or continuous beam shall be so proportioned that the clear distance between the lateral . restraints does not exceed 60 b Of 250b z -- d whichever is less, where d is the effective depth of the beam and b the breadth of the compression face midway betwecn the lateral restraints. For highstn:ngthdefonned barsof smde Fe41~. the values givenaboveshould be multiplied by 0.8. For a cantilever, the clear distance from the free end of the cantilever to the lateral restraint shall not 100b z exceed 25 b or _.d 24.2 Slabs Continuous Over Supports Slabs spanning in one direction and continuous over supports shall bedesigned according to the provisions applicable to continuous beams. whichever is less. 24 SOLID SLABS 24.3 24.1 General S~~bs Monolithic with Supports Bendingmomentsin slabs (except flat slabs)constructed monolithically with the supports shall becalculated by takingsuch slabs either as continuous over supports and The provisions of 13.2 for beams apply to slabs also. 39 IS 456: 2000 capable of free rotation.or as membersof a continuous framework with the supports, taking into account the stiffness of such supports. If suchsupports are formed due to beamswhichjustify fixityat the supportof slabs, then the effects on the supporting beam, such as, the bending of the web in the transverse direction of the hewn and the torsionin the longitudinal direction of the beam. whereverapplicable, shall also be consideredin the design of the beam. c) For two or more loads not in a line in the direction of thespan. if theeffective width of slabfor one load does notoverlapthe effective width of slab for anotherload, both calculated as in (a) above,thenthe slab for each loadcan be designedseparately. If the effectivewidth ofslabforoneload overlaps theeffective width of slab for an adjacent load, the overlapping portion of the slab shall be designed for the combined effectof the twoloads. 24.3.1 For the purpose of calculation of moments in slabs in a monolithic structure, it will generally be sufficiently accurateto assumethatmembersconnected to the ends of such slabs are fixed in position and direction at the ends remote from their connections with the slabs. Table14Values 01 k for Sbnply Supported and Continuous Slabs (Clause 24.3.2.1) 24.3.1 Slabs Carrying ConcentratedLoad O.S 0.6 0.7 0.8 0.9 1.0 and above ber where ber lef where effective width of slab, = distance of the centroid of the concentrated load from nearer support, Ir f = effective span, and a = width of the contact area of the 2.16 2.24 = 1.2a l +a ill = effective width, =distance of the concentrated load from the a = widt.h of contact area of the concentrated face of the cantilever support, and = constant havingthe valuesgiven inTable 14depending upon the ratio of the width of the slab (/~ to the effective span Ie{ , x 0.4 0.8 1.16 1.48 1.72 1.96 2.12 2.24 2.36 2.48 d) For cantilever solid slabs, the effective width shall he calculated in accordance with the following equation: ber = kx (1- ..!..)+ a k 51•• 0.4 0.8 1.16 1.44 1.68 1.84. 1.96 2.08 0.1 a) For a single concentrated load. the effective width shall be calculated in accordance with the following equation provided that it shall not exceed the actual width of the slab: = i lor CoatlDUQUI 0.2 0.3 0.4 24.3.2.1 If a solidslab supportedon twooppositeedges, carries concentrated loads the maximum bending moment caused by the concentrated loads shall be assumed to be resisted by an effective width of slab (measured parallel to the supportingedges) as follows: bd i lorSlmpl, Supported S.... load measured parallel to the supporting edge. Provided that the effective widthof the cantilever slab shall not exceed one-third the length of the cantilever slabmeasured parallel to thefixededge. Andprovidedfurtherthat when theconcentrated loadisplaced neartheextreme endsof the length of cantilever slab in the direction parallel to the fixed edge. the effective width shall not exceed the above value, nor shall it exceed half the above valueplus thedistanceof the concentrated load from the extreme end measured in the direction parallel to the fixed edge. . concentrated load from nearer support measured parallel to the supportededge. And provided further that in case of a load near the unsupported edge of a slab. the effective width shall not exceed the above value nor half the above valueplusthedistance oftheload from the unsupported edge. 24.3.2.2 For slabs other than solid slabs, the effective width shall depend on the ratio of the transverse and longitudinal flexural rigidities of the slab. Where this ratio is one, that is, where the transverse and longitudinal flexural rigidities arc approximately equal, the value of effective width as found for solid slabs may be -used. But as the ratio decreases, proportionately smaller value shall he taken. b) For two or more concentrated loads placed in a line in the direction of the span, the bending moment per metre width of slab shall be calculated separately for each load according to its appropriate effective width of slab calculated as in (a) above and added together for design calculations. 40 IS 456: 2000 signs),the total should be equal to that from (a). If the resulting support moments are significantly greaterthan the value from Table 26, the tension steel over the supports will need to be extended further. The procedure should be as follows: 1) Takethe spanmomentas parabolic between supports: its maximum value is as found from (d). 2) Determine the points of contraflexure of the new support moments [from (c)] with the span moment [from (1)]. 3) Extendhalfthesupporttensionsteelat each end to at least an effective depth or 12 bar diameters beyond the nearest point of contraflexure. 4) Extend the full area of the support tension steel at each end to half the distance from 24.3.2.3 Any other recognizedmethodof analysisfor Casel of Ilaba covered by 24.3.%.1 and 24.3.2.2 and fot all othet ~ase8 of slabs may be used with the approvai Of aM engineer*in-charge. 24.3.2.4 The critidil Medon for checking shear shall be as Jiven in 34.2.4.1. 24.4 Slabs SpaDllinllD two Directions at Rllbt ADII_ The slabs spanning in two directions at right angles and carryinS uniformly distributed load may be desilned by any acceptable theory or by usina coefficients liven in Annex D. For determining bending moments in slabs spanningin two directions at right anales and carrying coaeentrered load, any accepted method approved by the engineer-In-charge may be adopted. NOTS-The IDOII commonly UJed elastic methods are based on Apaud', or Wester-pard', theoryandthe most commonly uled limitItaJe of coUapse methodis basedonJohansen's yieldline theory. (3). 24.5 Loads on SuPportiDI Beams 14.4.1 Restrained Slab with Unequal Conditions at Adjacent Pan,I, The loads on beams supporting solid slabs spanning in two directions at right angles and supporting uniformly distributed loads, may be assumed to be in accordance with Fig. 7. In some cases the support moments calculated from Table 26 for adjacent panels may differ significantly. The following procedure may be adopted to adjust them: a) Calculate the sum of moments at midspan and IUpports (nea1ecting signs). b) treat the values from Table 26 as fixed end m<mieDts. c) According tCJ the relative stiffness of adjacent spans, distribute the fixed end moments across the supports, living new support moments. d) Adjult midspanmomentsuch that, whenadded to the support moments from (c) (neglecting 25 COMPRESSION MEMBERS 25.1 Definitions 25.1.1Columnor strut is a compressionmember, the effective lengthof whichexceeds three times the least lateral dimension. 25.1.2 Shortand SlenderCompression Members A compression member may be considered as short Dand hb · I when both the slenderncb; ~o. than 12: A LOAD IN THIS SHADED AREA TO BE CARRIED 8V BEAM 'e' LOAD IN THIS SHADED AREA TO BE CARRIED BY BEAN '// FlO. 2116 818/07-1 7 LOAD C ARRJIID BY SUPPORTING BEAMS 41 B are less IS 456 : 2000 where 1 = M effective length in respect of the major where b axis, D == Iry - b = D depth in respect of the major axis, effective length in respect of the minor axis, and width of the member, = = width-of that cross-section, and depthof the cross-section measuredin the plane under consideration. 25.4 Minimum Eccentricity All columns shall be designed for mmrmum eccentricity, equalto theunsupported length of column! compression member, 500 plus lateral dimensions/30, subject to a minimum of 20 rom. Where bi-axialbending is considered,it is 25.1.3 Unsupported Length sufficient to ensure that eccentricity exceeds the The unsupported length, I, of a compression member . minimum about one axis at a time. shall he taken as the clear distance between end It shall otherwise be considered as a slender restraints except that: a) in flat slab construction, it shall be clear distance between the floor and the lower extremity of the capital, the drop panel or slab whichever is the least. h) in beam and slab construction, it shall be the clear distance between the floor and the underside of the shallower beam framing into the columns in each direction at the next higher floor level. c) in columns restrained laterally by struts, it shall be the clear distance between consecutive struts in each vertical plane, provided that to be an adequate support, two such struts shall meet the columns at approximately the same level and the angle between vertical planes through the struts shall not vary more than 3Qt' from a right angle. Such struts shall be of adequate dimensions and shall have sufficient anchorage to restrain the member against lateral deflection. 26 REQUIREMENTS GOVERNING REINFORCEMENT AND DETAILING 26.1 General Reinforcing steelof same type and grade shall be used as main reinforcement in a structural member. However. simultaneous use of two different types or grades of steel for main and secondary reinforcement respectively is permissible. 26.1.1 Bars may be arranged singly. or in pairs in contact, or in groups of three or four bars bundled in contact. Bundledbars shall be enclosedwithin stirrups or ties. Bundled bars shall be tied together to ensure the bars remaining together. Bars larger than 32 mm diameter shall not be bundled. except in columns. 26.1.2 The recommendations for detailing for earthquake-resistant construction given in IS 13920 should be taken into consideration, where applicable (see also IS 4326). 26.2 Development of Stress in Reinforcement The calculated tension or compression in any bar at any section shall be developed on each side of the section by an appropriate development length or end anchorage or by a combination thereof. d) in columns restrained laterally by struts or beams, with brackets used at the junction, it shall be the clear distance between the floor and the lower edge of the bracket, provided that the bracket width equals that of the beam strut and is at least half that of the colurnn. 26.2.1 Development Length ofBars The development length Ld is given by ,a. 25.2 Effective Length of Compression Members _ L( 1 - - - In the absence of more exact analysis, the effective length ler' of columns may be obtained as described in Annex E. 4fbd where , = nominaldiameter of the bar, 25.3 Slenderness Limits for Columns a ~ =stressin bar at the sectionconsideredat design 25.3.1 The unsupported length between end restraints shall not exceed 60 times the least lateral dimension of a column. load, and t hd = design bond stress given in 26.Z.1.1. NOTES 1 The development IcnJlhincludca anchomae vDlues of hooks in tension reinforcement. 2 For bars of sections other than cireular. the development lenathshould be sufficient to develop the stras in the bar by bone" 25.3.2 If, in any given plane, one end of a column is unrestrained, its unsupported length, it shall not exceed JOOb 2 ---' [) 0°' ...",,: ..... 'lI I, :i 42 .c. .;. IS 456: 2000 16.2.1.1 Design bond stress in limit state method for plain bars in tension shall be as below: Grade ofconcrete M20 M25 M30 M35 Design bondstreSJ, f hd, N/mm2 1.2 1.4 1.5 1.7 M 40 and above 1.9 For deformed bars conforming to IS 1786these values shall be increased by 60 percent. 2) In the compression zone, front the mid depth For bars in compression. the values of bond stress for bars in tension shall be increased by 25 percent. b) Stirrups-Notwithstanding any of the provisions of this standard, in case of secondary reintorcement, such as stirrups and transverse ties, complete development lengths and anchorage shall be deemed to have been provided when the bar is bent through an angle The values of bond stress in working stress design, are given in B-2.1. 26.2.1.2 Bars bundled ;11 contact of the beam. of at least 90" round a bar of at least its own diameter and is continued beyond the end of the curve for a length of at least eight diameters, or when the bar is bent through an angle of 135 and is continued beyond the end of the curve for a length of at least six bar diameters or when the bar is bent through an angle of 1HO° and is The development length of each bar of bundled bars shall be that for the individual bar, increased by )0 percent for two bars in contact, 20 percent for three bars·in contact and 33 percent for four bars in contact. 0 26.2.2 Anchoring ReinforcingBars 26.2.2.1 Anchoring bars in tension a) Deformed bars may be used without end anchorages provided development length requirement is satisfied. Hooks should normally he provided for plain bars in tension. b) Bends and hooks conform to IS 2502 Bends and hooks shall J) Bends-The anchorage value of bend shall be taken as 4 times the diameter of the bar for each 45 bend subject to a maximum of 16 times the diameter of the bar. 2) Hooks-The anchorage value of a standard U-type hook shall be equal to J6 times the diamet.er of the bar. continued beyond the end of the curve for a length of at least four bar diameters. 26.2.2.5 Bearing stresses at bends The hearing stress in concrete for bends and hooks describedin IS 2502 need not be checked. The bearing stress inside a bend in any other bend shall be calculated as given below: t ' Bearing stress = Fht rei> where }/'ol =: tensile force due to design loads in a bar or group of hal's, 26.2.2.2 Anchoring bars in compression ,. = internal radius of the bend, and The anchorage length of straight bar in compression shall be equal to the development length of bars in compression as specified in 26.2..1. The projected length of hooks, bends and straight lengths beyond bends if provided for a bar in compression, shall only be considered for development length. ¢ = size of the bar or, in bundle. the size of har of equivalent area. 16.2.2.3 Mechanical devices [or anchorage Any mechanical or other device capable of developing the strengthof the bar without damage to concrete may be used as anchorage with the approvalof the engineerin-charge. 26.2.2.4 Anchoring shear reinforcement a) Inclined bars - The development length shan be as for bars in tension; this length shall be measured as under: 1) In tension zone, from the end of the sloping Of inclined portion of the bar, and For limit stale method of design, this stress shall not exceed I .5f~k 1+2~/a W tiere r.+' h h .. k IS t e. c aractensuc cube C· strength of concrete and a, for a particular bur or group of hars in contact shall he taken as the centre to centre distance between bars or groups of bars perpendicular to the plane of the bend; for a bar Of group of bars adjacent to the face of the member a shall he taken as the cover plus size of bar ( q». For working 'stress method of design. the bearing stress shall not exceed --~. J+2c/J/a 26.2.2.6 If a change in direction of tension or compression reinforcement induces a resultant force acting outward tending to split the concrete, such force IS 456: 2000 should betaken up by additional linka orstirrups. Bent tensionbar at a re-entrantangle should be avoided. 26.2.3 Curtailment 01 relll;on- R~;nforce",,"t ill Flexural Member, - 26.2.3.1 For curtailment. reinforcement .baIl eltead beyond the point at which it is no lonler required to resistflexure for a distance equalto the effective depth of the memberor 12timesthebardiameter, whichever . is greaterexceptat simplesupportor end of cantilever. In addition 26.2.3.2 to 26.2.3.5 .hall also be satisfied. NOTE-A point at which reinforcement I, 80 loftpl' required to resist flexure is where theresistance momentoflht 1eCti0ll, considering only the continuinl ban, is equal to the deaip moment. 26.1.3.2 Flexural reinforcement shall notbetenninated in a tension zone unless anyone of the following conditions is satisfied: a) The shear at the cut-off point does not exceed two-thirds that permitted, includinl the shear strength of web reinforcement provided. b) Stirrup area in excess of that required for shear and torsion is provided along each tennlnated bar over a distance from the cut-offpointequal to three-fourths the effective depth of the member. The excess stinup area shall be not less than 0.4 bIll" where b is the breadth of beam. s is thespacing and[, is the characteristic strength of reinforcemC:nt in N/mm 2• The resulting spacingshall notexceed dIs Pit where Ph is the ratio of the area of ban cut-off to the total area of bars at the section, and d is the effective depth. c) For 36 rnmandsmallerbars,thecontinuing bars provide double the area required for flexure at the cut-offpoint and the sheardoes not exceed three-fourths that permitted. ... -- M, '* .....- of lUiltllCe of tile section ......., IllNillforc.a.ent at abe aecdOD to . . . . . . tot..; ttl • 0.871, In tbI c... of liJpit sJate desip and thO penni••ible. . . (J. in-the case of working Stroll deillft; V = shearforce at the section due'to desip loads; Lo = sum of theanchorage beyondthecentre of the support and the equivalent ,p~J1orale value of any hook or mNhan~ ~ge at simple support; andat a point lit iltlWURaJ, bRis limited to the effecdvo dopth of die ""m~1l PJ 12;, whichever is pater; and diameter of bar. Thevalue of M. /Vin theabove expression may be incr••,ad by 30 percent when the ends of the reinforCOlftO,;r .... ~OJJtined by a compressive reaction. ; = 26.2.3.4 Ntgative moment ,,;nforcernent At leat one-third of the ~JaI ~inforc~nt provided for nepavi JIJOIft8tIt IldtflUPPOJt sball extend beyond the point of i"fbJodo" for It 4jstanee not less than the effective depth ofthl of 12, orone-sixteenth of theclearspan whichov" i, 8f8*. mom'* 26.2.3.5 Curtai"",,,' ofbUNII.d bar, Bars in a bundle shall terminate at difforln~ points spaced apartbynotleiS than40times the bardiamoter except for bundles Itoppin. at a support. 26.1.4 SpecialM,mber! Adequate end anchoralo shall be providod for .",10" reinforcement in flexural memben where roinfOJlJO" mcnt stress is not direcdy proportional to mOlMltl, suchas sloped. ltepped, or tapered footinp; brackets; deep beams; and members in which the tension reinforcement is not parallel to the comprel.ion fICO. 16.1.3.3 Positive momentreinforcement a) At least one-third the positive moment reinforcement in simple members and onefourth the positive moment reinforcement in continuous members shall extend along thesame face of the memberinto thesupport,to a length equal to Ld/3. b) When a flexural memberis part of the primary lateral load resisting system, the positive reinforcement required to be extended into the supportas described in (a) shall be anchored to develop its design stress in tension at the face of the support. c) At simple supports and at points of inftection, positive moment tension reinforcemeat shallbe limited to a diametersuchthat Ld computed for !.J by 26.2.1 does not exceed 26.%.5 R,inforclment Spllcin, Where splices are provided inthereinforcinl ban.they shall u f. 81 possible be away from the IeCUonl of maximum ItreS' and beltagered. It iancommendod that splices in flexural memben Ihould "Ol bf at sections whore the bendinl moment i. more than '0 percent of the momentof resistance; and not mON Chan halfthe barsshallbe spliced at a section. Where more than one·balf of tho ban are spliced at a section or wbere splices are mad. It point. of maximum stress, special precaution. shall bo eaken, 44 IS456:~ suchas increasing the lengthof lapand/oruSlnS spirals or closely-spaced stirrups around the length of the splice. -.u.l Lap ,plie" a) Lapsplicesshall not beusedforbars larger than' 36 rom; for larger diameters, bars may be welded (see 12.4); in cases where welding is not practicable, lapping of bars larger than 36 mm may be permitted, in which case additional spiralsshouldbe provided around the lapped bars. b) Lap splices shall be considered as staggered if the centre to centre distance of the splices is not Jess than 1.3timesthe laplength calculated as described in (e). c) Lap lengthincluding anchorage valueof hooks for bars in flexural tension shall be Ld tse« 26.2.1) or 30(/) whichever is greater and for direct tension shall be 2Ld or 30~ whicheveris greater. The straightlengthof the lap shall not be Jess than IS, or 200 mm. The following provisions shall also apply: Wherelap occurs for a tension bar located at: I) top of a section 8S cast and the minimum cover is less than twice the diameter of the lapped bar,the lap length shall be increased by a factor of 1.4. 2) comer of a section and the minimum cover to either face is less than twice the diameter of the lapped bar or where the clear distance between adjacent laps is less than 7S mm or 6 times the diameter of lappedbar. whichever is greater, the lap lengthshould be increased by a factor of ).4.' Where both condition (1) and (2) apply. the lap length should be increased by a factor of 2.0. . NOTE-Splices ia tension members shall be enclosed in spirals madeof bon DOl lessthan6 mmdiameter withpitch not lnofe than 100mm. d) The lap lengthin compression shan be equal to the development length in compression, calculated as described in ~.1.1. but not less than 24~. e) When bars of two differentdiameters are to be spliced, the lap le"gth shall be calculated on the basis of diameter of the smallerbar. t) When splicing of welded wire fabric is to be carried out, lap splices of wires shall be made so that overlap measured between the extreme cross wires shall be not less than thespacingof pross wires plus 100 mm, _> In case of b"ndlod bars, lapped splices of l1""dtcd ban shall bemade by splicingone bar at a time; suchindividual spliceswithina bundle shall be staggered. 16.1.5.2 Strength o/welds The following values may be used where the strength of the we1d has been proYed by tests to be at least as great 1$ d1~ of tho parent bar. .' a) Splices' in compression - For welded splices and mechanical connection, 100 percent of the desis" strength of joined bars. b) Splices in tension I) 80 percent of the design strength of welded bars (100 percent if welding is Itrictly supervised and if at any cross...aectionof the member not more than 20 percent of the tensile reinf(lr~tnent is welded). 2) \00 pcf~nt of design strength of mecha- nical connection. 16.2.5.3 End-bearing splices End-hearing splices shall be used only for bars in compression. The ends of the bars shall be square cut and concentric bearing ensured by suitable devices. 16.3 Spacinl of Relnloreenaent 26.3.1 For the purposeof this ~I.-"se. the diametor of round bar shall be its diamoto" and in the case of bars w~ich ~ro no, round or in tho case of deformed bars or crimpod ~It tho diamoter shall be taken as the <l,,,~etef of a oifcle .ivinJ an equivalent effecti ve arcs". Whero Ipacin. limitations and minimum CO"QfOtc cover (I" Z6A) are bued on bar diameter. a group of ban bundled in contact shall be treated as a linslo bar of diameter derived from the a n011\"'" total ~quiY_'enl aroa. J6.3.1 Minimum Distance Between IndividUfJI Bars The followi"g shall apply for .pacinl of ban: a) The _orizontal distance between two parallel main'reinforcinl bars shall usually be not less thantho lreato., of tho foUowina: I) ll-" di..meter of tho bar if the diameteR are e4l~alt 2) Th~ diameter of the larler bar if the diamolCrs are unoqual. and 3) S 111m moro than tho nominal maximum size of ~p~ _IPlalO. ~OTB-This does not preclude the use orllllpr size of D.I",.itel beyond the conceated reinfon:ement in the lAme member; lhe aize of ,"relates ,nay be naduoocl Ground con,clted reinforcement tQ comply with thil provision. b) Qreater horizontal distance than tho minimum specified in (a) should be prov~dod wherevor possible. However when needle vibrators aro 45 IS 456 : 2000 used the horizontal distance between bars of a group may be reduced to two-thirds the nominal maximum size of the coarse aggregate, provided that sufficient space is left between groups of bars to enable the vibrator to be immersed. c) Where there arc two or more rows of bars, the bursshall he vertically in line and the minimum vertical distance between the bars shall be 15 mrn, two-thirds the nominal maximum size of aggregate or the maximum size of bars, whichever is greater. 26.3.3 Maxi/nun, Distance Between Bars in Tension Unless the calculation of crack widths shows that a greater spacing is acceptable, the followingrules shall he applied to flexural members in normal internal or external conditions of exposure. a) Beams - The horizontal distance between parallel reinforcement bars, or groups, ncar the tension face of a beam shall not be greater than the value given in Table 15 depending on the amount of redistribution carried out in analysis and the characteristic strength of the reinIorcement. b) Slabs 1) The horizontal distance between parallel main reinforcement barsshallnotbemore thanthree times the effective depth of solid slab or 300 IntTI whichever is smaller. 2) The horizontal distance between parallel reinforcement bars provided against shrinkage and temperatureshall not be more than five times the effective depth of a solid slab or 450 mm whichever is smaIJer. 26.4 Nominal Cover to Reinforcement 26.4.1 Nominal Cover Nominal cover is the design depth of concrete cover to all steel reinforcements, including links. It is the dimension usedindesignand indicatedin the drawings. It shall be not less than the diameter of the bar. 26.4.2 Nominal Coverto MeetDurability Requirement Minimum values for the nominal cover of normalweight aggregate concrete which should be provided to all reinforcement, including links depending on the condition of exposure described in 8.2.3 shall be as given in Table 16. 26.4.2.1 However for a longitudinal reinforcing bar in a column nominal cover shall in any case not be less than 40 mm, or less than the diameter of such bar. In the case of columns of minimum dimension of 200 mm or under,whose reinforcing bars do not exceed 12mm, a nominal cover of 25 mm may be used. 26.4.2.2 For footings minimumcover shall be 50 mm. 26.4.3 Nominal Cover to Meet Specified Period of Fire Re..sistance Minimum values of nominal cover of normal-weight aggregateconcrete to be provided to all reinforcement including links to meet specified period of fire resistance shall be given in Table 16A. 26.5 Requirements of Reinforcement for Structural Members 26.5.1 Beams 26.5.1.1 Tension reinforcement a) Minimum reinforcement-The minimum areaof tensionreinforcementshall be not less than that .... Table 15 Clear Distance Between Bars tCtause 26.3.3) f). Percentage Redistribution to or from Section Considered -10 0 - 15 +I~ +30 Clear Distance Between Ban NIJnln2 nun mm mm mm mm 2~() 215 260 300 300 300 415 12~ 15~ 180 210 235 500 105 130 150 17S 195 N()TE - The spacingsgiven in the tableare not applicable to members subjectedto particularly agressive environmentsunlessin the calculation of'themoment of resistance, I., hasbeenlimited to300N/mm2 inlimitstartdesian ond alii limited to 16' N/mm2 in workin, stress design. 46 IS 456: 2000 Table 16 Nominal Cover to Meet Durability Requirements iClause26.4.2) Exposure Nominal Cencrete Cover In mm not Leu Than Mild 20 Moderate 30 Severe 45 Very severe 50 Extreme 75 NOTES 1 For main reinforcementup to 121nnldiameter bar for nliJd exposure the nominalcover may be reduced by 5 mm. 2 Unless specifiedotherwise. actual concretecover should not deviate from the requirednominalcover by + I 0 mm o 3 For exposurecondition'severe' and 'very severe'. reduction of 5 mm Inf:lY he made.whereconcretegrade is M35 and above. Table 16A Nominal Cover to Meet Specified Period of Fire Resistance iClauses 21.4 and 26.4.3 and Fig. I) ... Fire Resis- Nominal Cover Beams tance Ribs Slabs Columns Simply supported Continuous Simply supported Continuous Simply supported Continuous mm mm nun rnrn mm mm o.s 20 20 20 20 20 min 20 I 20 20 20 20 20 20 40 h 40 1.5 20 20 25 20 ~ 20 40 2 ~ 30 .:u 25 4S J.1 40 3 60 70 ~ .ll 5S 65 45 55 40 40 4 50 45 55 45 NOTES 1 The nominal covers liven relate specificallyto the minimummemberdimensionsgiven in Fig. I. 2 Casesthatlie below tbe boldlinerequireattention to the additional measures necessary to reducetherisksof spallingisee 21.3.1). given by the following: ~ = 0.85 fy bd A. = minimum area of tension reinforcement, = breadthof beamor the breadthof the web of 'f-beam. d f, Wherethedepthof the web in a beamexceeds750 mm, sidefacereinforcement shall be providedalongthe two faces. The total area of such reinforcement shall be not less than 0.1 percent of the web area and shall be where b 26.5.1.3 Side face reinforcement = effective depth, and = characteristic strengthof reinforcement in N/mm2• b) Maximum reinfo~eme",- The maximum area of tension reinforcement shall not exceed 0.04 bD. distributed equally on two faces at a spacing not exceeding 300 111m or web thickness whichever is less. 26.5.1.4 Transverse reinforcement in beamsfor shear and torsion The transverse reinforcement in beams shall be taken around the outer-most tension and compression bars. "In T-beams and f-beams, such reinforcement shall pass aroundlongitudinal barslocatedclose to the outer face of the flange. 26.5.1.2 Compression reinforcement 26.5.1.5 Maximum spacing ofshear reinforcement The maximum area of compression reinforcement shall not exceed 0.04 bD. Compression reinforcement in beams shall be enclosed by stirrups for effective lateral restraint. The arrangementof stirrups shall be The maximum spacing of shear reinforcement measured alongtheaxisof the membershallnotexceed 0.75 d for vertical stirrups and d for inclined stirrups at 45'\ where d is the effective depth of the section as specified in 26.5.3.2. 47 15456:2000 under consideration. 1ft no case shall the spacinl exceed 300 mm. 26.5.1.6 Minim"". ,ltear rein/orreNnt Minimum shear reinforcement in the form of stinups shall be providedsuch that: where AI. • total cross-sectional area of stirrup lop effective in shear. '. • stirrup SPacinl alonl tho Ieft8th of the member. b =- breadth of the beam or breadth of the I., • 26.5.2Slab, The rules liven in 36.1.2..1 and ZU.2.2 shall apply to slabs in addition to those ,twn in the appropriate clauses. 25.1.11 Minimwn "injorceIMnt Themild lteel reinforcemeat III lither tlli'ectidtl ill~tatil shall not be loa thin 0,IS~ftt " ' . ro\8l crosssectional .... Ho. . . tilt WI'Ue can bereduced to 0.12 peneIlt ~hen biSb strength deformed bars or welded wire fabric are used. 26.5.12 Mtuimum diGm't~r Thediameter of reinforciq banaball bOte~ ODe4(. eisht of the total thicblu of 1M .a.b. web of ftanled beam. and 26.5.3 Col...,., characteristic ItreDltb of the stirrup reinforcement in N/mm2 which shallnot be taken pater dian 415 N/mm2• 26.5.11 ~ reinforcement I) The cross-sectional area of lonaitudinal reinforcement, shall be not less than 0.8 pIIIIftl nor moro than 6 percent of the ~ sectional area of the column. aro.' ••. Where the maximum shearstresscalculated illels than half the permissible value and in memben of minor structural importance such u lintels. this provision need not be compliedwith. .VoIve NOTB-"' . . of6,... Ninf........ may prlCticai dtftlcultiel in pladnl-lDIbp8cdD. of ~; hence 10. . perceMII* I. Neommencled. WhentMn ~ the col_ below have to be . . . . . . . \'fmc in the column uDder eoDli~ . . peltentaae of steellhlll Z6.5.1.7 Distributioll oftorsto« Teinfol'C~nielll When a member is desilned for toni on (,~, 41 or 8-6) tonion reinforcement shall be providedu below: aUllI, DOlex~ 4 perce•. b) In any column that bas a IUJer cross-sectional a) The transverse reinforcement for tonion sball be rectanplar closed stirrups placed perpendicular to the WS of the member. The spacinl of the stirrup. shall not exceed the leaJt of .I., .I,:" and 300 mm, whele .I. and,. area than that required to support the load~ the minimum percenta,e of steel Ihall be bued upon the area of concrete requlNCl to resist the direct stress and Dot upon the actual area. c) The minimum number of loqil\kllftal ban provided in • column IbIIl be four in rectaDplar columns and six illcircullr columns. IR reapectively the short and lonl dimension. of the ltimap. b) Lonptudinal reinforcement shall be placed .. close asis practicable to the cornen oftbe croa.. section and in all casea, there shall be at leat one IonJitudinai bar in eachcom. of the tiel. When the croll-sectional dimension of the d) The bars shall not be less than 12 mm in diameter. e) A reinforced concrete column havinl helical reinforcement shall have at leut lix bin of lonlitudinal reinforcement within tho helical reinforcement. f) Ina helically _fmeed column. the lonptudinal bars shall be in contact with the helical reinforcement and equidistant around its inner member exceeds 450 mm, additional longitudinal bars.shall beprovided to satisfy the requirementl of minimum reinforcement and spacinl givenin 26.5.1.3. circumference. s) ·Spacina of lonptudinal bars meuured alonl the periphery of the column shall not exceed 26.5.1.8 Reinforcement in OanlOS of T-n L-beams shall satisfy the requirements in 23.1.1(b). Where tlaDles in teuioD, • part of the main tension reinforcement shall be dillribuled over the effective flanle width or a width equal to ~tonth of the span. whichever is smaller. If the effective flanle width exceeds one-tenth of the span, nominal lonaitudinal reinforcement shall be provided in the outer portions of the flap. are 300mm. h) In case of pedeStall in which the IORlitudinal reinforcement is Dot takeD in account instrenath calculations, nominaIlonptudinai reinforcement notless. than0.15 percentof thecross-sectional area' shall be provided. 48 IS 456: 2000 NOTE - Pedestal is a compreuion member. the effective lenlthof which does notexceed three time.theleast lateral reinforcement need not. however, exceed 20 mm (see Fig. 11). dimension. c) Pitch anddiameter of laura;tits 26.5.3.2 Transverse reinforcement a) General-A reinforced concrete compression J) Pitch-The pitch of transverse reinforce- mentshall be not more than the least of the following distances: member shall have transverse or helical reinforcement so disposed that every longitudinal bar nearest to the compression face has effective lateral support against buckling subjectto provisions in (b). Theeffective lateral support is given by transverse reinforcement either in the fonn of circular rings capable of taking up circumferential tension or by polygonal links(lateral ties)withinternal angles not exceeding 13.50 • The ends of the transverse reinforcement shall be properly anchored [see 26.2.2.4 (b)]. b) The least lateral dimension of the compression members; ii) Sixteen times the smallest diameterof thelongitudinal reinforcement bar to be tied: and iii) 300 mm. i) 2) Diameter-The diameter of the polygonal links or lateral tiesshall be notlessthanonefourth of the diameter of the largest longitudinal bar. and in no case less than Arrangement of transverse reinforcement 16mm. 1) If the longitudinal bars are not spaced more than 75 mm on either side. transverse reinforcement needonlyto go roundcorner and alternate bars for the purpose of providing effective lateral supports (set Fig. 8). 2) If the longitudinal bars spaced at a distance of not exceeding 48 times the diameter of the tie are effectively tiedin twodirections. additional longitudinal barsinbetween these barsneedto be tiedin onedirection by open ' ties (see Fig. 9). 3) Where the longitudinal reinforcing bars in a compression member are placedin more thanonerow, effective lateral support to the longitudinal bars in the inner rows may be assumed to have been provided if: i) transverse reinforcement is provided for the outer-most row in accordance with 26.5.3.2, and 1) Pitch-Helical reinforcement shall be of regular formation with the turnsof the helix spaced evenly and its endsshall be anchored properly by providing one and a half extra turns of the spiral bar. Where an increased load on the column on the strength of the helical reinforcement isallowed for, thepitch of helical turnsshall benotmore than75mm, normorethanone-sixth of thecorediameter of thecolumn. norless than2.5 mm, norless thanthreetimesthediameter of the steelbar forming the helix. .In other cases, the requirements of 26.5.3.2 shall be complied with. 2) The diameter of the helical reinforcement shall be in accordance with 26.5.3.2(c) (2). 26.5.3.3 Incolumns where longitudinal barsareoffset at a splice, the slopeof the inclined portion of the bar with the axis of the column shall not exceed 1 in 6. and the portionsof the bar aboveand belowthe offset shall be parallel to the axis of the column. Adequate horizontal support at the offset bends shall be treated as a matterof design. and shall be provided by metal ties, spirals. or parts of the floorconstruction. Metal ties or spirals so designed shall be placed near (not morethaneight-bar diameters from) the pointof bend. The horizontal thrust to be resisted shall be assumed as one and half times the horizontal components of the nominal stress in the inclined portion of the bar. Offsetbarsshall be bentbefore they are placedin the forms, Where column faces areoffset75mmormore, splices of vertical barsadjacent to theoffsetfaceshall be made by separate dowels overlapped as specified in 26.2.5.1. ii) no bar of the inner row is closer to the nearest compression face than three times the diameter of the largest bar in the inner row (see Fig. 10). 4) Where the longitudinal bars in a compression member are grouped (not in contact) andeachgroup adequately tiedwith transverse reinforcement inaccordance with 26.5.3.2, thetransverse reinforcement for the compression member as a whole may be provided on the assumption thateachgroup is a single longitudinal bar for purpose of determining the pitch and diameter of the transverse reinforcement inaccordance with 26.5.3.2. The diameter of such transverse 2116 BIS/07-8 d) Helical reinforcement 49 IS 456 : 2000 27.1 Structures in which marked changes in plan dimensions take place abruptly shall beprovided with expansion onjointsat thesection where such changes occur. Expansion joints shall be so provided that the necessary movement occurs with a minimum resistance at the joint. The structures adjacent to the joint should preferably be supported on separate columns or walls but not necessarily on separate foundations. Reinforcement shall not extend across anexpansion jointand thebreak between thesections shall be complete.' 27.2 The details as to the lenith of a structure where expansion joints have to beprovided canbe detennined after taking into consideration various factors. such as temperature, exposure toweather. thetime andseason ofthelaying of the concrete. etc. Normally structures exceeding 45 m in lenith are designed with one or more expansion joints. However in view of the large number of factors involved in deciding the location. spacing and nature of expansion joints. the provision of expansion joint in reinforced cement concrete structures should be left to the discretion of the designer. IS 3414 gives the design considerations, wJtich need to be examined and provided for. Alldimensions In millimetres. Alldimensions Inmlllimetres. Flo. 8 Flo. 9 27 EXPANSION JOINTS TRANSVERSE REINFORCEMENT ... '" 1\\ 'ND'VIDUAL GROUPS Alldimensions in millimetres. FIG. FrG. 11 10 50 IS 456: 2000 SECTION 4 SPECIALDESIGN REQUIREMENTS FOR STRUCTURAL MEMBERS AND. SYSTEMS 28 CONCRETE CORBELS 28.2.4 Resistanceto Applied Horizontal Force 28.1 General Additional reinforcement connected to the supported member should be provided to transmit this force in its entirety. A corbel is a short cantileverprojectionwhichsupports a load bearing member and where: 29 DEEP BEAMS a) . the distance av between the line of the reaction to the supported load and the root of the corbel is less than d (the effective depth of the root of the corbel); and 29.1 General a) A beamshall be deemedto bea deep beam when b) the depth at the outer edge of the contact area of the supported load is not less than one-half of the depth at the root of the corbel. the ratio of effective span to overall depth. ~ is less than: 1) 2.0 for a simply supported beam; and The depth of the corbel at the face of the support is determined in accordance with 40.5.1. 2) 2.5 for a continuous beam. b) A deep beam complying with the requirements of 29.2 and 29.3 shall be deemed to satisfy the provisions for shear. 28.2 Design 28.2.1 Simplifying Assumptions The concrete "and reinforcement may be assumed to act as elements of a simple strut-and-tie system, with the following guidelines: 29.2 Lever Arm The lever arm z for a deep beam shall be detemined a~ below: a) The magnitude of the resistance provided to horizontalforce shouldbe not less than one-half of the design vertical load on the corbel (see also 28.2.4). a) For simply supported beauts: z b) Compatibility of strains between the strut-and.. tie at the corbel foot should be ensured. = 0.2 (I + 2D) when I ~ I - D ~ 2 ~ 2.5 or z = 0.61 It should be noted that the horizontal link requirement described in 28.2.3 will ensure satisfactory serviceability performance. I when - < 1 l) b) For continuous beams. z = 0.2 (I + 1.5 D) 28.2.2 Reinforcement Anchorag« when 1 S - I D or At thefrontfaceof the corbel, the reinforcement should be anchored either by: z =0.5 I / when - < 1 D where / is the effective span taken as centre to centre distance between supports or 1.15 times the clearspan, whichever is smaller, and D is theoverall depth. a) welding to a transverse bar ofequal strength - in this case the hearing area of the load should stop short of the faceof the supportby a distance equal to the cover of the tie reinforcement, or b) bending buck the bars to form a loop - in this case the bearing area of the load should not project beyond the straight portion of thebarsforming themain tension reinforcement, 19.3 Reinforcement 29.3.1 Positive Reinforcement The tensile reinforcement required to resist positive bending moment in any span of a deep beam shall: 18.1.3 Shear Reinforcement a) extend without curtailm-..~r1t between supports; b) be embedded beyond the face of each support, so that at the face of the support it shall have a development length not less than 0.8 LtJ; where L,j is the development length (see 26.2.1). for the design stress in the reinforcement; and Shear reinforcement should be provided in the form of horizontal links distributed in the upper two-third of the effective depth of root of the corbel; this reinforcement should be not less than one-half of the area of the main tension reinforcement and should be adequately anchored. 51 IS 456: 2000 c) be placed within a zone of depth equal to 0.25 D - 0.0' I adjacent to the tension face of the beam where D is the overall depthand I is the effective span. 29.3.2 Negative Reinforc,ment a) Termination of reinforcement - Por tensile reinforcement required to resist negative bending moment over a support ofa deep beam: 1) It shall be permissible to tenninate notmore than half of the reinforcement at a distance of O.~ D from the face of thesupport where D is as defined in 29.2;and 2) The remainder shall extend over the full span. b) Distribution-When ratio of clear span to overall depth is in the range 1.0 to 2.5. tensile reinforcement over a support of a deep beam shall be placed in two zones comprising: ' 1) a zone ofdepth0.2D. adjacent to the tension face. which shallcontain a proportion of the • . tension steel given by O.S where (~ - o.s) = = 2) I clearspan. and D overall depth. a zone measuring 0.3 D on either side of the mid-depth of the beam, which shall contain the remainder of the tension steel, evenly distributed. For spantodepthratios lessthanunity. the steel shall be evenly distributed over a depthof 0.8 D measured from the tension face. 29.3.3 Vertical Reinforctmt1l1 If forces are applied to a deepbeam in sucha way that hanging action is required. barsor suspension stil'NPS shallbe provided to carry all the forces concerned. 19.3.4 Side Face Reinforcement Side face reinforcement shall comply with require.. ments of minimum reinforcement of walls (ste 32.4). 30 RIBBED. HOLLOW BLOCK ORVQIDEDSLAB 30.1 General This covers the slabs constructed in one of the ways described below: a) As a aeries of concrete ribswithtoPPinlcaston forms which may be removed aftertheconcreto has set; b) As a series of concrete .ribs between precast blocks which remain part of the completed ItNcture; the top of the ribs may be connected by a toPpinlofconcrete of thesame strenath as that usedin the ribs; and c) With a continuous top and bottom face but containing voids of rectangular, oval or othershape. 30.2 Analysis or Stnacture The moments and forces due to desian loads on continuous slabs maybeobtained by themethods liven in Section 3 for solid slabs. Alternatively, the slaba may be designed as a seriesof simply supported spans provided they arenotexposed to weather or corrosive conditions; wide cracks may develop at the supports and the engineer shall satisfy himselfthat these will not impair finishes or lead to corrosion of the reinforcement. 30.3 Shear Where hollow blocks are used, for the purpose of calculating shear stress. the rib width may be increased to takeaccount of the wan thickness of the block ononesideof therib; with narrow precast units. the width of the jointing mortar or concrete may be included. 30.4 Deflection Therecommendations fordeflection inrespect of solid slabs maybeapplied toribbed. hollow blockor voided construction. Thespan to effective depthratiosliven in 23.2 for a flanged beam are applicable but when calculating the final reduction factor for web width. the rib width for hollow blockslabs may be assumed to include the walls of the blocks on both sidesof the rib. For voided slabsand slabsconstructed of box or I-section units. aneffective ribwidth shall be calculated assumins all material below the upper flange of the unitto be concentrated in a reetanaular rib hlvins the same cross-sectional areaand depth. 30.5 Sizeand Poeltlonof Rib•. In-situ ribs shall be not less than 65 mm wide. They shall be spaced at centres not greater than 1.~ apart and their depth. excluding any topping, shall be not more thanfour times their width. Generally ribs shall be formed alons eachedge parallel to the spanof one way slabs. Whenthe edge is built into a wall or rests on a beam, a ribat leastas wideas the bearing shall be fonned alons the ed,e. m 30.6 Hollow Blocks and Formen Blocks and fonners may be of any suitable material. Hollow clay tiles for the filler type shall conform to IS 39~ 1 (Part I). When required to contribute to the IS 4S6: 2000 structural strengthof a slab they shall: a) be made of concrete or burnt clay; and b) have a crushins strength of at least 14 N/mm2 measured on thenetsection when axially loaded in the direction ofcompressive stressin theslab. toll' measured centre to centre of supports. b) Middl~ strip - Middle stripmeans a desisn strip bounded on each of its opposite sides by the column strip. c) Panel-« Panel means that part of a slabbounded on each of its four sides by the centre-line of a columnor centre-lines of adjacentspans. 30.' ArraDlemeDt of Reinforcement The recommendations liven in 26.3 resardinl maximum distance between bars apply toareas ofsolid concrete inthisfonn ofconstruction. Thecurtailment. anchorage and cover to reinforcement shall be as described below: a) At least SO percent of the total main reinforcement shall be carried through at the bottom on to the bearinl and anchored in accordance with 36.2.3.3. b) Wherea slab.which iscontinuous oversupports, has been designed as simply supported, reinforcement shallbeprovided overthesupport to control cracking. This reinforcement shall have a cross-sectional area of notless thanonequarter that required in the middle of the adjoining spans and shall extend at least onetenth of the clear span into adjoining spans. c) In slabs with pennanent blocks, the side cover to the reinforcement shall not be less than 10 mm. In all other cases. cover shall be provided according to 26.4. 31.2 Proportlonlnl 31.2.1 Thickness of Flat Slab The thickness of the flat slab shall be generally controlled by considerations of spanto effective depth ratios given in 23.2. For slabs with drops conforming to 31.2.2. span to effective depth ratios liven In 23.2 shall be applied directly; otherwise the span to effective depth ratios obtained in accordance with provisions in 23.2 shall bemultiplied by0.9. For this purpose. thelongerspan shall be considered. The minimum thickness of slab shall be 12S mm. 31.2.2 Drop The drops whenprovided shall be rectangular in plan. and have a lengthin each direction not less than onethirdof the panellengthin thatdirection. For exterior panels. the width of drops at right angles to the noncontinuous edgeandmeasured from thecentre-line of the columns shall be equal to one-half the width of drop for interiorpanels. 30.8 Precuts Joists and HoUow Filler Blocks 31.2.3 Column Heads The construction with precast joists and hollow concrete filler blocks shall conform to IS 6061 (Part 1) and precastjoist and hollowclay filler blocksshall confonn to IS 6061 (Part 2). Where column heads are provided, that portion of a column head which lies within thelargestrightcircular cone or pyramid that has a vertex angleof 90°and can be included entirely within the outlines of the column and the column head, shall be considered for design purposes (Stt Fig.12). 31 FLATSLABS 31.1 General 31.3 DetermlnatioD of Bendinl Moment The term flat slab means a reinforced concrete slab 31.3.1 Methods 01 Analysis and Desig" It shall be pennissiblc to design the slab system by one of the following methods: a) The direct design method as specified in 31.4. and b) The equivalent frame method as specified in 31.5. In each case the applicable limitations given in 31.4 and 31.S shall be met. with or without drops. supported generally without beams. by columns with or without flared column heads (see Fig. 12). A flat slab may be solid slab or may haverecesses fonnedon the softlt ~o thatthe soffit comprises a series of ribs in two directions. The recesses may be fonned by removable or permanent filler blocks. ' 31.1.1 For the purpose of this clause, the following definitions shall apply: . a) Column strip - Column strip means a design strip having a width of 0.2S ' 2, but not greater than 0.25 'ion each side of the columncentreline, where I. is the span in the direction moments are beingdetermined, measured centre tocentreof supports and' 2 is thespantransverse 31.3.2 Benc#ng Moments in Panels with Marginal Beams or Walls Wherethe slab is supported by a marginal beam with a depthgreaterthan 1.5timesthe thickness of the slab. or by a wall, then: S3 IS 456 : 2000 ....-~........--r- CRITICAL SECTION 'OR SHUR IMMfDIATlLY ADJACENT TO COLUM 12A SLAB WIT Hour DROP & COLUMN WITHOUT COLUMN HEAD CRITICAL SECllON FOR SHEAR 12 B SLAB WITH DROP & COLUMN WITH COLUMN HEAD , ,--I'. ,,' /" ANY CONCRITE IN THIS ARIA TO BE NEGLECTED IN THE CALCULATIONS 12 C SLAB WITHOUT DROP" COL UMN WITH COLUMN HEAD NOTE - D. is the diameterof column or column head to be considered for desi... and d ia effective depth of alab or drop II IIpproprillte" FlO. 12 CRJ11CAL SEC110NS FOR SHEAR IN FLAT SLABS a) the total loadto be carried by the beamor wall shall comprise those loadsdirectly on the wall or beam plusa uniformly distributed loadequal to one-quarter of thetotalloadon theslab,and b) the bending moments on the half-column strip adjacent to the beam or wall shall beone-quarter of the bending moments for the fll'St interior column strip. 31.3.3 Transfer of Bending Moments to Columns When unbalanced gravity load, wind, earthquake, or otherlateral loadscausetransfer of bending moment between slab and column, the flexural stresses shall be investigated using a fraction, a of the moment given by: 1 a-~ -l+~ aJ 3 fa, where a. = overall dimension of tile critical section a2 for shear in the direction in which moment acts,and overall dimension of the critical section for shear transverse to the direction in which moment acts. = A slab width between linesthatare one andone-half slab or drop panel thickness; 1.5 D, on each side of thecolumn or capital may be considered effective, D being the size of thecolumn. Concentration of reinforcement overcolumn headby closer spacing oradditional reinforcement may beused to resist the moment on this section: 31.4Dlreet Destp Method 31.4.1 Limitations Slabsystem designed bythedirect design method shall fulfil the following conditions: a) There shall be minimum of three continuous spans in eachdirection, b) Thepanels shallbe rectangular, and the ratioof the longer span totheshorter spanwithin a panel shallnot be greater than2.0, c) It shall be permissible to offsct columns to a maximum of 10 percent of the span in the direction of the offset notwithstanding the provision in (b), d) The successive span lenllhs in each direction shall not differ by more than one-third of the longer span. The end" spans may be shorterbut not longer than the interior spans, and IS 456: ZOOO Exteriornegative designmoment: e) The deSiSD liveloadshallnotexceedthreetimes the desian dead load. --.O.6S 31.4.2 Total Design Moment/ora Span 1+- ac 31.4.11 In the direct desip method, the total design moment for a span shall be determined for a strip bounded laterally by the centre-line of the pane) on eachsideof the centre-line of the supports. 31.4.2.2 The absolute sumofthepositive andaverase ne,ative bendina momenta in each direction shall be takenu: Win Mo · 8 a c is the ratio of flexural stiffness of the exterior columns to the flexural stiffness of the slab at a joint taken in the direction moments are being determined and is liven by EX a • =:.a. s, = sum of the flexural stiffness of the columnsmeetingat thejoint; and K. = flexural stiffness of the slab, expressed as moment per. unit rotation. = total moment; W = design load on an area '2 '.; M" In = clearspan extending from face to face of '2 31.4.3.4 It shall bepermissible to modify thesedesign moments by up to 10percent. so 10nlas the totaldesign moment, M., for the panel in the direction considered is not less than that required by 31.4.1.1. columns, capitals, brackets or walls, but not less than 0.651.; length of span in the direction of Mo ; and = length of span transverse to ' r 31.4.3.5 The negative moment section shall be designed toresist the IB1Jcr of the twointerior negati ve design moments determined for the spans framing into a common support unless an analysis is made to distribute the unbalanced momentin accordance with the stiffness of the adjoining parts. 31.4.2.3 Circular supports shall be treated as square supportshaving the same area. 31.4.Z.4 When the transverse span of the panels on eitherside of thecentre-line of supports varies, 12 shall be taken as the averageof the transverse spans. 31.4.Z.5 Whenthespan adjacent and parallel to anedge is being considered, the distancefrom the edge to the centre-line of the panel shan be substituted for lz in 31.4.2.2. 31.4.4 Distribution of Bending Mo~,.ts Across the Panel Width Bending moments at critical cross-section shall be distributed to the column strips and middle strips as 31.4.3 Negativ« and Positive DesignMoments specified in 31.5.5as applicable. 31.4.3.1 The negative desiBn moment shall be located at the face of rectangular supports, circular supports being treated as square supports having the same area. 31.4.3.2 In an interior span, the total design moment Mu shall be distributed in the following proportions: 0.65 Negativedesign moment Positivedesign moment 0.35 31.4.5 Moments in Columns 31.4.5.1 Columns builtintegrally withthe slabsystem shall bedesigned to resistmoments arisingfrom loads on the slab system. 31.4.5.1 At an interior support, the supporting members above and below the slab shall be designed toresistthe momeat M givenby thefollowing equation, indirectproportion to theirstiffnesses unless a general analysis is made: 31.4.3.3 In an end span, the total design moment M" shall be distributed in the following proportions: Interior negativedesign moment: 0.7S _ O.l~ 1+- M =O.OS (W d +O.Sw, )111: -w~ 1 I; I:' 1+al: at where Positivedesign moment: Wei' WI 0.63- • where where 'I = K e O.2~ '2 1+ac = design dead and live respectively, per unit area; = length of span transverse to the direction of M; 5S loads IS 456: 2000 I. = ac = w;.I'l b) Eachsuchframe maybeanalyzed in itsentirety, or, for vertical loading, each floor thereofand the roof may be analyzed separately with its columns being assumed fixed at their remote ends. Where slabsarethusanalyzed separately, it may be assumed in determining the bending moment at a givensupport thattheslab is fixed at any support two panels distant therefrom provided the slab continues beyond the point. c) For the purpose ofdetermining relative stiffness of members. the moment of inertiaof any slab or column may be assumed to be that of the gross cross-section of the concrete alone. d) Variations of moment of inertiaalong the axis oftheslabonaccount of provision ofdropsshall be taken into account. In the case of recessed or coffered slab which is made solid in the region of thecolumns. thestiffening effectmay be ignored provided the solid part of the slab doesnotextendmorethan0.15 'eI' intothespan measured from the centre-line of the columns. Thestiffening effect offlared column heads may be ignored. length of the clear span in the direction of M, measured face to face of supports; IK --&'I' where Kc and K. areas defined K. in 31.4.3.3; and and I:. referto the shorterspan. 31.4.6 Effects of Pattern Loading In thedirectdesign method. when theratioof liveload to dead loadexceeds O.S : a) thesumoftheflexural stiffnesses of the columns above and below the slab. IKe' shall be such that ex. is notlessthantheappropriate minimum value ex. IltIa specified in Table t 7. or b) if the sum of the flexural stiffnesses of the columns. IKe' does not satisfy(a). the positive design moments for the panelsball bemultiplied by the coefficient P. given by the following equation: 31.5.2 Loading Pattern 31.5.2.1 When the loading pattern is known. the structure shall be analyzed for the load concerned. ex. is theratioof flexural stiffness of thecolumns above and below the slabto the flexural stiffness of theslabs at a joint taken in the direction moments are being determined and is givenby: Table17Minimum PermissibleValues of exc (Clause 31.4.6) ImpoHd LoadIDelld Load ex = IKe: c (1) IK • where Kc and K. are flexural stiffnesses of column and slab respectively. 31.5 Equivalent Frame Method 31.5.1 Assumptions The bending moments and shear forces may be determined by an analysis of the structure as a continuous frameand the following assumptions may be made: a) The structure shall be considered to be madeup of equivalent frames on column lines taken longitudinally and transversely through the building. Each frame consists of a row of equivalent columns or supports, bounded laterally by the centre-line of the panelon each side of the centre-line of the columns or supports. Frames adjacent'and parallel to anedge shall be bounded by the edge and the centreline of the adjacentpanel. Ratlo~ VII. ora.... (2) (3) II O.S O.S to 2.0 o 1.0 1.0 1.0 1.0 1.0 2.0 2.0 2.0 2.0 2.0 3.0 3.0 3.0 3.0 3.0 0.5 0.6 0,8 0.7 0.7 0.8 1.0 1.25 2.0 O.S 0.8 1.0 1.2S 2.0 0.5 0.8 1.0 1.25 2.0 1.2 1.3 1.5 1.6 1.9 4.9 1.8 2.0 2.3 2.8 13.0 31.5.2.1 When the live load is variable but does not exceed three-quarters of the dead load. or the nature of the live load is such that all panels will be loaded simultaneously, the maximum moments may be assumed to occurat all sections whenfull design live loadis on the entireslab system. S6 IS 456: 2000 31.5.2.3 For other conditions of live load/dead load ratioand when all panelsare not loadedsimultaneously: greater than three-quarters of the value of 12, the length of span transverse to the direction moments are being determined, the exterior negative moment shall be considered to be uniformly distributed across the length 31.5.5.3Column strip: Positivemomentforeach span a) maximum positive moment near midspan of a panel may be assumed to occur when threequarters of the full design live load is on the panel and on alternate panels; and '2' b) maximum negative moment in the slab at a For each span. the column strip shall be designed to resist 60 percent of the total positive moment in the panel. support may be assumed to occur when threequarters of the full design live load is on the adjacent panels only. 31.5.5.4 Moments in the middle strip 31.5.1.4 In no case shall design moments be taken to be less than those occurring with full design live load on all panels. The middle strip shall be designed on the following bases: a) That portion of the design moment not resisted by the column strip shall be assigned to the adjacent middle strips. b) Each middle stripshall be proportioned to resist the sum of the moments assigned to its two half middle strips. c) The middlestrip adjacentand parallelto an edge supported by a wall shall be proportioned to resist twice the moment assigned to half the middle strip corresponding to the first row of interior columns. 31.5.3Negative Design Moment 31.5.3.1 At interior supports, the critical section for negative moment, in both the column strip and middle strip, shall be taken at the face of rectilinear supports, but in no case at a distance greater than 0.175 II from the centre of the column where II is the length of the span in the direction moments are being determined, measured centre-to-centre of supports. 31.5.3.2 At exterior supports provided with brackets or capitals, the critical section for negative moment in the direction perpendicular to the edge shall be taken at a distance from the face of the supporting element not greater than one-half the projection of the bracket or capital beyond the face of the supporting element. 31.5.3.3 Circular or regular polygon shaped supports shall be treated as square supports having the same area. 31.6 Shear in Flat Slab 31.6.1 The critical section for shear shall be at a distance d/2 from the periphery of the column/capital/ drop panel,perpendicular to the planeof the slab where d is the effective depth of the section (see Fig. 12). TIle shapein plan is geometrically similarto the support immediately below the slab (see Fig. 13A and 13B). NOTE - Forcolumn sections withre-entrant angles. thecritical section shall be takenas indicated in Fig. 13Cand 130. 31.5.4 Modification ofMaximum Moment Moments determined by means of the equivalentframe method, for slabs which fulfil the limitations of 31.4 may be reduced in such proportion that the numerical sum of the positive and average negative moments is not less than the value of total design moment M" specified in 31.4.2.2. 31.6.1.1 In the case of columns near the free edge of a slab, the critical section shall be taken as shown in Fig. 14. 31.6.1.~ When openings in flat slabs are located at a distance less than ten times the thickness of the slab from a concentratedreaction or when the openings are located within the column strips. the critical sections specified in 31.6.1 shall be modified so that the part of the periphery of the critical section which is enclosed by radial projectionsof the openings to the centroid of the reaction area shall be considered ineffective (.\"ee Fig. 15), and openings shall not encroach upon column head. 31.5.5 Distribution of Bending Moment Across the Panel Width 31.5.5.1Columnstrip: Negativemomentat an interior support At an interior support, the column strip shall be designed to resist 7S percent of the total negative moment in the panel at that support. 31.5.5.2 Column strip:Negative momentatanexterior support a) At an exterior support. the column strip shall be designed to resist the total negative moment in the panel at that support. b) Where the exterior support consists of a column or a wall extending for a distance equal to or 2116 815/07-9 31.6.2 Calculation ofShear Stress The shear stress tv shall be the sum of the values calculated according to 31.6.2.1 and 31.6.2.2. 31.6.2.1 The nominal shear stress in flat slabs shall be takenas V I b d where V is the shear forcedue to design load, bit is th~) periphery of the critical section and d is the effective depth. 57 15456: 2000 r-------l 'a:': '';', ': . . .. t: ••::' . . II ~~. '; :~: I • I , •• ' CRITICAL SECTION I .. L_ I SUPPORT d/2 ~tT SUliPORT SECTION COLUMN ICOLUMN HEAD 13A SUPPORT SECTION rr-, -l. d/2 SUPPORT SECTION CRITICAL SECTION [ I ., ,'..•: ) d/2 ;...... ""'.' • I •.1"" ~:~":'.,~ . r :.. ~I . I d/2 L - ;i;-1 '4 \. " "." t NOTE - d i. the effec:tive depthof the nat slab/drop. FlO. 13 CarneAL SScnONS IN PLAN FOR SHEAR IN fLAT SLABS FREE CORNER ~'ReE L.-r eDGE I I I I I ~.' •••'. . "".~. 'VCRITICAL seCTION :~· .... •. ~:~~ ;. ~~ ; ~," ...... ' I ~__ d/2 L __ ~ _ ~/~-- T CORNeR COLUMN CRITICAL SeCTION 148 " A Fro. 14 EFFEcr OF FRBB BOOBS ON CRrneAL SBC110N FOR SHEAR 31.6.2.2 When unbalanced gravity load, wind, earthquake or other fo~s cause transferof bending moment betweenslab and column. a fraction (I - ex) of the moment shall be considered transferred by eccentricity of the shear about the centroid of the critical section. Shearstresses shall betaken all varying linearly about the centroid of the critical section. The value of a shall be obtained from the equation given in 31.3.3. 31.6.3 Permissible ShearStress 31.6.3.1 When shear reinf~ment is not provided. the calculated shearscress at the critical section shall not exceed k."C~. S8 IS 4~6: 2000 .......---4M-- OPENING SUBTRACT FROM PERIPHERY r-I i , II COLUMN OPENING COLUMN ..L d/2 , . - - - :':~:~' . :~~:; ~~~'J~~~~ j ..................11I6 J : «n en r ~tr , i L I I :'-CRITICAL I SECTION I ''''·.~~:.~''':-+-AI 0'-'·".' L I 1 I , __.II - - 15 A 158 PENlNG ,, I I I I I I I , t I ...- I , : CRITICAL SECTION Il.. ~, ,. · : ..•.. ; . . 0 ..' I T -- ~ oj, • ':'." "..: il~:· '!: ~. COLUMN I "--CR ITICAL I SECTION JI "---- ...--..J • REGARD OPENING AS FREE EDGE 1St 15 D FlO. 15 EFFECf OF OPENINGS ON CRmCAL SEmON FOR SH£AR where k. 2 times the slab thickness, except where a slab is of cellular or ribbed construction. =(O.S + Pc) but not greaterthan 1, Pc beingthe ratio of shortside to longside of the column! capital; and tt 31.7.1Area ofReinforcement When drop panels ~ used. the thickness of drop panel for determination of areaof reinforcement shall be the lesserof the following: a) Thickness of'drop, and b) Thickness of slab plus one quarter the distance between edge of drop and edge pf capital, 31.7.3 Miniml4nl Length ofReinforcement a) Reinforcement in flat slabs shall have the minimum lengths specified in Fig.16. Larger lengths of reinforcement shallbe provided when required by analysis. b) Where adjacent spans are unequal. theextension of negative reinforcement beyond each face of the common column shall be based on the longer span. e) The lengthof reinforcement for slabs in frames not braced against sideways and for slabs resisting lateral loads shall be determined by analysis but shall not be less than those prescribed in Fig. 16. =0.25 [l;; in limit state method of design, and 0.16 [l;; in working stress method of design. 31.6.3.2 When the shear stress at the critical section exceeds the value given in 31.6.3.1, but less than 1.S 1:( shear reinforcement shall be provided. If the shear stress exceeds I.S 1 c the flat stab shall be t redesigned. Shear stresses shall be investigated at successive sectionsmoredistantfromthe supportand shear reinforcement shall be provided up to a section where the shear stress does not exceed 0.5 t c . While designing the shear reinforcement, the shear stress carried by the concreteshall be assumed to be 0.5 t~ and reinforcement shall carry the remaining shear. 31.7 Slab Reinforcement 31.7.1 Spacing The spacing of bars in a flat slab, shall not exceed S9 IS4S6: 2000 MINIMUM -~ oe lteE" ! r~ ""; 0'..ltIItCENt... .. ~ ..A ...t 10 ~ ~ ; i WitHOUT DftOft .....NIL .IC1I0N RIMA.NOIR ----:-+-~~~~-H t-t------t-ir:t-r- !I II ~jIII~c., !~ -.....c== OP r-C-~~ '1.~ ~·l--c-4 jill, I-c- , H----lr-:--:-:--------J.-t--::=--------;!'%H •~ ~ I ip , 10 .-"'r I ., ...... c I - tlO "'''' ,. ~ Ir"'" "'''' "'... 'I jill tlO _ _ ~ ...... , --I.'~ / RIMAINDIR 0-.'( "'... ~\. ~ c ... 1-+----l~H----~~--¥f-i-----~---~~ !i a r"+!f-----or" ::t ~ ..o "'''' 10 * =a ..I .......N OIR, " ~ f- ~ "'''' "'... _ - ,,~----PII '10 " ' ' ' ' - ~ C ' I "'''' "'... ~~ f --I s..... N-l,,- ~rCLIAIt '''AN'''.r-'ACE O~ SU ....ORT-" (. I--~A(I Of' SU -_ ~ t." INTllllOII SU .. f"OI'T.... t ~ llCfI"lOIt SU..I"OItT-- t INO SLA. CONTI,,"MVI ICONtlNUITY ....OVOIO. CliO SLA. COHflNUI"" IXT.lll011 SU ....OftT - D I:-CLIAIt ~ BarLength fmm Fac« of SlqIport Minimum Length Muimum Lenath Mark a b c d e J g Length 0.14/, 0.201. 0.22 I. 0.30 I. 0.33/. 0.201. 0.24/. • Bent ban at cllccrior supports may beused if a pneraI analyais is niIde. NOTS..... D is !hediamecer of Cbc column and the di.'IICI\Sion of Cbc rcetanpllr colUlllD in thedinodon. . . COIlIiderltion. FlO. 16 MlNlMUM BENDJOINT LOCAll0NS AND EXTENSIONS POR RmNFoRCBMENT IN FLAT SLABS 60 IS 456: 2000 31.7.4 Anchoring Reinforcement a) All slab reinforcement perpendicular to a discontinuous edge shall have an anchorage (straight, bent or otherwise anchored) past the internal face of the spandrel beam. wall or column, of an amount: 1) Forpositive reirforcement - not less than 150 mm except that with fabric reinforcement having a fully welded transverse wire directly over the support, it shall be permissibleto reduce this length to one-half of the width of the support or SO mm, whichever is greater; and 2) Fornegative reinforcement - such that the design stress is developed at the internal face, in accordance with Section 3. b) Where the slab is not supported by a spandrel beam or wall, or where the slab cantilevers beyond the support. the anchorage shall be obtained within the slab. 31.8 Openings In Flat Slabs Openings of any size may be provided in the flat slab if it is shown by analysis that the requirements of strength and serviceability are met. However, for openings conforming to the following. no special analysis is required. a) Openings of any size may be placed within the middle half of the span in each direction. provided the total amount of reinforcement required for the panel without the opening is maintained. b) In the area common to two column strips, not more than one-eighth of the width of strip in either span shall be interruptedby the openings. The equivalent of reinforcement interrupted shall be added on all sides of the openings. c) In the area commonto one columnstripand one middle strip, not more than one-quarter of the reinforcementin either stripshall be interrupted by the openings. The equivalent of reinforcementinterrupted shall be addedon all sides of the openings. d) The shearrequirements of 31.6shall be satisfied. 32 WALLS as perempirical procedure givenin31.2.The minimum thicknessof walls shall be 100rom. 32.1.1 Guidelines or design of walls subjected to horizontaland verticalloads are given in 32.3. 32.2 Empirical Desllll Method for Walls Subjected to Inplane Vertical Loads 32.2.1 Braced Walls Walls shall be assumedto be braced if they are laterally supported by a structure in which all the following apply: a) Walls or vertical braced elements are arranged in twodirections so as to providelateralstability to the structure as a whole. h) Lateralforcesare resistedby shear in the planes of these walls or by braced elements. c) Floor and roof systems are designed to transfer lateral forces. d) Connections between the wall and the lateral supports aredesignedto resista horizontal force not less than 1) thesimplestaticreactionsto thetotalapplied horizontal forces at the level of lateral support; and 2) 2.5 percent of the total vertical load that the wallis designedto CaJTy at the levelof lateral support. 32.1.2 Eccentricity o/Vertical Load The design of a wan shall take account of the actual eccentricity of the verticalforcesubject to a minimum value of O.OS t. The vertical load transmitted to a wall by a discontinuous concrete floor or roof shall be assumed to act at one-third the depth of the bearing area measured from the span face of the wall. Where there is an in-situ concrete floor continuous over the wall, the load shall be assumed to act at the centre of the wall. The resultant eccentricity of the total vertical load on a braced wall at any level between horizontal lateral supports, shall be calculated on the assumption that the resultanteccentricity of all the verticalloadsabove the upper support is zero. 32.2.3 Max;mrlm Effectiv« Height to Thickness Ratio The ratio of effective height to thickness. Hwelt shall not exceed 30. 31.2.4 Effective Height The effectiveheight of a braced wall shall be taken as follows: a) Where restrained against rotation at both ends 31.1 General Reinforced concrete walls subjected to direct compression or combined flexure and direct compression should be designed in accordance with Section 5 or Annex B provided the vertical reinforcement is provided in each face. Braced walls subjected to only vertical compression may be designed by 61 IS 456: 2000 J) floors 0.75 /1w or 2) intersecting walls or similar members whichever is the lesser. 0.75 [J) h) Where not restrained against rotation at hoth ends by I) floors 1.0 II ow or 2) intersecting walls or similar members whichever is the lesser. 1.0 L1 II \Ii L, :;:; where = shear force due to design loads. ~I d = wall thickness. = n.R >< L~ where L", is the length of the wall 32.4.2.. ] rJndc, no circumstances shall the nominal shear stress r vw m walls exceed 0.17 t; in limit state method and 0 12/. l in working stress method. 32.4.3 Design Shear Strength of' Concrete the unsupported height of the wall, = the horizontal distance between centres The design shear strength of concrete in walls, t n v ' without shear reinforcement shall be taken as below: a) For Hw ILw~ 1 of lateral restraint. =(3,0 -Il K 32.2 . 5 Design Axial Strength. of Wall t(.w 111e design axial strength Pu~ per unit length of a braced wall in compression may be calculated from the following equation: where K1 is 0.2 in limit state method and 0.13 in working stress method. P l 1W = 0.3 (t - Lesser of the ·~';·dlJf:~~ above and .I'ro'lJ where e at TIght i. r w z: angles to the plane of the wall determined in accordance with 32.2.2, and . L'cl]c'Jlafcd from (a') . .... (H .v / I..: ~ J ) .1(., ",: :r\: .:-----,--- .~----.- . -. . . . . (/-'\" / 1.... , _.. , ) where K, ~, p.n4~ in Jir"it "f~~tt' n\(~1hod and 0.03 in workinc st.rt~~.;s method. but shall be e'l :: addi tiona} eccentricity due to sle ndcrness effect taken as /-1 we' I 2 500 t. 32.~~ Lw ) K, b) For I(./L w > J 1.2 e - 2e)fck = thickness of the wall, = eccentricity of load measured w/ not less than K~ ,\;~T~' in allY v.r-c. where K, Walls Subjected to Combined Horizontal is f),l.t; in linut state rnethod and 0.) 0 in and Vertical Forces working stress method. 32.3.1 When horizontal forces are in the plane of the wall. it may be designed for vertical forces in accordance with 32.2 and for horizontal shear in accordance with 32.3. In plane bending may be neglected in case a horizontal cross..section of the wall is always under compression due to combined effect of horizontal and vertical loads. ~~2 . 4.4. Design oJ' Shear Reiniorcemcnt Shear reinforcement shall he provided to carry a shear equal to V "'\;w.t (OJ~ L.. . ).'In case of working stress method Vl1 is replaced by V. The strength of shear reinforcement shall be calculated d~ per 40.4 or B~S.4 with A"" defined as below: l 32.3.2 Walls subjected to horizontal forces A \, oI perpendicular to the wall and for which the design axial load does not exceed 0.04 .f~k Ai' shall be designed as slabs in accordance with the appropriate provisions under 24, where Ait is gross area of the section. - = P (0.8 L w w) t where Pw is determined as follows: a) For walls where Hw ' Ly,:S 1. Pw shall be the Jesser of the ratios of either the vertical reinforcement area or the horizontal reinforcement area to the cross-sectional area of wall in the respective direction. 32.4 Design for Horizontal Shear 32.4.1 Critical Section/or Shear The critical section for maximum shear shall be taken at a distance from the base of O.S Lw or 0.5 H.., whichever is less. b) For walls where HwI Lw > 1, PVi shall he the ratio of the horizontal reinforcement area to the cross-sectional area of wall per vertical metre. 32.4.2 Nominal Shear Stress The nominalshear stress t\lW in wallsshallbe obtained as follows: r yw = Vu / t.d 32.5 Minimum Requirements for Reinforcement in Walls The reinforcementfor walls shall be providedas below: 62 IS 456: 2000 a) the minimum ratio of vertical reinforcement to gross concrete area shall be: be taken as the following horizontal distances: a) Where supported at top and bottom risers by beams spanning parallel with the risers. the distance centre-to-centre of beams; 1) 0.001 2 for deformed bars not larger than 16 mm in diameter and with a characteristic strength of 415 N/mm2 or greater. b) Where spanning on to the edge of a landing slab. which spans parallel, with the risers (see Fig. 17). a distance equal to the going of the stairs plus at each end either half the width of the landing or one metre. whichever is smaller; and 2) 0.001 5 for other types of bars. 3) 0.( :)1 2 for welded wire fabric not larger than 16 mm in diameter, b) Vertical reinforcement shall be spaced not farther apart than three times the wall thickness nor450mm. c) Where the landing slab spans in the same direction as the stairs. they shall be considered as acting together to form a single slab and the span determined as the distance centre-to-centre of the supporting beams or walls. the going being measured horizontally. c) The minimum ratio of horizontal reinforcement to gross concrete area shalt be: 1) 0.002 0 for deformed bars not larger than 16 mm in diameter and with a characteristic strength of 415 Nzmm' or greater. 33.2 Distribution of Loading on Stairs 2) 0.0025 for other types of bars. In the case of stairs with open wells, where spans partly crossing at right angles occur, the load on areas common to any two such spans may be taken as onehalf in each direction a~ shown in Fig. 18. Where flights or landings are embedded into walls for a length of nor less than I 10 mm and are designed to span in the direction of the flight. a 150 mm strip may be deducted from the loaded area and the effective breadth of the section increased by75 mm for purposes of design (see Fig. 19). 3) 0.002 () for welded wire fabric not larger than 16 rntn in diameter. d) Horizontal reinforcement shalt be spaced not farther apart than three times the wall thickness nor 450 mm. NOTE _.'. The minimum remforcement may not always be sufficient to provide adequate resrsrance to the effects of shrinkage and temperature 32.5.1 For walls having thickness more than 200 mm, the vertical and horizontal reinforcement shall be provided in two grids, one near each face of the wall. 33.3 Depth of Section 111e depth of section shalt be taken as the minimum thickness perpendicular to the soffit of the staircase. 32.5.2 Vertical reinforcement need not he enclosed by transverse reinforcement as given in 26.5.3.2 for column. if the vertical reinforcement is not greater than 0.0 I times the gross sectional area or where the vertical reinforcement is not required for compression, 34 FOOTIN(;S 34.1 General 33.1 Effective Span of Stairs Footings shall be designed to sustain the applied loads. moments and forces and the induced reactions and to ensure that any settlement which may occur shall be as nearly uniform as possible. and the safe bearing capacity of the soil is not exceeded (sa IS 1904). The effective span of stairs without stringer heams shall 34.1.1 In sloped or stepped footings the effective 33 STAIRS I I I 1K I I I I ~, ~ I • It- UP i ~x- •x4- GOING (G) ---+'v-i-v-l FIG. 17 x y <1m <1m SPAN IN METRES G·X·Y <1m >'m G.X + 1 >'m <1m G·Y·' >lm >'m G., + 1 ,---. EFfECTIVr-: SPAN FOR STAIRS SUPPORTED AT EACH END IW LANDINGS SPANNING PARALLEL WnH THE RISERS 63 IS 456: 2000 UP .c I 8 E AM ! I I~N , w THE LOAD ON ARE COMMON TO TWO SYSTEMS TO 81£ TAKEN AS ONE HAL,. IN EACH DIRECTION I Flo. 18 LoADINO ON STAIRS WITH OPEN WELLS FlO. 19 LoADINO ONSTAIRS Bun.T INTO WAJ,.LS cross-section in compression shall be limited by tho areaabovethe neutral plane, andtho angle of slopeor depth andlocation of stepsshall besuchthatthe desip requirements aresatisfied ateverysection. Sloped and stepped footings that are designed as a unit shall be constructed to assure action as a unit. where q" • 34.1.2 Thickness at the Edge 01 Footing Inreinforced andplainconcrete footings, thethickness at theedgeshallbe notless than 150mm forfootings on soils, norless than300mmabove the topsof piles for footings on piles. 34.1.3 Inthecaseof plainconcrete pedestals, theangle between the planepassing through the bottom edgeof the pedestal and the corresponding junction edge of the column with pedestal and the horizontal plane (see Fig. 20) shallbe governed by the expression: 34.2 Momenband Fore. 34.1.11n the case of footings on piles, computation for moments and shears may be based on the assumption that the reaction from any pile is concentrated at the centreof the pile. tan a leII. = calculated maximum bearing pressure at the baseafthe pedestal in N/mm2, and characteristic stren,th of concrete at 28 days in N/mm2• 34.2.2 Forthepurpose ofcomputin, stresses infootings which support a round oroctagonal concrete column or pedestal, the face of the column or pedestal shall be taken as the side of a square inscribed within the perimeter oftheround or octagonal column or pedestal. 34.2.3 Bending Moment ~ 0.9pooq" +1 34.2.3.1 The bending moment at any section shall be determined by passing through the section a vertical I.. COLUMN I I PLAIN CONCRETE PEDESTAL Flo. 20 64 IS 456: 2000 plane which extends completelyacross the footing,and computing the moment of the forces acting over the entire area of the footing on one side of the said plane. 34.2.3.2 The greatest bending moment to be used in the design of an isolated concrete footing which supports a column. pedestal or wall, shall be the momentcomputed in the mannerprescribedin 34.2.3.1 at sections located as follows: a) At the face of the column, pedestal or wall, for footings supporting a concrete column, pedestal or wall; 34.3 Tensile Reinforcement The total tensile reinforcement at any section shall provide a moment of resistance at least equal to the bending moment on the section calculated in accordance with 34.2.3. 34.3.1 Total tensile reinforcement shall be distributed across the corresponding resisting section as given below: a) In one-wayreinforcedfooting, the reinforcement extending in each direction shall be distributed uniformly across the full width of the footing; b) Halfway between the centre-line and the edge of the wall, for footings under masonry walls; and h) In two- way reinforced square footing, the reinforcementextending in each direction shall be distributed uniformly across the full width of the footing; and c) Halfway between the face of the column or pedestal and the edge of the gussetted base, for footings under gussetted bases. c) In two-way reinforced rectangular footing. the reinforcement in the long direction shall be distributed unifonnly across the full width of the footing. For reinforcement in the short direction, a central band equal to the width of the footing shall be marked along the length of the footing and portion of the reinforcement determined in accordance with the equation given below shall be uniformly distributed across the central band: 34.2.4 Shear and Bond 34.2.4.1 The shear strength of footings is governed by the more severe of the following two conditions: a) The footing acting essentially as a wide beam, with a potential diagonal crack extending in a plane across the entire width; the critical section for this condition shall be assumed as a vertical section located from the face of the column, pedestal or wall at a distance equal to the effective depth of footing for footings on piles. Reinforcement in central band width 2 Total reinforcement in short direction = ~ + 1 b) Two-way action of the footing, with potential diagonal cracking along the surfaceof truncated where cone or pyramid around the concentrated load; in this case, the footing shall be designed for shear in accordance with appropriate provisions specified in 31.6. is the ratio of the long side to the short reinforcement shall be uniformly distributed in the outer portions of the footing. 34.4 Transfer of Load at the Base of Column 34.2.4.2 In computing the external shearor any section througha footing supportedon piles, the entire reaction from any pile of diameter D (1 whose centre is located D /2 or more outside the section shall be assumed as p:oducing shear on the section; the reaction from any pile whose centre is located Dr/2 or more inside the section shall be assumed as producing no shear on the section. For intermediate positions of the pile centre, the portion of the pile reaction to be assumed as producing shear on the section shall be based on straight line interpolation between full value at D(1/2 outside the section and zero value at DI'/2 inside the section. The compressive stress in concrete at the base of a column or pedestal shall be considered as being transferred by bearing to the top of the supporting pedestalor footing.The bearing pressureon the loaded area shall not exceed the permissible bearing stress in direct cornpression multiplied by a value equal to K but not greater than 2; ~A; where 34.2.4.3 The critical section for checking the development length in a footing shall be assumed at the same planes as those describedfor bendingmoment in 34.2.3 and also at all other vertical planes where abrupt changes of section occur. If reinforcement is curtailed, the anchorage requirementsshall be checked in accordance with 26.2.3. 2116 815/07-10 ~ side of the footing. The remainder of the 65 AI = A2 = loaded area at the column base. supporting area for bearing of footing, which in sloped or .stepped footing may be taken as the area of the lower base of the largest frustum of a pyramid or cone contained wholly within the footing and having for its upper base, the area actually loaded and having side slope of one vertical to two horizontal; and IS 456: 2000 For working stress method of design the permissible bearingstresson fullarea of concreteshall be takenas 0.25!c,,; for limitstatemethodof designthepermissible bearing stress shall be 0.45 let. 34.4.1 Where the permissible bearing stress on the concretein thesupporting or supported memberwould be exceeded, reinforcement shall be provided for developing the excess force, either by extending the longitudinal bars into the supporting member, or by dowels (see 34.4.3). 34.4.2 Where transfer of force is accomplished by reinforcement, the development length of the reinforcement shall be sufficient to transfer the compression or tension to the supporting member in accordance with 26.2. 34.4.3 Extended longitudinal reinforcement ordowels of at least O.S percentof the cross-sectional area of the supportedcolumn or pedestal and a minimum of four bars shall be provided. Where dowels are used, their diameter shall no exceed the diameter of the column bars by more than 3 mm, 34.4.4 Column bars of diameters larger than 36 mm, in compression only can be dowelled at the footings with bars of smaller size of the necessary area. The dowel shall extend into the column. a distance equal to the development lengthof the column bar and into the footing, a distance equal to thedevelopment length of the dowel. 34.5 Nominal Reinforcement 34.5.1 Minimum reinforcement and spacing shall be as per the requirements of solid slab. 34.5.2 The nominal reinforcement for concrete sections of thickness greater than 1 m shall be 360 mmz per metre length in each direction on each face. This provision doesnotsupersede therequirement of minimumtensilereinforcement based on the depth of the section. IS 456: ZOOO SECTION 5 STRUCTURAL DESIGN (LIMITSTATE METHOD) 35 SAFETYANDSERVICEABILITY REQUIREMENTS 35.1 General In the method of design based on limit state concept, the structure shall be designed to withstand safely all loads liable to act on it throughoutits life; it shall also satisfy the serviceability requirements, such as limitationson deflectionand cracking.The acceptable limit for the safety and serviceability requirements before failure occurs is called a 'limit state' . The aim of design is to achieve acceptable probabilities that the structure will not become unfitfor the use for which it is intended, that is, that it will not reach a Iimit state. 35.1.1 All relevant limit states shall be considered in design to ensure an adequate degree of safety and serviceability. In general, the structure shall be designed on the basis of the most critical limit state and shall be checked for other limit states. 35.1.2 For ensuring the above objective, the design should be based on characteristic values for material strengths and applied loads, which take into account the variationsin the materialstrengthsand in the loads to be supported. The characteristic values should be based on statistical data jf available: where such data are not available they should be based on experience. The 'design values' are derivedfrom the characteristic values through the use of partial safety factors, one for material strengths and the other for loads. In the absence of special considerationsthese factors should have the values given in 36 according to the material. the type of loading .and the limit state being considered. 35.2 Limit State 01CoDapse The limit state of collapse of the structure or part of the structure could be assessed from rupture of one or more critical sections and from bucklingdue to elastic or plastic instability (including the effects of sway where appropriate) or overturning. The resistance to bending,shear,torsionand axial loads at every section shall not be less than the appropriate value at that section produced by the probable most unfavourable combination of loads on the structure using the appropriate partial safety factors. 35.3 Limit States of ServiceabUlty 35.3.1 Deflection Limiting values of deflections are given in 23.2. 35.3.2 Cracking Cracking of concrete should not adversely affect the appearance or durability of the structure; the acceptable limitsof crackingwould vary withthe typeof structure and environment. Wherespecificattention is required to limit the designedcrack width to a particular value. crack width calculation may be done using formula given in Annex F. The practical objective of calculating crack width is merely to give guidance to the designer in making appropriate structural arrangements and in avoiding gross errors in design, which might result in concentration and excessive width of flexuralcrack. The surfacewidthof the cracks should not, in general, exceed 0.3 mm in members where cracking is not harmfuland does not have any serious adverseeffects uponthe preservation of reinforcingsteel nor upon the durability of the structures. In members wherecracking in the tensile zone is harmful either because they are exposed to the effects of the weatheror continuously exposedto moistureor in contactsoil or groundwater, an upperlimitof 0.2 mm is suggestedfor the maximum width of cracks. For particularly aggressi ve environment, such as the 'severe' category in Table 3, the assessed surface width of cracks should not in general,exceed 0.1 mm. 35.4 Other Limit States Structures designed for unusual or special functions shall comply with any relevant additional limit stale consideredappropriateto that structure. 36 CHARACTERISTIC AND DESIGN VALUES AND PARTIALSAFETYFACTORS 36.1 Characteristic Strength of Materials The term 'characteristicstrength' means that value of the strengthof the materialbelowwhichnot more than 5 percent of the test results are expected to fall. The characteristic strength for concrete shall be in accordance with Table 2. Until the relevant Indian Standard Specifications for reinforcing steel are modified to include the concept of characteristic strength, the characteristic value shall be assumed as the minimum yield stress 10.2 percent proof stress specified in therelevant Indian Standard Specifications. 36.2 Characteristic Loads The tenn 'characteristic load' meansthat valueof load which has a 9S percent probability of notbeingexceeded during the life of the structure. Since data are not available to express loads in statistical terms, for the purpose of this standard, dead loads given in IS 875 (Part 1). imposed loads given in IS 875 (Part 2), wind loads given in IS 875 (Part 3), snow load as given in IS 875 (Part 4) and seismic forces given in IS 1893 shall be assumed as the characteristic loads. 61 IS 456: 2000 36.3 Design Values 36.4.2PartialSafety Factor Ym for Mateiral Strength 36.3.1 Materials 36.4.2.1 Whenassessing thestrength of a sttucturcor structural memberfor the limit stale of collapse. the values of partial safetyfactor. -r.. should be taken as I.S for concrete and US forsteel. The design strength of the materials.!.J is givenby where NOTE - y. values are .a1ready incorporated ill the equations and tables aiven ill this .tandard for limit state. = characteristic strength of the material f design. (see 31).1). and Ym 36.4.2.2 Whenassessing the deflection, the material properties such as modulus of elasticity should be taken 8S those associated with the characteristic strength of the material. = partial safety factor appropriate to the material and the limit state being considered. 36.3.2 Loads 37 ANALYSIS The design load. FI! is given by 37.1 Analysis of Stnacture Fd=FYr Methods of analysis as in 22 shall be used. The material strength to beassumed shallbecharacteristic values in the determination of elastic properties.of members irrespective of the limit state being considered. Redistribution of thecalculated moments may be madeas givenin 37.1.1. 37.1.1. Redistribution of Moments in Continuous Beamsand Frames The redistribution of moments may be carried out satisfying the following conditions: a) Equilibirum between the interal forces and the extemalloads is maintained. h) Theultimate moment of resistance provided at any section of a member is not less than 70 percent of the moment at that sectionobtained from an elastic maximum moment diagram covering all appropriate combinations of loads. c) Theelastic moment at anysection in a member due to a particular combination of loads shall where F = Yf = partial safety factor appropriate to the characteristic load (see 36.2).and nature of loading andthelimitstatebeing considered. 36.3.3 Consequences ofAttainingLimit State Where theconsequences of a structure attaining a limit state are of a serious nature such as huge loss of life and disruption of the economy. higher values for Yf and Ym thanthosegivenunder36.4.1 and36.4.2may be applied. 36.4 Partial Safety Factors 36.4.1 PartialSafety Factor Yf for Loads The values of Yf givenin Table 18 shall normally be used. Table 18 Valuesof Partial Safety Factor Yf for Loads (Clause.t 18.2.3.1.36.4.1 andB-4.3) Load Combination .. (I) DL+/L DL+WL Unlit State 01 CoIIapIe DL IL WL DL IL (2) (3) (4) (5) (6) 1.0 I.S I.S or . 091) DL+/L+ WL Limit Statel of SenlceabUllJ ... ... 1.2 1.0 1.0 1.S 1.0 -- 1.0 WL (7) 1.0 0.8 0.8 NOTES 1 Whileconsidering earthquake effects. substitute EL for WL 2 For lhe limitstatesof serviceability. thevoluca or 1, liven in thistableareapplicable forshan termeffects.Whileasses.inathe loftg term effectsdueto enep thedead load and that part of the live loadlikelyto be permanent mayonly be conlidered. n This valueis to be considered whenstability apinst overturning or stressrevenal il critical. 68 15456: 2000 not be reduced by more than 30 percentof the numerically largestmomentgivenanywhere by the elastic maximum moments diagramfor the particular member. covering aU appropriate combination of loads. d) At sections where the moment capacity after redistribution is less than that from the elastic maximum moment diagram. the following relationship shall be satisfied: b) The maximum strain in concrete at the outennostcompression fibreis takenas 0.003 5 in bending. c) The relationship between thecompressive stress distribution inconcrete and the sttainin concrete may be assumed to be rectangle. trapezoid. parabola or any other shape which results in prediction of strengthin substantial agreement with the results of test. An acceptable stressstrain curve is given in Fig. 21. For design purposes. the compressive strengthof concrete inthe stnaeture shallbe assumed to be 0.67times the characteristic strength. The partial safety factor y. = 1.5 shall be applied in addition to this. 5L+ 8M SO.6 d 100 where Xu = depth of neutral axis. = d effectivedepth. and 6M percentage reduction in moment. e) In structures in which the structural frame provides the lateral stability. the reductions in moment allowed by condition 37.1.1 (c) shall be restricted to 10 percentfor stnactures over 4 storeysin height. NOTE - Pordie streu·llrlin CUM ill rrlJ. 21 die deaip stressblock plIIUIDClerI_ IS follows ('flfI Pia. 22): = • 0.36lot' x. Area ofsuessblock Depthof celItle of colllplalive force • 0.42 x. fromthe extreme fim ift compression when: = chancteriatic c:omprasive lballth ofconcme. lIIlCI I~ x. = depCh of neutnl WI. 37.1.2 AnalysisofSlabs Spanning in lWo Directions at RightAngles 38 LIMIT STATE OF COLLAPSE: FLEXURE d) The tensilestrengthof the concreteis ignored. e) The stresses in the reinforcement are derived from representative stress-strain curve for the type of steel used. 'JYpica1 curves are given in Fig. 23. For design purposesthe partial safety factor Ym • equal to 1.15 shallbeapplied. 38.1 Assumpdons f) The maximum strain in the tension reinforce- Yield line theory or any other acceptable method may be used. Alternatively the provisions given in Annex D may be followed. ment in the section at failure shall not be less than: Design for the limit state of collapse in flexure shall be basedon the assumptions given below: a) Plane sections nonnal to the axis remain plane after bending. --!:t.+0.002 1.15E. where _.r-------t f, = characteristic strengthof steel. and fa E, (H7fCk t III III III Ill: 0.67 fck Irm t- III 0·002 = modulus of elasticity of steel. T O'42X u Xu ~ 0·03S STRAIN- FIG. 21 STRESS-STRAIN CURVE R>R CONCREm FIG. 69 22 STRESS BLOCK PARAME'I1!RS O·36fc k Xu 18456: 2000 ~..------fy ,, / I t I I I STRESS I I I I I , •• -ZOOOOO , , "/".".2 I I ·0001 '000' -0001 SlRAIN--. 23A Cold Worked Defonned Bar ,..-------- " 'r l-------- "".15 t £,-200000 N/mm' 238 STEEL BAR WITH 0mNn'E YIELD POINT FlO. 23 REPRESENrATIVB STRESS-S11tA1N CURVES fOR RElNPORCBMENT NOTE - The limiting values of the depth of neutraluis for 31.1118 as foUows: 38.1 (c) for flexure, the following shallbe assumed: diffe~nl gradesof steelbased on theassumptions in f., x.. _ld 2SO O.~3 415 0.48 0.46 a) 1be maximum compressive strain in concrete in axial compression is taken as 0.002. b) 1be maximum compressive strain at the highly compressed extreme fibre inconcrete subjected to axial compression and bending and when thereis notensionon the section shall be0.003 S minus 0.75 times the strain at the least compressed extreme fibre. SOO The expression for obtaining the moments rea.iltance for ~e:tanlUlar and T-Sectionl. bIIlld OIl the lIIUIIIpliouof .1, 118 given in Annex G. 0' 39 LIMIT STATEOF COLLAPSE: COMPRESSION 39.2 MW-w EeceatrIdty 39.1 AlSUlDpdoM In addition to' the assumptions given in 38.1 <a) to All members incompression shallbedesigned for the minimum eccentricity inICCOIdance with25.4. Where 70 IS 456: 2000 calculated eccentricity is larger, the minimum eccentricity should be ignored. 39.3 Short Axially LoadecI Me.ben in COlDpnaloD The member shall be designed by considering the assumptions given in 39.1 and the minimum eccentricity. When the minimum eccentricity as per 25.4 does not exceed O.OS times the lateral dimension, the members may be designed by the followins equation: . PI where Pu I.. 39.6 Members Subjected to Combined Axial Load and Biaxial BenellD. The resistance of a member subjected to axial force and biaxial bending shall be obtained on the basis of assumptions given in 39.1 and 39.2 with neutral axis so chosen as to satisfy the equilibrium of load and moments abouttwoaxes.Alternatively suchmembers may be designed by the following equation: + [ ]a. S [~]a. Al Atu~1 M uy = 0.4'et .A + 0.67f, .A c • ux1 Ie = moments about x and y axes axial load on the member. = characteristic compressive strensthof the characteristic strength ofthecompression reinforcement, and is relatedto PulPtJI where Py Z =0.4S let · Ac + 0.7S 1,. Ale For values of Pu'PUI 0.2 to 0.8, the valuesof a. vary linearly from 1.0to 2.0.For values less than0.2, aa is 1.0; for values greater than 0.8. Q. is 2.0. = 39.4 Compression Memben with ReDeal Relnforcemeat 39.7 Slender Comp....lon Memben The strength of compression members with helical reinforcement satisfyin. the requirement of39.4.1shall be taken as 1.0~ timesthe strensth of similarmember with lateralties. 39.4.1 Theratioof the volume of helical reinforcement to the volume of the core shall not be less than 0.36(A.IAc-l)f*'f, where A. pss area of the section, fa The design ,of slender compression members (see 25.1.1) shall be based on the forces and the moments determined froman analysis of thestructure, including the effect of deflections on moments and forces. When the effect of deflections are not taken Into account in the analysis. additional momentgiven in 39.7.1 shall be takenintoaccountin the appropriate direction. 39.7.1 The additional moments M. and M.'I shall be calculated by the ~ollowinl fonnulae: = = areaof the core of the helically reinforced columnmeasured to the outside diameter of the helix, M = PyD concrete, and M characteristic strength of the helical reinforcement but not exceeding where Pu 41~N/mm2. 39.5 Memben Subjected to Combined Axial la Load aDd Unlulal BeDeIlD, Amember subjected to axial force anduniaxial bending shall be desisned on the basisof 39.1 and 39.3. .y {!a.}2 2000 D u • characteristic compressive strensthof the I, = due to design loads, maximum uniaxial moment capacity foranaxialloadof Pu' bending about x and y axes respectively, and Q. Ale == area of longitudinal reinforcement for columns. Ac = MU l t MaYI = Area of concrete, t, = • where concrete, Ac 10 • ..M..{!.2.}2 2000 b = axial loadon the member, =effective length in respect of the major axis. 'ey D NOTE - The deli... of member lubjecttocombined uialload and uniuial bendin. will involve leftIlhy calculation by trill and error. In orcI. to overcome these difticuldes intonacuoD diql1UDl may beUIed. The. havebeenprepand aDd published by 8 IS in •SP : 16 Deilin aida for reinforced concreto to IS456'. =effective lenlth inrespect of the minor axis. =depth of the cross-section at right angles to the major axis, and b = width of the member. Fordesignof section, 39.5or 39.6as appropriate shall apply. 71 18456: __ NOTES 1 Acolumn maybe considered brKedin a Jivenplaneif1alaal stability to the I1nICtUIe • I whole is provided by waUl or bracin. or bultJaliDi deliped to . .ill aIl1alerll f - . in that plane. It shouldotberwi. be eoDlictered _ UDbncecI. 2 In the cue of a bmced cola. . without uy tnnmne loadl occurriq in itaheiPt, the additional moment Ihallbeadded to an inidal momeDt equalto lum of 0.4 MI' and 0.6 "'w2 where Mwj is the laqer end moment and MI' is the smaller end moment (IllUmed neptive Ifthecolumn iI bent indouble curvature). In DO CIIe shall the initial molDeD! be lei. than 0.4 M.2 nor Ihctotal momeat incluclilll theinitialmomeat be lesathaD Md - For\1Dbraced columu, the IdditiODll moment shall be added to theend momenta. 3 UnbrKed compmsionmemben.11 anyliven level or 1tOre)'. lubject to lateral load are Ulually coDltrained to cleftect equally. In suCh cueallenclcmeu redoforucla colUllUl may be taken _ the _venae for all eolUIDDI ICtinI ill the same diJection. 39.7.1.1 The values given by equation 39.7.1 may be multiplied by the followins factor: ,,= P",-Ij SI 40.2 Desip Shear Strenath 01Coaerete 40.2.1 Thedesign shearstrength of concrete in beams without shear reinforcement is liven in Table 19. 40.11.1 For solidslabs, the desi,n shearstrength for concrete shall be fele, where Ie has the values given below: Overall Dtpth 300 or 275 150 m 200 175 ISO or 01Slab, mm more less Ie 1.00 1.0S 1.10 I.IS 1.20 1.25 1.30 NOYS - nul provilion shall not apply to flatslaba forwhicb 31.6 shall apply. 40.2.2 ShearStrength of Mtmbtrs undtr Axial Compression PUI-I\ where p. • axialloadon compression member, p. Ph of the beam. The negative sign in the fonnul. applies when the bending moment My increases numerically in the same direction as the effective depth d increases. and the positive sign whenthemomentdecreases numerically in thisdirection. = as defined in 39.6, and = axial loadcorresponding to the condition For members subjected to axial compression Pu' the design shearstrength of concrete, given in Table 19, shall be multiplied by the following factor : 6 I + 2.!L A' but·not exceeding 1.5 of maximum compressive strain of = 0.003 5 in concrete and tensile strain of 0.002 inoutermost layeroftension steel. 40 LIMIT STATE OF COLLAPSE: SHEAR 40.1 NomIuI Shear S..... The nominal shear ,tress in beams of unifonn depth Aball be obtained by the followina equation: t ~ y • . .:.L b. where V. :I shearforce due to desip loads; b • breadth of themember, which forflanled section shall be taken u the breadth of the web. b..: and d effective depth. = 40.1.1 B'DmI of Varying Depth In the case of beams of varyinS depth the equation shall be modified u: V. :I: M, f •• v d I Jet where Pu axial compressive forcein Newtons, A. = gross areaof theconcrete section in mm', and let. characteristic compressive stl1nath of concrete. = = 40.13 With She"rReinforcement Under no circumstances. even with shear reinforcement. shall the nominal shearstressin beams tv execed t cmu liven in Table 20. 40.2.3.1 For solid slabs, the nominal shear stress shall not exceed half the appropriate values given in Table 20. 40.3 MInimum Shear RelDforeement When tv is lessthan 'tc liven in Table 19,minimum shearreinforcement shall be provided in accordance with 26.5.1.6. tanfJ 40.4 DesAp of Shear lleIIlforeemeDt When e, exceeds 1 c given in Table 19. shear reinforcement shall be provided inanyof thefollowing forms: a) Vertical stinups. b) Bent-up ban alona withstirrups, and btl where b and d are the sameas in 40.1. M• • bendinl moment at the section, and ~ • anile between the top and the bottom edps 1 v' V.' 72 18456: 2000 Table 19 DesIp Shear ~tre"'" 01Concrete, 't c ' NI.....r (Cltuues4O.2.1. 40.2.2. 40.3. 40.4. 4O.S.3. 41.3.2. 41.3.3 and41.4.3) l00~ ,.. btl CoDcnte Gnde , - MIS M20 M2S M30 M3S M40IIld above (l) (2) (3) (4) (5) (6) (7) ~0.t5 0.28 0.35 0.46 0.28 0.36 0.48 0.56 0.62 0.61 0.12 0.29 0.36 0.49 0.29 0.37 0.29 0.25 0.50 0.1S 1.00 1.2S I. SO 1.1S 2.00 2.25 2.50 2.7S 0.54 0.60 0.64 0.68 0.11 0.7S 0.79 0.81 0.82 0.82 0.11 0.11 0.11 0.71 3.00 nnd 0.71 0.82 0.37 0.50 0.59 0.61 0.73 0.18 0.82 0.50 0.59 0.66 0.11 0.76 0.80 0.84 0.88 0.9t 0.94 0.$1 0.64 0.10 0.14 0.78 0.82 0.85 0.88 0.90 0.92 0.86 0.90 0.93 0.96 0.99 0.96 0.30 0.38 0.51 0.60 0.68 0.74 0.79 0.84 0.88 0.92 0.95 0.98 1.01 above NOTE - The termA Is the arell of lonaltudinll1ten.lon reinforcement which conllnues at IClISt oneeffective depth beyond the section bein, considered exc;pt at supponwhere the full areaof tension reinforcement maybe usedprovided thedetllilina confonn.to 16.1.1 and26.1.3 Table 10 Maximum Shear Stress, f c _ll , N/mmJ ( Cia",,, 40.2.3. 40.2.3.1. 4O.S.1 arad 41.3.1 ) Concrete Gncle MIS M20 M2S M30 M3S 2.5 2.' 3.1 3.S 3.7 c) Inclined stirrups. Where bent-up bars are provided. their contribution towards shear resistance than not be more than half thatof the total shearreinforcement. Shear reinforcement shallbe provided tocarry a shear equal to Vu - f'~ bd The atrenath of ahcar reinforcement V... shall be calculated u below: where A V • II: des ian shear strenath of the concrete. Iv Ir 0.8.7 Iy.-\vd ( . ) sma + cosa sv a c) For 5in,1e bar or 5in,Ie group of parallel bars. all bent-up at thesame cross-section: 21H1815/07_11 e, b b) Forinclined stirrups or a series of barl bent-up at different cross-sections: VU1 III s. _ 0._87...;./',1...A,...;.y~d U1 • 'tv total cross-sectional area ofstirrup legs or bent-up ban within a distance s.' specina of the stirrups or bent-up bars alona the lenath of themember, nc)tninal shear SIre.S, •• a) For vertical stirrupa: d 73 M40 lIIId IIbove 4.0 II: • breadth of the member which for flan.ed beams, shall be taken as the breadth of theweb b•• characteristic ItrenJthof thestirrup or bent-up reinforcement which shall not be taken Jreaterthan 41~ N/mm 2, III anale between the inclined stirrup or bent- upbarandthe axis of the member. notless than 4'°. and :; effective depth. III = IS 456: 2000 NOTES is given by: 1 Where more(hanone type of shear reinforcement is used to reinforcethe same portion of the beam. the total shear resistance shallbecomputed asthesumof the resistance for the varioustypes separately. 2 Theareaof the stirrupsshallnot belessthan the minimum specified in 26.5.1.6. AI' = ayb (Tv - 2d fJa,) I 0.87/" ~ O.4ay b/O.87 ~ Thisreinforcement should be provided within themiddle three quarters of (lv' wherea y is less than d. horizontal shear reinforcement will be effective than vertical. 40.5 Enhanced Shear Strength of Sections Close to Supports 40.5.3 EnhancedShear Strength Near Supports (SimplifiedApproach) 40.5.1 General Shear failure at sections of beams and cantilevers without shear reinforcement wiIJ normally occur on plane inclined at an angle 30° to the horizontal. If the angle of failure plane is forced to be inclined more steeply than this [because the section considered (X - X) in Fig. 24 is close to a support or for other reasons}, the shear force requiredto produce failure is increased. The enhancement of shear strength may he taken into account in the design of sections near a support by increasing design shear strength of concrete to 2d reI a; provided that design shear stress at the face of the support remains less than the values given in Table 20. Account may be taken of the enhancement in any situation where the section consideredis closer to the face of a supportor concentrated loadthan twice the effective depth. d. To be effective. tension reinforcement should extend on each side of the point where it is intersected by a possible failure plane for a distance at least equal to the effective depth, or be provided with an equiv rlent anchorage. The procedure givenin 40.5.1and40.5.2 may be used for all beams. However for beams carrying generally uniform load or where the principal load is located farther than 2d from the face of support, the shear stress may be calculated at a section a distance d from the face of support. The value of t c is calculated in accordance with Table 19 and appropriate shear reinforcement is provided at sections closer to the support, no funher check for shear at such sections is required. 41 LIMIT STA1'E OF COLLAPSE: TORSION 41.1 General In structures, where torsion is required to maintain equilibrium, members shall be designed for torsion in accordance with41.2,41.3 and41.4. However. for such indeterminate structures where torsion can be eliminated by releasing redundant restraints. no specific design for torsion is necessary, provided torsional stiffness is neglectedin the calculation of internal forces.Adequate control ofanytorsional cracking isprovided by theshear reinforcement as per 40. N()TE - The approach to design in this clause is as follows: 40.5.2 Shear Reinforcementfor Sections Close to . Supports Torsional reinforcement is not calculated separately from that required for bending and shear. Instead the lotal longitudinal reinforcement is determined for a fictitious bending moment which is a function of actual bending moment and torsion; If shearreinforcement is required. the total areaof this NOTE - The shearcausing failure is thatocting on, section X-X. FIG. 24 SHEAR FAILURE NEAR SUPPORTS 74 IS 456: 2000 similarlyweb reinforcement is determined for 3 fictitious shear which is a function of actual shear and torsion. where '~I is the torsional moment, D is the overalldepth of the beam and b is the breadth of the beam, 41.1.1 The design rules laid down in 41.3 and 41.4 shall apply to beams of solid rectangular cross.. section. However, these clauses may also be applied to flanged beams, by substituting bw for b in which case they are generally conservative; therefore specialist literature may be referred to. 41.4.2.1 If the numerical value of M l as defined in 41.4.2 exceeds the numerical value of the moment A1 longitudinal reinforcement shall be provided on , 11 the flexural compression face, such that the beam can also withstand an equivalent M e2 given hy 41.2 Critical Section Me2 == M, - Mu ' the moment M~.2 being taken as acung in the opposite sense to the moment Mu ' Sections located less than a distance d. from the face of the support may be designed for the same torsion as computed at a distance d, where d is the effectivedepth. 41.4.~' Transverse Reinforcement 41.3 Shear and Torsion Two legged closed hoops enclosing the corner longitudinal bars shall have an area of cross-section 41.3.1 Equivalent Shear A~\" given by Equivalent shear, Vc ' shall be calculated from the formula: A sv :::; _ 7:J SV + Vu s v _.. hi lil (O.H7 j~) 2.5 eft ((J.~7./; ) , hut the total transverse reinforcement shall not be less than where (f\.e - f c V," = equivalent. shear, Vu = shear, 1·u = torsional moment, and b 0.87 J~ where = breadth of beam, The equivalent nominal shear stress. .lb.s,. 'tv.. in this case shall be calculated as given in 40.1, except for substituting \'u hy Vc' The values of r vc shall not exceed the values of tt' mall given in Table 20. "1:, torsional moment, '<I _. s,. = shear force, bi 41.3.2 If the equivalent nominal shear stress, 't\'l' docs not exceed tl' given in .ablc 19, minimum shear d, .~. 0- spacing of the stirrup reinforcement. centre-to-centre distance hctwccn Ct uner bars in the direction of the width. centre-to-centre distance between corner bars, reinforcement shall he provided as per 26.5.1.6. h 41.3.3 If t v\. exceeds t, given in Table 19. both longitudinal and transverse reinforcement shall he - breadth of the member, t, .- characteristic strength of the stirrup reinforcement, 41.4 Reinforcement in Members Subjected to Torsion tw equivalent shear stress as specified in 41.4.1 Reinforcement for torsion, when required, shall consist of longitudinal and transverse reinforcement, '(... provided in accordance with 41.4. 41.3.1, and 41.4.2 Longitudinal Reinforcement In all normal cases. the deflection of a flexural member will not he excessive if the ratio of its span to its effective depth is not greater than appropriate ratios given in 23.2.1. When deflections arc calculutcd according to Annex C, they shall not exceed the permissible values given in 23.2. where = bending moment at the cross-section, and t: (. I + !J u shear strength of the concrete as rt.~r Table It) . 42.1 Flexural Members M d =Mu +M, M. = - 42 LIMIT STATI~ OF SF:RVll~EABII.4IT\': n E:I~~I.lE<.:'rl ON The longitudinal reinforcement shall he designed to resist an equivalent bending 1l10111Cnl, Md - given by Mu - lb·) 1.7 75 IS 456: 2000 • 43 LIMIT STATE OF SERVICEABILITY: CRACKING 43.2 Compression Members Cracks due to bending in a compression member subjectedto a design axial load greater than O.2fc.. Ac' whereJet I" is the characteristiccompressivestrength of concrete and Ac is the area of the gross section of the member, need notbe checked. A member subjected to lesser load than 0.2 let Ac may be considered as flexural member for the purpose of crack control (see 43.1). 43.1 Flexural Members In general,compliance with the spacing requirements of reinforcement given in 26.3.2 should be sufficient to control flexural cracking. If greater spacing are required, the expectedcrack width should be checked by formula given in Annex F. "I) IS 456: ZOOO ANNEXA (Clause 2) LIST OF REFERREDINDIAN STANDARDS nIle IS No. 269 : 1989 Specification for ordinary Portland cement, 33 grade (fourth IS No. 1642: 1989 Code of practice for fire safety ofbuildings (aenn) : Details of construction (first I'tvilio1l) 1186: 1985 Specification for high strength deformed steelbarsand wiresfor concrete reinforcement (third revision) 383 : 1970 Specificationfor coarse and fine aggregates from natural sources for concrete (second revision) 432 (Part 1) : Specification for mild steel and medium tensile steel bars and hard-drawn steel wire for concrete reinforcement: Part 1 Mild steel and medium tensile steel bars (third revision) 1982 4SS: 1989 Specification for Portland slag cement (fourth revision) 516 : 19S9 Method of test for strength of concrete 875 Codeof practicefor designloads (other than earthquake) for buildingsand structures : ntle m'uioll) 1791 : 1968 Specification for batch type concrete mixers(StCoM revision) 1893 : 1984 Criteria for earthquake resistant design of structures (fourth nvision) 1904: 1986 Code of practice for design and construction of foundations in soils : General requirements (third revision) 2062 : 1992 Steel for general structural purposes (fourth Tn'uion) 2386 (Part 3) : 1963 Methods of test for aggreptes for concrete: Part3 Specific pavity, density, voids, absorption and bulking 2502: 1963 Code of practicefor bendingand fixing of bars for concrete reinforcement (Part 1) : 1987 Dead loads - Unit weights of building material and stored materials (second revision) (Part 2) : t 987 Imposed loads (second revision) (Part 3) : 1987 Wind loads (second revision) (Part 4) : 1987 Snow loads (second revision) (Part S) : 1987 Special loads and load combinations (second revision) 2S05: 1980 Concrete vibrators-Immersion type - General requirements 1199: 1959 Methods of sampling and analysis of concrete 2506: 1985 1343 : 1980 Code of practice for prestressed concrete (first revision) General requirements for screed board concrete vibrators (first revision) 2514 : 1963 1489 Specification for Portland pozzolana cement : Specification for concrete vibratingtables 2751 : 1979 Recommended practice for welding of mild steel plain and (Part 1) : 1991 Fly ash based (third revision) (Part 2) : 1991 Calcined clay based (third revision) 1566 : 1982 1641 : 1988 deformed bars for reinforced construction (first Tn'ision) 3025 Specification for hard-drawn steel wire fabric for concrete reinforcement (second revision) Code of practice for fire safety of buildings (general): General principles of fire grading and classification (first revision) Methods of sampling and test (physical andchemical) forwater and waste water: (Part 17) : 1984 Non-filterable residue (total suspendedsolids) (first ~vision) (Part 18) : 1984 Volatile and fixed residue (total filterable and non-filterable) (first revision) 77 IS 456: 1000 IS No. Title IS No. Title (Part 22) : 1986 Acidity (first revision) (Part 3) : 1972 Concrete reinforcement (Part 23) : 1986 Alkalinity (first revision) (Part 4) : 1972 Typesof concrete (Part 24) : 1986 Sulphates (first revision) (Part S) : 1972 Pormworkfor concrete (Part 32) : 1988 Chloride (first revision) (Part 6) : 1972 Equipment,tool and plant 3414 : 1968 Code of practice for design and installationofjoints in buildings (Part 7) : 1973 3812 : 1981 Specification for fly ash for use as pozzolana and admixture (first revision) Mixing, laying, compaction, curing and other construction aspect (Part 8) : 1973 Properties of concrete (Part 9) : 1973 Structuralaspects (Part 10) : 1973 Tests and testing apparatus (Part 11) : 1973 Prestressedconcrete (Part 12) : 1973 Miscellaneous 395I (Part 1) :. 1975 Specification forhollow claytiles for floorsand roofs: Part 1Filler type (first revision) 403I(Part S): 1988 Methods of physical tests for hydraulic cement : Part S Determination of initialand final setting times (first revision) 4082 : 1996 Recommendations on stacking and storage of construction materialsand componentsat site 6909: 1990 Specification for supersulphated cement 7861 Code of practice for extreme weatherconcreting : (Part 1) : 1975 Recommended practice for hot weather concreting (Part 2) : 1975 Recommended practice for cold weather concreting (second revision) 4326: 1993 4656: 1968 4845 : 1968 Code of practice for earthquake resistantdesign and construction of buildings (second revision) 8041 : 1990 Specification for form vibrators for concrete Specification for rapid hardening Portland cement(second revision) 8043 : 1991 Definitions and terminology relating to hydrauliccement Specification for hydrophobic Portland cement(second revision) 8112 : 1989 Specification for 43 grade ordinary Portland cement (first revision) 9013 : 1978 Method of making, curing and determining compressive strength of accelerated cured concrete test specimens 9103 : 1999 Specification for admixtures for concrete (first revisiom 9417 : 1989 Recommendations for welding cold worked bars for reinforced concrete construction (j; rst 4925 : 1968 Specification for concrete hatching and mixing plant 4926: 1976 Specification for ready-mixed concrete (second revision) S816: 1999 Method of test for splitting tensile strength of concrete (first revision) 6061 Codeof practiceforconstruction of floor and roof with joists and filler blocks: (Part 1) : 1971 With hollow concrete filler blocks (Part 2) : 1971 With hollow clay filler blocks (first revision) 6452: 1989 6461 r~\lision) Specification for high alumina cement for structural use 11817 : 1986 Classification of joints in buildings for accommodation of dimensional deviations during construction 12089: 1987 Specification for granulatedslag for manufactureof Portland slag cement 12119 : 1981 General requirements for pan mixers for concrete Glossary of terms relating to cement: (Part J) : 1972 Concrete aggregates (Part 2) : 1972 Materials 78 IS 456: 1000 IS No. IS No. Title 12269 : 1981 Specification for S3 grade ordinary Portland cement 12330: 1988 Specification for sulphate resisting Portland cement 12600 : 1989 Specification for low heat Portland cement 13311 Methods of non-destructive testing of concrete: Title (Pan I) : 1992 Ultrasonic pulse velocity (Pan 2) : t 992 Rebound hammer 13920: 1'993 Code of practice for ductile detailing of reinforced concrete structures subjected to seesmic forces 14687 : 1999 Guidelines for falsework for concrete structures 79 IS 456: 2000 ANNEX B (Clauses 18.2.2,22.3.1,22.7.26.2.1 and 32.1) STRUCTURAL DESIGN (WORKING STRESS METHOD) 8-1 GENERAL c) The stress-strain relationship of steel and concrete, underworking loads,is a straight line. B-l.1 General Desiln Requirements d) The modular ratio m has the value 280. The general design requirements of Section 3 shall apply to this Annex. 30'cbc wherea c~hc is permissible compressive stress due to bending in concretein N/mm2 as specified in Table21. 0-1.2 Redistribution of Moments Exceptwherethe simplified analysis usingcoefficients (see 22.5) is used, the moments over the support" for any assumed arrangement of loading, including the deadload moments may each be increased or decreased hy not more than 15 percent, provided that these modified moments over the supports are used for the calculation of thecorresponding moments in the spans, NOTE- The expression given for m panially takes into account long-termeffects such as creep. Therefore this In is not the same Wi the modular ratio derived bDSC~d on the valueof Ef: givenin 6.2.3.1. B-2 PERMISSIBLESTRESSES B-2.1 PermL.sible Stresses in Concrete Permissible stressesfor the variousgradesof concrete shall he taken as those given in Tables 21 uno 23. 8-1.3 Assumptions for DesilD of Members In the methods based on elastic theory, the following assumptions shall be made: NOTE - For increase in strength with Qie 6.1.1 shall be upplicable.The values of permissible stres~ shall he nbruined hy interpolation betweenthe gradesof concrete. ill At any cross-section. plane sections before bending remain plain after bending. B-2.1.1 DirectTension For members in direct tension, when full tension is taken by the reinforcement alone, the tensilestressshall be not greater than the values given below: b) All tensile stresses arc taken up by reinforcement and none by concrete. except as otherwise specifically permitted. Grad« til COli f,., M I() M I~ M20 M2~ M~O M3~ M40 M4~ 1.2 2.0 2.8 3.2 3,6 4.0 4.4 4.8 M~O It T",I.fUt Stress, Nllnlll' The tensile stress shall be calculatedas F 0-2.2 Permissible Stresses in Steel Reinforcement A". +mA. t Pennissiblc stresses in steel reinforcement shell not exceed the values specified in Table 22. f where FL 8-2.2.1 In flexural members the value of 0'.. given in Table 22 is applicable at the centroid of the tensile = total tension on the member minus pre- reinforcement subject tothecondition thatwhen more than one layer of tensile reinforcement is provided, tension in steel. if any, before concreting: A\: ~.2 = cross-sectional areaot'concrete excludina the stress at the centroid of the outermost layer shall not exceed by more than 10percent the value given in any finishing material and rcinforcina stee]: n, == modular ratio: and A.. = cross-sectional area of reinforcing steel TobIe 22. 8-2.3 Increase in Permlaslble Stresla Wherestresses dueto wind(orearthquake) temperature and shrinkage effects are combined with those due to dead, live and impact load, the stresses specified in Tables 21 22 and 23 may be exceeded upto a limit of in tension. n-1.1.% Bond Stressfor Deformed Bars t In the case of defanned bars conforming to IS 1786, the bond stresses given in Tahle 21 may be increased by 60 percent. 33.!. percent. Wind and seismic forces need not be 3 considered as acting simultaneously. 80 IS 456: 2000 Table 21 Permissible Stresses in Concrete (Clauses B·l.3. B·2.1. B-2.l.2.B-2.3 and B·4.2) All values in Ntmml . <Yrade 01 Concrete Permissible Stress In Compression (1) Permissible Strea Bending Direct In Bond (Averale) for Plain Bars In Tension (2) (3) (4) <, 0" M 10 3.0 2.5 M 15 5.0 4.0 M20 7.0 5.0 0.8 M2S 8.5 6.0 0.9 M30 10.0 8.0 1.0 1.1 0.6 M 35 11.5 lJ.O M40 13.0 10.0 12 M45 14.5 11.0 1.3 M 50 16.0 t2.0 1.4 NOTES I The values of permissible: shear stress in concrete are given in Table 23. 2 The bond stress given in col 4 shall be increased by 25 percent for bars in compression. multiplication of the appropriatemaximumpermissible stress as specified under B-2.1 and B-2.2 by the coefficient C, given by the following formula: B-3 PERMISSIBLE LOADS IN COMPRESSION MEMBERS B-3.1 Pedestals and Short Columns with Lateral Ties The axial load P permissible on a pedestal or short column reinforced with longitudinal bars and lateral ties shall not exceed that given by the following equation: C r where C, I", b where 0n = permissible stress in concrete in direct compression. A,. = cross-sectional area of concrete excluding any finishing material and reinforcing steel. 0"" = permissible compressive stress for column bars, and A", = cross-sectional area of the longitudinal steel. = reduction coefficient: = effective length of column; and = least lateral dimension of column; for column with helical reinforcement, b is the diameter of the core. For moreexact calculations, the maximum permissible stresses in a reinforced concrete column or part thereof having a ratio of effective column length to least lateral radius of gyration above 40 shall not exceed those which result from the multiplication of the appropriate maximum permissible stresses specified under B.2.1 and 0-2.2 by the coefficient C, given by the following formula: NOTE - The minimumeccentricity mentioned in 25.4 may he deemed to be incorporated in the above equanon. Cr B-3.2 Short Columns with Helical Reinforcement =1.25 _ le~ IbO'min where i miP is the least radius of gyration. The permissible load for columns with helical reinforcementsatisfying the requirementof 39.4.1 shall be 1.05 times the permissible load for similar member with lateral ties or rings. B-3.4 Composite Columns a) Allowable load - The allowable axial load P on a composite column consisting of structural steel or cast-iron column thoroughly encased in concrete reinforced with both longitudinal and spiral reinforcement. shall not exceed that given hy the following formula; B-3.3 Long Columns The maximum permissible stress in a reinforced concrete column or part thereof having a ratio of effectivecolumn length to least lateraldimensionabove 12 shall not exceed that which results from the 2116815/07-12 =1.25 _.!SL 48b 81 IS 456: 2000 Table 22 Permissible Stresses in Steel Reinforcement (Clauses 8-2.2, 8-2.2.1, B-2.3 and B..4.2) No. l2) (l) i) ii) Permissible Stresses In N/mm2 Type of Stress In Steel Reinforcement SI Tension ( 0"1 or Mild Steel Ban Conforming to Grade I of IS 4J2 (Pan I) MediumTensile Steel Conforming to IS 432 (Port 1) forming to IS 1786 (Grade Fe 41S) (3) (4) (5) 011) a) LJp (0 and including 20 mm 140 b) Over 20 rom 130 Compression in column I Half the guaranteed yield stress subject to a maximum of 190 High YieldStrength Deformed Bars Con- 230 230 130 130 190 bars (all) iii) Compressionin bars in a bean) or slab when the compressive resistanceof the concrete is taken into account iv) Compressionin bars in a beam or slab where the compressiveresistance of the concrete is not taken into account: The calculated compressive stress in the surrounding concrete multiplied by 1.S times the modularratio or 0.: whicheveris lower a) Up to and including 20mm b) Over 20 mm 140 I Half the guaranteed yield stress subject to a maximum of 190 190 J90 130 NOTES 1 For high yield strengthdeformedbars of Grade Fe SOO the permissible stress in direct tension and flexural tension shall be Oj~.f~. The permissiblestresses for shear and compression reinforcement shall be as for GradeFe 415. 1 For welded wire fabric conformingto IS 156fl, the permissible value in tension CJIII is 230 Nzmm'. 3 For the purpose of this standard, the yield stress of steels for which there is no clearly defined yield point should be taken to be 0.2 percent proof stress. 4 When mild steel conforming to Grade II of IS 432 (Part I) is used, the permissible stresses shall be 90 percent of the permissible stressesin col 3,or if the designdetailshave already beenworkedout on thebasisof mildsteelconformingto GradeI of IS 432 (Pan I); the area of reinforcement shall be increased by 10 percent of that required for Grode I steel. where 20 percent of the gross area of the column. If a hollow metal cote is used, it shall be filled with concrete.The amount of longitudinal and spiral reinforcement andtherequirements as to spacing = permissible stress in concrete in direct (J cc compression: At" = net area of concrete section; which is (J ~. = of bars, details of splices and thickness of protectiveshelloutside the spiral, shall conform to require- rnents of 16.5.3. A clearance of at least 75 mm shall be maintained between the spiral and the metal core at aJl points, except equal to the gross area of the concrete section - AIC - Am; permissible compressive stress for column bars; A = cross-sectional area of longitudinal bar ~(.' (J me = that when the core consists of a structural steel H-column, the minimum clearance may be reinforcement; allowable unit stress in metal core, not to reduced to 50 mrn, exceed 125 N/mm 2 for a steel core, or 70 N/mm2 for a cast iron core; and Am = the cross-sectional areaof thesteel or cast c) Splicesand connections ofmetalcores- Metal cores in compositecolumns shall be accurately milled at splices and positive provisions shall Metal core and reinforcement - The crosssectional area of the metal core shall not exceed another. At the column base. provisions shall be iron core. b) be made for alignment of one core above 82 IS 456: 2000 made to transfer the load to the footing at safe unit stresses in accordancewith 34. The base of the metal section shall be designed to transfer the load from the entire composite columns to the footing. or it may be designed to transfer the load from the metal section only. provided it is placed in the pier or pedestal as to leave ample section of concrete above the base for the transfer of load from the reinforced concrete section of the column by means of bond on the vertical reinforcement and by direct compressionon the concrete. Transferof loads to the metal core shall be provided for by the useof bearingmembers, suchas billets,brackets or other positive connections, these shall be provided at the top of t.he metal core and at intermediate floor levels where required. The column as a wholeshall satisfy the requirements of formula given under (a) at any point; in addition to this, the reinforced concrete portion shall be designed to carry, according to a-3.1 or B-3.2 as the case may be, all floor loads brought into the column at levels between the metal brackets or connections. In applying the formulae under B-3.1 or 8-3.2 the gross area of column shall be taken to be the area of the concrete section outside the metal core, and the aJlowable loadon the reinforced concrete section shall be further limited to 0.28.t::k times gross sectional area of the colurnn. b) TIleresultant tension in concrete is not greater than 35 percentand 25 percentof the resultant compressionfor biaxial and uniaxial bending respectively, or does not exceed three-fourths, the 7 day modulus of rupture of concrete. NOTES 1a = lu.• 1 P for columnswithties where P. A. and A,. +1.5mA-.. ' A... definedin B-3.1and m is the modularratio. 2 O'l. huIII ::: ZM where M equals the moment and Z equals modulus of section. In the caseof sectionssubjectto moments in twodirections, the stress shall becalculated separately nod added algebraically. 8-4.2 Design Based on Cracked Section If the requirements specified in 8-4.1 are not satisfied, the stresses in concrete and steel shall be calculated by the theory of cracked section in which the tensile resistance of concrete is ignored. If the calculated stresses are within the permissible stress specified in Tables21, 22 and 23 the section may be assumed to be safe. NOTE- The maximum stress in concrete and steel may be found fromtablesandchartsbasedon thecrackedsectiontheory ordirectly by determining the no..stresslinewhichshouldsatisfy the following requirements: a) The direct load shouldhe equal to the algebraic sum of the forces on concreteand steel, b) The moment of the external loads about any reference lineshouldbeequalto the algebraic sumof the moment of the forces in cancrete (ignoring the tensile force in concrete) and steel about the same li~. "and d) Allowable Load on Metal Core Only - The metal core of composite columns shall be designed to carry safely any construction or other loads to be placed upon them prior to their encasement in concrete. c) B-4 MEMBERS SUBJECTED TO COMBINED The moment of the external loads about any other reference lines should be equal to the algebraic sum of the mOlneft1 of theforcesinconcrete (ignoring thetensile forcein concrete)and steel about the same line. AXIAL LOAD AND BENDING B4.3 Members Subjected to Combined Direct Load and Flexure 8-4.1 Design Based on Uneracked Section A member subjected to axial load and bending (due to eccentricity of load. monolithic construction, lateral forces, etc) shall be considered safe provided the following conditions are satisfied: Members subjected to combined directloadand flexure and shall be designed by limit slate method as in 39.5 afterapplying appropriate load factors as given inTable 18. a Ct, cal a) ace. + (1 chc,cal ~ 1. B-S SHEAR 0cbc B-S.l Nominal Shear Stress where ace,e,l! The nominal shear stress r v in beams or slabs of unifonn depth shall be calculated by the following equation: = calculated direct compressive stress in concrete, <Tce = permissible axialcompressivestress in concrete, ach~,f.~aal = calculated bending compressi ve tv stress in concrete, and ache V =- bel where = permissible bending compressive V = shear force due to design loads, stress in concrete. 83 IS 456: 2000 b = breadthof the member, whichfor flanged sections shall be taken as the breadth of B-S.Z.l.1 For solid slabs the permissible shear stress in concrete shall be kfc where k has the value liven the web, and below: d = effective depth. Ovemlldepth 300ar 275 2SO 22S 200 175 150(1" ofslab, mm more less k 1.00 1.05 1.10 1.1S 1.201.25 1.30 B-S.l.1 Beamsof Varying Depth In the case of beams of varying depth, the equation NOTE- This does not apply to l1at slabs for which31-' shall apply. shall be modified as: 8-5.2.2 Shear Strength of Members Under Axial Compression For members subjected to axial compression P. the permissible shear stress in concrete t c given in Table 23, shalt be multiplied by the following factor: v ± Mlanfj f v = bd d where t y ' V, band d are the same as in B-5.1, M = ~ ~ =1+~' but not exceeding 1.5 bending moment at the section, and A.fc:k = angle between the top and the bottom edges of the beam. where p = axial compressive force in N, The negative sign in the formula applies when the bending moment M increases numerically in the same direction as the effective depth d increases, and the positivesign when the momentdecreasesnumerically in this direction. 8-5.2 Design Shear Strength A, = Ie.. = characteristic compressive strength of concrete. grossareaof theconcrete sectionin mm', and 8-5.2.3 With Shear Reinforcement or Concrete When shear reinforcement is provided the nominal shear stress f c in beamsshall not exceed f c ..... given in Table 24. 8-S.2.1 The permissible shear stress in concrete in beams without shearreinforcement is given in Table 23. Table 23 Permissible Shear Stress in Concrete (Clauses B-2.1,B-2.3, 8-4.2, 8-5.2.1, B-S.2.2, B-s.3, B-S.4, 8 ..5.5.1, 8.5.5.3, l00~ B·6.~.2.B-6.3.3 and 8-6.4.3 and Tabl~ 21) Permissible Shear Stress in Concrete, t c' N/mm J bd Grade of Concrete MIS M20 M2S M30 M3S M40 and above (I) (2) (3) (4) (S) (6) (7) 0.20 0.23 S O.IS 0.18 0.18 0.19 0.20 0.20 0.25 0.22 0.22 0.23 0.23 0.23 O.SO 0.29 0.30 0.31 0.31 0.31 0.32 0.7S 0.34 0.3S 0,36 0.37 0.37 0.38 1.00 1.25 1.50 0.37 0.39 0.40 0.41 0.42 0.42 0.40 0.42 0.44 0.45 0.45 0.46 0.42 0.45 0.46 0.48 0.49 0.49 1.7~ 0.44 0.47 0.49 O.SO 0.52 0.52 2.00 0.44 0.49 O.SI 0.53 2.25 2.S0 0.44 0.~3 o.~s 0.'4 0.'6 0.55 0.56 0.S7 0.58 0.S7 0.60 O.SS 0.57 0.60 0.62 0.63 2.7S 0.44 0.51 0.51 0.51 3.00 and 0.44 o.s: 0.44 o.sa 0.60 0.61 above NOTE- A. is thatareaof longitudinal tension reinforcclncnt which continues at leastoneeffedivc deplhbeyond the lettian beiDI considered exceptat support.~ wherethe full area of tension reinforcement may be usedprovided the detai1inlconfotml to 26.2.2and 26.2.3. 84 IS 456: 2000 8-5.2.3.1 For slabs, T shall not exceed half the value of f t mal given in Table 24. greater than 230 N/mn1 y 2 , = angle between the inclined stirrup or ex bent-up bar and the axis of the member, not less than 45u • and B-S.3 Minimum Shear Reinforcement When t y is less than t c given in Table 23. minimum shear reinforcement shall be provided in accordance with 26.5.1.6. = effective depth. d Nf)TE -- Where mort.than one type of shear reinforcementis used to reinforce the same portion of the beam. the Iota) shear B-5.4 Design of Shear Reinforcement resistance shall be computed as the sum of the resistance for the various types separately. The area of the stirrups shall not be When tv exceeds t, given in Table 23, shear reinforcement shall beprovidedin any of the following less than the minimumspecified in 26.5.1.6. forms: 8-5.5 Enhanced Shear Strength of Sections Close to Supports a) Vertical stirrups, b) Bent-up bars along with stirrups. and c) Inclined stirrups. 8-S.5.1 General Shear failure at sections of beams and cantilevers Where bent-up bars arc provided, their contribution towards shear resistance. shall not be more than half that of the total shear reinforcement. without shear reinforcement will normally occur on plane inclined at an angle 30" to the horizontal. If the angle of failure plane is forced to ~c inclined more Shear reinforcementshall beprovided to carry a shear equal to V- 'tc.bd. The strengthof shear reinforcement V!' shall be calculated as below: a) For vertical stirrups steeply than this Ibecause the section considered (X - X) in Fig. 24 is close to a support or for other vs = O'sv reasons], the shear force required to produce failure is increased. The enhancement of shear strength may be taken into account in the design of sections near a support hy increasing design shear strength of concrete, ',. to 2d r/a,. provided that the design shear stress at the face of support remains less than the values given in Table 23. Account may be taken of the enhancement in any situation where the section considered is closer to the face of a support of concentrated load than twice the effective depth, d. To be effective, tension reinforcement should extend on each side of the point where it is intersected hy a possible failure plane for a distance. at least equal to the effective depth, or be provided with an equivalent anchorage. Asv d Sv h) For inclined stirrups or a series of bars bent..up at different cross-sections: ~ = C1sv ~v d (sin a + cos a) Sv c) For single bar or single group of parallel bars, all bent-up at the same cross-section: ~ =G. v Asv SiD ex where Asv = totalcross-sectional areaof stirrup legs or bent-up bars within a distance, 8-5.5.2 Shear Reinforcement for Sections Close to Supports = spacing of the stirrups or bent-up bars along the length of the member, ~~y tc = b = breadth of the member which for flanged beams, shall be taken as the breadth of the web bwt = (J"y If shear reinforcement is required, the total area of this is given by: design shear strength of the concrete, permissible tensile stress in shear reinforcementwhichshall not be taken = A" avb ( f v .. 2d fJav )/O.87fy ~ O.4a v b /O.R~f) This reinforcement should be provided within the middle three quarters of avo Where Q v is less than .l. horizontal shear reinforcement will be more effective than vertical. Table 24 Maximum Shear Stress, "r ma.' N/mm1 (Clauses 8-5.2.3. 8·5.2.3. t, 8..5.5,1 and B-6.3.1) Concrete Grade \'m••' N/mm 1 M )~ M20 M2~ MJO 1.6 1.8 1.9 2.2 85 ~1 2.J 40 and above 2.5 IS 456: 2000 v 8-5.5.3 Enhanced Shear Strength Near Supports (Simplified Approach) = shear. T = torsional moment, and b = breadth of beam. The procedure given in D-S.S.l and 8-5.5.2 may be used for all beams. However for beams carrying generally uniform load or where the principal load is located further than 2 d from the face of support, the shear stress may be calculated at a section a distance d from the face of support. The valueof tc The equivalent nominal shear stress, 'Ye' in this case shalJ be calculated as gi yen in B-5.1, except for substituting V by Ve • The values of 1'vc shall not exceed the values of 'c max given in 'fable 24. is calculated B-6.3.2 If the equivalent nominal shear stress in accordance with Table 23 and appropriate shear reinforcement is provided at sections closer to the support, no further check for such section is required. 8-6 TORSION 8-6.1 General In structures where torsion is required to maintain equilibrium, members shall be designed for torsion in accordance with8-6.2, 8-6.3 and 0-6.4. However, for such indeterminate structures where torsion can be eliminated by releasing redundent restraints, no specific design for torsion is necessary provided torsional stiffness is neglected in the calculation of internal forces. Adequate control of any torsional cracking is provided by the shear reinforcement as per B-S. 8-6.4 Reinforcement in Members Subjected to Torsion B-6.4.1 Reinforcement for torsion, when required, shall consist of longitudinal and transverse reinforcement. B-6.4.2 Longitudinal Reinforcement The longitudinal reinforcement shall be designed to resist an equivalent bending moment, Mr l , given by Mel :::M+Mr where M = bending moment at the cross-section, and NOTE- The approachto design in this clause for torsionis as follows: Torsional reinforcement is not calculated separately from that required for bending and shear. Instead the total longitudinal reinforcement is determined for n fictitious bending moment which is a function of actual bending Ml = T moment and torsion; similarly web reinforcement is (J+D/b) 1.7 ,where T is the torsional moment, D is the overall depth of the beam and b is the breadth of the beam. B-6.4.2.1 If the numerical value of Ml as defined in 8-6.4.2 exceeds the numerical value of the moment M longitudinal reinforcernent shall be provided on the flexural compression face, such that the beam can also withstand an equivalent moment Mt.2 given by Mez Ml-M, the momentMe2 being taken as acting in the opposite sense to the moment M. determinedfor a fictitious shearwhichis Il function of IlCtual shear and torsion. 8-6.1.1 The design rules laid down in 8·6.3 and 8-6.4 shall apply to beams of solid rectangular cross-section. However, these clauses may also be applied to flanged beams by substituting bw for b, in which case they are generally conservative; therefore specialist literature may be referred to. t = B-6.2 Critical Section 8-6.4.3 Transverse Reinforcement Sections located less than a distance d. from the face of the support may be designed for the same torsion as computed at a distance d, where d is the effective depth, Two legged closed hoops enclosing the corner longitudinal bars shall have an area of cross-section A.y ' given by -,v =bId)T,s;"+ 2.5dV'Sv(J,v A B-6.3 Shear and Torsion (Jay B-6.3.1 Equivalent Shear (tv. - t c) b.s a.v formula: • b • where T = torsional moment. where ~ t but the totaI 1 transverse reinforcement shall not be less than Equivalent shear, Ve shall be calculated from the v = V+1.6 T 'rye does not exceed fe' given in Table 23. minimum shear reinforcement shall be provided as specified in 26.5.1.6. 8-6.3.3 If 1'ye exceeds 1'\; given in Table 23, both longitudinal and transverse reinforcement shall be provided in accordance with B-6.4. = equivalent shear, V 86 = shear force. y IS 456: 2000 hi = = ri. :::: sv b ::: spacing of the stirrup reinforcement, 0' ,"v centre-to-centredistance betweencorner bars in the direction of the width, = per In iss i bIe tc ns i 1est rc ssin she ar reinforcement, t \'(' = equivalent shear stress as specified in centre-to-centredistance betweencorner bars in the direction of the depth, 't \ = shearstrengthof the concreteas specified 8-6.3.J., and in 'fable 23. breadth of the member, 87 IS 456: 2000 ANNEX C (Clauses 22.3.2, 23.2.1 and 42.1) CALCULATION OF DEFLECTION Col TOTAL DEFLECTION For continuous beams, deflection shaJl be calculated using the values of It' lit 'and Mr modified by the following equation: C-I.l Thetotaldeflection shallbe takenasthe sumof the short-term deflection determined in accordance with C-2 and the long-term deflection, in accordance with C-) and C-4. Xe = k. [ XI +2 Xl] + (I - k l ) Xo where C-2 SHORT-TERM DEFLECTION Xe = modified valueof X, XI' Xl = values of X at the supports, XII = valueof X at mid span, k, = coefficient givenin Table 2S, and X valueof It'I" or Mr as appropriate. C-2.1 The short-term deflection maybecalculated by the usual methods for elastic deflections using the short-term modulus of elasticity of concrete, E( and an effective moment of inertia leff given by the following equation: = I C-3 DEFLECTION DUE TO SHRINKAGE C-3.! The deflection due to shrinkage a.. may be computed from the following equation: 2 ae. = k3 Y'cs 1 where I, where k, is a constant depending upon the suppon . conditions, O.S for cantilevers, 0.125 for simply supported members. 0.086for members continuous at one end, and 0.063for fully continuous members. = moment of inertiaof the cracked section, M, = cracking moment, equal to ferYtI" where I., is the modulus of rupture of concrete, I g, is the moment of inertia of the gross section about the centroidal axis, neglecting the reinforcement, andY,is the distance from centroidal axis of gross section. neglecting the reinforcement, to extreme fibre in tension. M = maximum moment under service loads, z = lever arm. .r = depth of neutral axis. d = effective depth. b w = breadth of web.and b breadth of compression face. e v; is shrinkage curvature equal to k. =t where f:ea is theultimate shrinkage strainof concrete (Set 6.2.4). k. = =0.72 x P,~ s 1.0for 0.25 s P.- Pc < 1.0 = 0.65 x 1',~ s 1.0 for PI - r, ~ 1.0 1', 1', Table 2S Values of Coefficient,k, (Clause C-2.1) 0.5 or less 0.6 0.7 0.8 0.9 1.0 J.I 1.2 1.3 1.4 o 0.03 0.08 0.16 0.30 0.50 0.73 0.91 0.97 1.0 NOTE - *1 is given by where MI' M! Mf , . M,.! = supportmoments. lind = lixed end momenta. 88 IS 456: 2000 where where P=~andP=~ 'bd c· ai.cc(pmn) = initial plus creep deflection due to permanentloads obtained using an elastic analysis with an effective modulus of elasticity, bd and D is the total depth of the section, and I is the length of span. C-4 DEFLECTION DUE TO CREEP E ce C-4.1 The creep deflection due to permanent loads and aL'C(fICI'II') may be obtained from the following equation: 2116 818/07-13 = ~. 9 beingthe creepcoefficient, 1+8' ai(.,erm) 89 = short-term deflection due to permanent load using Ec • IS 456: 2000 ANNEX D (Clauses 24.4 and 37.1.2) SLABSSPANNING IN TWO DIRECTIONS o-i RESTRAINEDSLABS D-I.6 Ata discontinuous edge,negative moments may arise. Theydepend on the degreeof fixity at the ~ge of theslab but, in general,tensionreinforcement equal to SO percent of that provided at mid-spanextending 0.1 I into the span will be sufficient. 1)-1.0 When the comers of a slab are prevented from lifting, the slab may he designedas specifiedin D-I.l to D-l.11. D-1.1 The maximum bendingmoments per unitwidth in a slab are given by the following equations: D-t.7 Reintorcement in edge strip, parallel to that edge, shallcomplywith the minimum given in Section 3 and lhp. requirements for torsion given in D-t.S to 1)..1.10. u, =ax wi; My :::(X )' wlx2 D·UI Torsion reinforcement shall be providedat any corner where the slab is simply supported on both edges meeting at that comer. It shall consist of top and bottom reinforcement, each with layers of bars placed parallel to the sides of the slab and extending from the edges a minimum distance of one-fifth of the shorterspan.The area of reinforcement in each of these four layers shall be three-quarters of the area required for the maximum mid-span moment in the slab. where u. and <Xy art:coefficients given in Table 26, w M., My = total design load per unit area, = moments on strips of unit width spanning I. and ly respectively, and I, and I y = lengths of the shorter span and longerspan respectively. D-l.2 Slabsareconsidered all divided ineachdirection into middlestrips and edge strips as shown in Fig. 25 the middle strip being three-quarters of the widthand each edge strip one-eightof the width, 0-1.3 The maximum moment... calculatedas in 0.1.1 apply only to the middle strips and no redistribution shall be made. {)-1.4 Tensionreinforcement providedat mid-span in the middle strip shall extend in the lower part of the slab to within 0.25 I of a continuousedge, or O. J5 lof a discontinuous edge. 0-1.5 Over the continuous edges of a middle strip, the tensionreinforcement shallextendin the upperp,art of the slab a distanceof O. J5 1fromthe support.and at least 50 perceent shall extend a distance of 0.3 I. ,_.--t:t---I r~ T-'--Iii I •I MIOOLE STRIP l-i 1 ~ 25A 1E0G 1ST I I I oJ- Ly -----J j FOR SPAN 0-1.9 Torsion reinforcement equal to half that described in D-t.S shall be provided at a corner contained by edges over only one of which the slab is continuous. D-l.tO Torsion reinforcements need not be provided at any comer containedby edges over both of which the slab is continuous. V D-1.11 Torsion I. is greater than 2, the slabs shall be designed as spanningone way. 0-2 SIMPLY SUPPORTEDSLABS D-Z.1 When simply supported slabs do not have adequate provision to resist torsion at comers and to prevent the corners from lifting, the maximum r Ly -, l "------!'!!'!.~---~-. ~ . ~. . .1 L-----.-sToi----- ~ MIOOL.I STRP l- ~ 258 FOR SPAN ~ PIO. 25 DIVISION Of SLAB IN1U MIDl>LE AND EOOE STRIPS 90 .+, IS 456: 2000 Table 26 Bending Moment Coefficients for Rectangular Panels Supported on Four Sides with Provision for Torsion at Corners (Clau.fcs Case Type of Panel and No. Mumenls COlLctldered D- J .1 alit} 24.4. 1) Short Span (~oemcient5 fl. (Values Leng Span or 1,11. ) Coemclenltt (2) (I) Interior P(",~/.~: Negative moment at continuous edge Positive rnornentat nlid-span 2 4 ~ (, On« Ltm~ EtiNt Discontinuous: Negative moment at continuous edge Positive moment at mid-span 1.2 1.3 1.4 1.5 1.75 2.U (3) (4) (~) (6) (7) (8) (9) ClO) O.O's1 O.OJ9 0.053 0.041 0.060 0.065 0.049 0.032 0.024 (II) O.()32 0.037 0.024 0.028 O.04J 0.032 (lOJ6 O.OJ7 O.04J 0.OJ2· (Ul48 O.(H6 0.055 0.041 (l.O57 0.064 0.06& 0.037 0.019 0.044 0.048 0.052 0.028 0.044 O.03J OJl~2 n.OS1 0.063 ()J)44 0.047 Ooll67 OJ}51 0.077 n.()J9 O.O~9 0.085 O,()65 0.028 0.084 0.063 0.091 0.069 ().{n~ O.()47 0.045 O.fl28 O.cn7 (),02H O.()~I ()'O~7 Negative moment at continuous edge 0.047 O.05J (Ul60 o.oe.. s n.n71 0.075 Positive moment .&1 null-span O.(n~ 0.040 O.()4~ O.()4<J ().O~J ().O~6 TwoShort EtlJ.:e'.~ /Ji.\TO,,,i'UIfIUS: Nc~ativc moment at continuous edge Positive moment at mid-span n.045 O,()49 o.n56 0.043 0.059 0.044 0.065 0.069 ().()~7 0.052 0.040 0.060 ().(n~ 0.045 0.049 (U)~2 O.()J~ (Un~ O.04J 0,051 0.057 0,{.>63 0.068 0.080 O.08R ().cn~ 0.057 O.04J n.064 0.071 O.07lJ O.USO O.O~:l 0.051 O.fKlO 0.084 n.064 ().()l) J n.04S 0.069 OJ)'}? 0.073 0.043 Positive moment at .....d-span ().tl4~ O.O~I ().O~9 (l.(Xl~ 0.071 0.076 0.087 0.096 O.04~ Fo"I' EdJ.:I·.\' Discontinuous: Pll\itivl~ moment at mid-span ().()~(; 0,064 0.072 0.079 O.08S 0.089 0.107 ().O~6 0.047 Two /""IIg Hd~('." Discontinuous: O,()4~ '1'1,,·(,(, 1:·tI,t:t',\' [)i,f",mt;NulIlI.\· (Ollt' l.oll}! Edg« Continuous): Ncgntive moment at continuous edge Pn'\ltivc moment at Il'lid-silan X 'I'. 1.1 Two Adjllft'''' Edges Discontinuous: Negative moment at continuous edge Positive moment at mid-span 7 ~ 1.0 One Slulrl EtIJ.!e Continuous: Negative moment at continuous edge Positive moment at mid-span ] for All Values of (l, ,.. Thrc« EII~("'t Di.'t((lIlt;""o,,... Shorl Edge,' Conunuous) : «(Jill' O.()~7 Negative moment at eonunuous edge 9 0.100 and u x and a y are moment coefficients given in Table 27 moments per unit width arc given by the following equation: =a, ~'" I; ., My =a y ,,\./; D-2.I.l A;t least 50 percent of the tension reinforcement provided at mid-span should extend to the supports. The remaining 50 percent should extend to within 0.1 II or 0.1 ly of the support. as appropriate. Mx where M \ . M Y• ~v91 • .l'I are same ~\S those in D-I.l, Table 27 Bending Moment Coefficients for Slabs Spanning in Two Directions at Right Angles, Simply Supported on Four Sides tClausc D-2.1) 1,/1, a . (Iv 1.0 1.1 I.:! 1.3 1.4 I.~ 1.7~ 2.0 2.5 vo O,()62 0.074 ()'()84 O.09J O.()l)9 0.104 o.us (l.IIS 0.122 0.124 O.(l62 0.061 O.OSl) ().()~~ o.os: 0.046 n.O]7 0.029 0.020 (lO14 91 IS 456: 1000 ANNEX E (Clmue 25.2) EFFECTIVE LENGTH or COLUMNS E.l Intheabsence ofmoreexactanalysis, the effective length ofcolumns inframed structures may be obtained E.2 Todetermine whether a col\JIDD is I DO sway or a swaycolumn, stability indexQmay becomputed u from the ratioofeffective lengthto unsupported length givenbelow: 'et l' givenin FiS.26 whenrelative displacement of the ends of the column is prevented and in Fil. 26 when relative lateral displacement of the ends is Dot prevented. In the lattercase, it is recommendded -that . where ~D Bum of axial loads on all column in the the effective length ratio 1,,11 may not be taken to be ~. storey, less than 1.2. A. elutically computed first order lateral NOTES deflection, 1 Aprea 26 and 27 are reproduced from -The Structural H. totallatera1 forceactiDlwithintheitorey, EnaiDCCJ" No.7, Volume 52, July 1974by the penniuioa and of the Council of the In.titutioD of Structural Enpaeen, h. = height of the storey. U.K. If QS 0.04,thenthecolumn in theframe may betaken IK as no sway column, otherwise the column will·be 2 In Pip. 26 and 27.1l. ud III ale equal to IK c+ b considered as sway columnn. where the lummatioD is to be done for the memben £.3 For normal usagelSSuminl idealized conditions. framin. intoa joiat at top andbottom respectively; and Kc the effective length I" of in a given plane may be and K.. bein, the flexural stiffness for column and beam assessed on the basisof Table 28. respectively. = = = U HINGED 1·0 .........- . . -..............- w-.....,~ ............... ~I FIXED D III M ;: FlO. 26 EFncnvI LBNant RATIOS POI A COLUMN IN A PRAMI. wrrH NOSWAY 92 IS 456: 2000 HINGED1.0 0.7 t ~1 0.6 II:--+--+-~~_~r--~ O.S .......--+--~--+-~ 0.3 0.2 0.1 FIXED 0 0 0.2 0.3 0.1 ~2 c w .. 0.' 0.5 0.6 0.7 0.8 0.9 1.0 )( u:: Flo. 27 EFFF.('-IVE LENGTH RI\TIOS FOR A COLUMN IN A FRAMEWITHOUT RESTRI\INT AGAINST SWAY 2116 BISl07-14 HINGED IS 456: 2000 18W.28 Meed.. Leaatb el Com,...... Menaben (C'au#~3) ...... ..... n.wlleal Deane 01 EDd Ranlnt 01 Com".. • lon Memben VlIIatol (2) (I) Effectively heldIn position and rutrained apinst rotation in bothends Bft'ectively held in position at bothends. rutrained apinst rotation at oneend Effectively heldin position at bothends. but not restrained qainst rotation Efl'ectively held in position and rutrained apinst rotation at one end. and lit the other restrained apinst rotation but not held lnposition EfI'cctlvely heldin position lIIld restrained apinst rotation in one end, and at the otherpertlally restr· ainedagainst rotltioo but not heldin position I I I ! •.ll._••.• ....... ........ Valuetl (3) (4) 0.501 0.651 0.701 0.101 UIOI 1.00 I 1.00 I 1.201 ~ 1.501 Effectively heldin position lit oneend but not n:1trained qainst rotation, lIIld It theotherend ratntined apillSt rot8lion but not hcldin position 2.00 I 2.00 1 Effectively held in position lIIId mtrained qainst rotation It one end but not held in position normtnined qainst rotation lit the othcrend 2.00 I 2.001 L NOTE- I is the lIASlIpported /enathof c:ompmaion member. 94 IS 456: 2000 ANNEX F (Claus" 3.5.3.2 and43.1) CALCULATION OF CRACK WIDTH Provided that the strain in the tension reinforcement is limitedto 0.8F/ E•• thedesip surface cock width. whichshould not exceed the appropriate valueJiven in 35.3.2 may be calculated from the following equation: Design surfacecrack width where a", neutral axis. = the maximum compressive stress in the concrete. the tensile stressin the reinforcement. and E. the modulus of elasticity of the reinforcement Alternatively. as an approximation. it will normally besatisfactory tocalculate thesteelstresson thebasis ofa cracked section andthenreduce thisbyan amount equal to the tensile force generated by the triangular distributions. having a value of zero at the neutral axis and a value at the centroid of the tension steel of llol/mm2 instantaneously. reducing to 0.55 N/mm2 in thelong-term. acting overthetension zonedivided by the steel area. Forarectangular tension zone. thisgives I. t. = = =distance from thepointconsidered to the surface of the nearest longitudinal bar. C.. =minimum coverto the lonJitudinal bar; Em =average steel strain at the level considered. h = overall depthof the member. and x =thedepthfromthecompression faceto the x b (h-x)(a-x) £m =depth of the neutral axis. = £1 - 3E.A.(d-x} where The average steelstrain em maybe calculated on the = A. areaof tension reinforcement. b = width of the section at the centroid of the tension steel. basisof the following assumption: The concrete and the steel are bothconsidered to be fully elastic intension andincompression. The elastic modulus of the steelmaybetaken as 200 kN/mm2 and the elasticmodulus of the concrete is as derived from the equation givenin 6.2.3.1 bothin compression and , in tension. £1 Theseassumptions are illustrated in Fig.28. where h the overall depthof the section. = = strain at the levelconsidered. calculated a = d = ignoring the stiffening of the concrete in the tension zone. distance from the campression faceto the pointat which the crack width is being calculated. and effective depth. Ie './Ee I h ~""'--ST"88 • A. • SECTION CRACKED IN CONC'fETE 1 N'",,,,Z IN SHORT TERM O'SS HI'" ",2 IN LONG TERM STRESS STRAIN FIG. 28 95 IS 456: 2000 ANNEX· G (ClGu,,38.1) MOMENTS OF RESISTA.NCE FOR RECTANGULAR AND T·SECTIONS G·O The momenta of rosistance of rectanlular and T-Iectionl baled onthe .I.umptlona of38.1 areaiven in this annex. . exceeds the Ilmitllil value, M u. compr•••lon " the followln, reinforcement may be obtained from equation: G·l RECTANGULAR SECTIONS whore G-l.l SectloM Without COmprelllOD Relntorcement Mu • My 16m' d are lame u in G·I.l, f.,. desiln strell in compre.lion reinforcement correlpondiol to a strain of I The momerrt of resistance of rectanlular section. without compression reinforcement should be obtained as follows: a) Detennine the depth of netutral axia from the followin, equation : ·0.0035 .xu• mu 3 • 0.87 Ix Asc d where 0.36 kkb.d Xu. JIIIII b) If the value of xuld is less than the limiting value (see Note below 38.1), calculate the moment of resistance by the following expression : Mu =0.87 f y ~l AI&: d' • depth of compression reinforcement from compression face. The total area of tension reinforcement shall be == obtained from the following equation : Astir) dll( -bdfek If the value of xuld is equal to the limiting value. the moment of resistance of the section is given by the following expression: Mu tUm the limitinl value of Xu from 38.1. = areaofcomp'e8Sioo reinfcrcement, and A.=A. 1 +A1t2 where c) (xu,mu -d'} A•l AM 1 ~ =0.36 -xu.dmax- ( 1 -0.42 -xu,dmax- )bd Jek d) If XuI d is greater than the limiting value. the G-Z FLANGED SECTION section should be redesigned. In the above equations. .xu depth of neutral axis. d effectivedepth, characteristic strength of reinforce.. .t.y ment, G-2.1 For xu< Dr' the moment of resistance may be calculated from the equation givenin G-l.1 • G·2.2 The limiting value of the moment of resistance of the section may be obtained by the following equation whenthe ratio Dr I d does not exceed0.2 : = = = = area of tension reinforcement. t: = = area of the tensile reinforcement for a singly reinforced section for Mg. Um' and AIt... = Alie f.Ie.: I 0.871.'I " 2 Alit :: area of the total tensile reinforcement• 2 =0· 36~(1-0 I' b d Mu d ·42 Xu ,max d ) Jek w characteristic compressive strength of concrete. b - +0.4Sfek (b f -bw)Df ( width of the compression face. d-pt) Mu.lin, -- limiting moment of resistance of a section without compression . where Mu. reinforcement, and xu. ;iI"~ = Iimitingvalueof Xu = bw =breadthof the web, and bI from 39.1. G-l.2 Section with Compression Reinforcement Where me ultimate moment of resistance of section andt.c are same as in G-l.1. breadth of the compression face/flange, oXu.mtAI• d D, = thickness of the flange. 96 IS 456: 2000 G-Z.Z.I When the ratlo Dr/el exceeds 0,2, the moment of resi~tllnce of the section may be calculated by the following equation: Mil =0.36 XU.;I'" (1-0.42 XU'~lllIJl )/ek bwd r-h)Yr(d-t ) +0.45hk(b w 2 where )', = (0, JS Xu + 0.65 D,.), but not greater than DI , and the other symbols ore Maine I1S in 0-1.1 nnd G·Z.2. 0-Z.3 For xHI "U~_ > x" > D the moment of resistance . muy be calculated by the equation" given in G-Z.2 when J) Ix does not exceed 0.43 and a·Z.2.1 when f " . , • • n/xLI exceeds 0.43; In both caMe" substituting XU' ma_ ny xu' J , IS 456: 2000 ANNEX H (Forrword) COMMI1TEE COMPOsmON Cement andConcrete Sectional Committee, CBD 2 CItGi,.,.,. III H.C. VIIVISYAlYA ·C ib·, .15dt0ml, 63~. MalleI B. . . . . 560003 DR S.C. AHLUWALIA SHRI B. O. Shiite A COIIICnIetion TechllOlOl)' Ltd. PuIlC The Associated Cement Companies Ltd, Mumbai G. R. BHARnKAI SHRI T. N. TIWAItI DR D. GHOSH (Al~ma,~) CtUEPBNOIMD!I (OsSIaN) SUPSRINTENDINO BNOINEI!I (SclS) (Alt~17UI1~) CHIEP BNGINBER, NAVAOAM DAM SUPERINTENDING BNOINIIR (QCC) Central Public Work.Department, New Delhi Sardar S.-ovar Narman Nipm Ltd,GandbiDapr (Alt,,,",,,) CHIEF ENoINEEI(RBsEAlat-CUM-DlIBCTOl) RBsEARCH OPFIca (CoNcurs TBOINOLOOY) (Al"I'IUJI') lnilation and PowerROle8R:h Institute. Amritaar DIRECTOR JOINT DlRBCTOR (Al'~ntI.I'~) A.P. Bnsineering Rcaearch LaboI'llOriel, Hyderabad DlRECI'OR (CMDD) (N&W) DEPUTY DIRECTOR (CMDD)(NWItS) (Alt.mtlI.) Central Water Commission, New Delhi SHI. Hyderabad Industries Ltd. Hyderabad K. H. GANOWAL V. PA1TA8H1 (AllerlUlle) SHRI SHII V. K. GHANEKAIt Stnlctural EnaiDeering Research Centre (CSIR). Ohaziabad SHRI S. GOPlNA11I The IndiaCementaLtd, Chenaai SHill SHill R. TAMILAKAitAN (AII~mtAI.) GaaaoD Dunkerley... Co Ltd. Mumbai S. K. GUHA THAKUITA S. ~ SHII SANKAIlANARAYANAN (Al',,,",'e) Ceatral SuUdi.., Raeardllnltiture (CSIR). Roorbe SHit; N. S. BHAL DR SHRI I.SHAD MAsooo (A/"mtlt,) Cement Corporation of India. New Delhi N. C. JAIN JOINT Dlucroa STANDARDS (8&5) (CB-I) (CB-II)(Alicia,,.,.) JOINTDI~ STANDARDS (8&5) SHiI Researth. Deai.... cl StaDdIrdI OrpnlzIdoa (Ministry of Railway), Luckaow N. G. JOSHI D. Km.ua (A"~,,",,~) IDdian Hume Pipes Co Ltd.Mumbai D. K. KANUNOO NatiODll Tell House, Calcuaa SHIll ~ SHII SHI. B.R. MI!&NA (AI"".",.) SHitI P. KllSHNAMUmtY S. CHADAVAmIY (AII,17tIIt,) LInen and Toubro Limited. Mumbai SHII OR A. G. MADHAYA RAo SHII K. MANI (AIt~ruI~) StructlIrai Enlineerinl ResearchCcnn (CSIR),Chenaaa SHIIJ.SUUP HOIpilal services CODl~ C;orporation (lacIia) Ltd, NewDelhi SHI. PaAJIULl.A KUMAI Ministry of Surface Tnmspod, Depuunent of Surf. . Tranapolt (Roads WiD,), New Delhi SHI' P. P. NAIR (A"~mat~) (CUllliauetJ till flGI' 99) IS 456: ZOOO (CtRitillll,d /tTl". pal' 98) M,mbcrJ R,p"J,ntlllll MDt. SBClBTAIV Central Board of Irription and Power, NewDelhi DIIICIOI (OVIL) (Alt,""",) SRI S. K. NATHANI. SO I Engineer·in-ehief'l Branch, Army Headquarters, NewDelhi DR A.S. 00IL,BB (Alt'l7Itlt,) SKII S. S. Central Road Research Institute (CSIR), NewDeihl SBlHIA SMa. SATANDII KUMAR (Alt,mat,) SHII Y. R. PHuu. . SMRI A.K. SHAlMA (AI""",,,) Indian Roads Conll'ell, NewDelhi Da C. RAJICUNAl National Council forCement andSuildin. Materials, NewDelhi DR K. MOHAN (Alr,na",,) Directorate 0eneraI of Supplies and Disposal., NewDelhi SHI' O. RAMDAS 8HRI R. C. SHARMA(AII,mal,) SMRI S. A. RIDDI SHII OammoD lDdia Ltd,Mwnbal Geololica1 Survey of India, CaI~utta J. S. SANOANCRIA N. AOARWAL (A.lt,nul',) SMR. L. SH1.VBNKATACH~ Central Soil and Material. Reaeard\ Station, NewDelhi SHII N. CHANDRASBICAIAN (Alt,rnat,) Su....NTIINDINO ENOINIBR (DISION) ExBCUnVI ENOINEER (S.M.R.DlVlSION) (Alltrn"te) Public Works Department, Government of TamilNadu. Chennai SHR. A. K. CHADHA Hindustan Prefab Ltd. New Delhi SHRI J. R. SIL ,Alt,na"t,) DR H.C. VISYBSVARAYA SHI. D.C. CHATURVBDI (All,nun,) The Institution of Engineers (India), Calcutta SHIll VINOD KUMAI Director General. 8IS (Ex·ldficio M,mber) Director (Civ En,.) M,mber-S,crtlar;e.f SHRI J. K. PRASAD Addl Director (Civ Engg). DIS SHRI SANJAY PANT Deputy Director(Civ Engl), DIS Panel for Revision of Design Codes CllftV',..' National Councilfor(:ement and Buildin. Materials, BallabBarb DR C. RAlKUMAIt. M,,,,.,, Structural Engincerina Research Centre,Ghaziabad Gammon IndiaLtd. Mumbai Central PublicWorksDepartment, New Delhi CentralPublicWorks Department. New Delhi National Councilfor Cement and Building Materials. Ballabgarh V. K. GHAN8KAJl SHa. S. A. RIDDI SHa, JOSB KURIAN SHII DR A. K. MITrAL DR S.C.MAm DR AND.. KUMAR (Alternatt) University of Roorkee, Roorkee Schoolof Planning and Architecture, NewDelhi PRop A.K. JAIN DR V.THllUVINODAM (Cllntinued on page 1(0) 99 IS 456: 2000 tContlnuedfrom Pdf.:~ 99) Special Ad-Hoc Group for Revision of IS 456 Ctwvtntr DR H.C. VI5VBSVARYA 'Chandrikn' ot I~th Cro14~, 63·64,Mnlleswnnun, Bonplore 560 OO~ Mtmbtr.f Rtpre,felltltlN Stnu S.A. Rr;;ODI Gammon Indio Ltd, Muulbai DR C. RAJKUMAR NnrinnQl Council forCement and Building MnterinlR, Rollnhgnrh MGIPRRND-2116815/2OO7-10,OOO. 100 Bureau of Indian Standards BIS is a statutory institution established under the Bureau of Indian Standards Act, 1986 to promote harmoniousdevelopmentof the activities of standardization, markingand quality certification of goods and attending to connected matters in the country. Copyright BIShasthe copyrightof all itspublications. No partofthesepublications maybereproduced inanyformwithout the prior permission in writing of 81S. This does not preclude the free use, in the course of implementing the standard, of necessary details, such as symbols and sizes, type or grade designations. Enquiries relating to copyright be addressed to the Director (Publications), BIS. Review or Indian Standards Amendments are issued to standardsas the need arises on the basisof comments. Standardsare also reviewed periodically; a standard along with amendments is reaffirmedwhensuch review indicatesthat no changes are needed; if the review indicatesthat changesare needed, it is taken up for revision. Users of Indian Standards should ascertain that they are in possessionof the latest amendments or edition by referringto the latest issue of 'BIS Catalogue' and 'Standards: Monthly Additions'. This Indian Standard has been developed from Doc: No. CED2 (5525 ). Amendments Issued Since Publication Amend No. Date of Issue Text Affected BUREAU OF INDIAN STANDARDS Headquarters: Manak Bhavan, 9 Bahadur Shah ZafarMarg, New Delhi 110002 Telephones: 23230131,2323-3375,23239402 Regional Offices: Telegrams: Manaksanstha ( Common to all offices) Telephone Central: Manak Bhavan, 9 Bahadur Shah Zafar Marg NEWDELHI 110002 23237617 { 23233841 Eastern: 1/14C. I. T. SchemeVII M,V. I. P. Road,Kankurgachi KOLKATA 700054 Northern: SeQ 335-336, Sector34·A, CHANDIGARH 160022 23378499,23378561 { 2337 862~,23379120 Southern:C. I. T. Campus, IVCrossRoad, CHENNAI 600 113 22S4 1216,2254 1442 { 22542519,2254231 S Western: Manakalaya, E9 MIDC,Marol,Andheri(East) MUMBAI 400093 28329295,2832 7858 { 28327891,28327892 603843 { 609285 Branches: AHMEDABAD. BANGALORE. BHOPAL. BHUBANESHWAR. COIMBATORE. FARIDABAD. GHAZIABAD. GUWAHATI. HYDERABAD. JAIPUR. KANPUR. LUCKNOW. NAGPUR. NALAGARH. PATNA. PUNE. RAJKOT. THIRUVANANTHAPURAM. VISAKHAPATNAM. Printed atGovt, of Indica Press. Mayapuri, Ring Road. New Delhi 110064